data_SR3CAIR2O9_FINAL_publ

_refine_ls_shift/su_max          0.10
_refine_ls_shift/su_mean         0.01
_computing_structure_refinement  GSAS
_refine_ls_number_parameters     51
_refine_ls_goodness_of_fit_all   1.77
_refine_ls_number_restraints     0
_refine_ls_matrix_type           full
_cell_measurement_temperature    300

#==============================================================================

# 8. Phase information from GSAS

_pd_phase_name                   
'from /Volumes/Main/SkyDrive/lab/SrCaIrOmanuscript/SR3CAIR2O9_small'
_cell_length_a                   17.1475(9)
_cell_length_b                   5.7126(4)
_cell_length_c                   9.8841(6)
_cell_angle_alpha                90.0
_cell_angle_beta                 125.1364(31)
_cell_angle_gamma                90.0
_cell_volume                     791.786(11)
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 21/c'
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -x,+y+1/2,-z+1/2
-1 -x,-y,-z
-2 +x,-y+1/2,+z+1/2

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS


loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Sr Sr1 0.2543(17) 0.5358(25) 0.7509(24) 1.0 Uiso 0.0182(7) 4
Sr Sr2 0.4174(12) 0.0274(32) 0.0796(26) 1.0 Uiso 0.0182(7) 4
Sr Sr3 0.9218(13) 0.5241(32) 0.0880(27) 1.0 Uiso 0.0182(7) 4
Ca Ca1 0.0 0.5 0.5 1.0 Uiso 0.0122(34) 2
Ca Ca2 0.5 0.0 0.5 1.0 Uiso 0.0122(34) 2
Ir Ir1 0.1668(9) 0.9957(28) 0.8359(23) 1.0 Uiso 0.0126(8) 4
Ir Ir2 0.3265(9) 0.4987(25) 0.1591(23) 1.0 Uiso 0.0126(8) 4
O O1 0.4346(13) 1.0265(33) 0.6231(29) 1.0 Uiso 0.0164(6) 4
O O2 0.8822(12) 0.994(4) 0.0401(26) 1.0 Uiso 0.0164(6) 4
O O3 0.0911(14) 0.735(4) 0.7139(26) 1.0 Uiso 0.0164(6) 4
O O4 0.0683(14) 0.288(4) 0.1777(24) 1.0 Uiso 0.0164(6) 4
O O5 0.4117(15) 0.814(4) 0.8482(30) 1.0 Uiso 0.0164(6) 4
O O6 0.7496(16) 0.792(5) 0.5346(25) 1.0 Uiso 0.0164(6) 4
O O7 0.7231(15) 0.212(4) 0.9883(30) 1.0 Uiso 0.0164(6) 4
O O8 0.3833(13) 0.219(4) 0.3050(29) 1.0 Uiso 0.0164(6) 4
O O9 0.2318(18) 0.501(4) 0.2047(31) 1.0 Uiso 0.0164(6) 4

# If you change Z, be sure to change all 3 of the following
_chemical_formula_sum            'Ca Ir2 O9 Sr3'
_chemical_formula_weight         831.37
_cell_formula_units_Z            4

# MOLECULAR GEOMETRY

loop_
      _geom_angle_atom_site_label_1
      _geom_angle_atom_site_label_2
      _geom_angle_atom_site_label_3
      _geom_angle
      _geom_angle_site_symmetry_1
      _geom_angle_site_symmetry_2
      _geom_angle_site_symmetry_3
      _geom_angle_publ_flag
  Sr2       Sr1       Sr2                90.8(4)      1_556  .      1_566  N
  Sr2       Sr1       Sr2                86.9(5)      1_556  .     -2_566  N
  Sr2       Sr1       Sr3                89.3(5)      1_556  .      2_645  N
  Sr2       Sr1       Sr3               177.0(5)      1_556  .      2_655  N
  Sr2       Sr1       Sr3                87.3(5)      1_556  .     -1_666  N
  Sr2       Sr1       Ca1               121.4(5)      1_556  .      1_555  N
  Sr2       Sr1       Ca2              52.29(30)      1_556  .      2_656  N
  Sr2       Sr1       Ir1               124.2(7)      1_556  .      1_555  N
  Sr2       Sr1       Ir1               122.8(7)      1_556  .     -2_575  N
  Sr2       Sr1       Ir2                53.5(5)      1_556  .      1_556  N
  Sr2       Sr1       Ir2               127.5(6)      1_556  .     -2_576  N
  Sr2       Sr1       O2                128.5(7)      1_556  .      2_645  N
  Sr2       Sr1       O3                124.4(8)      1_556  .      1_555  N
  Sr2       Sr1       O5                 92.7(7)      1_556  .      1_555  N
  Sr2       Sr1       O6                 44.1(7)      1_556  .      2_646  N
  Sr2       Sr1       O7                124.7(9)      1_556  .      2_656  N
  Sr2       Sr1       O7                 88.0(7)      1_556  .     -1_667  N
  Sr2       Sr1       O8                 43.4(8)      1_556  .     -2_566  N
  Sr2       Sr1       O9                144.4(8)      1_556  .     -2_576  N
  Sr2       Sr1       Sr2                94.3(6)      1_566  .     -2_566  N
  Sr2       Sr1       Sr3               178.3(8)      1_566  .      2_645  N
  Sr2       Sr1       Sr3                91.6(4)      1_566  .      2_655  N
  Sr2       Sr1       Sr3                94.0(5)      1_566  .     -1_666  N
  Sr2       Sr1       Ca1               127.7(6)      1_566  .      1_555  N
  Sr2       Sr1       Ca2                57.5(4)      1_566  .      2_656  N
  Sr2       Sr1       Ir1                56.6(4)      1_566  .      1_555  N
  Sr2       Sr1       Ir1               128.7(6)      1_566  .     -2_575  N
  Sr2       Sr1       Ir2                58.8(5)      1_566  .      1_556  N
  Sr2       Sr1       Ir2                56.8(5)      1_566  .     -2_576  N
  Sr2       Sr1       O2                140.5(7)      1_566  .      2_645  N
  Sr2       Sr1       O3                 90.0(7)      1_566  .      1_555  N
  Sr2       Sr1       O5                 39.4(6)      1_566  .      1_555  N
  Sr2       Sr1       O6                 92.8(9)      1_566  .      2_646  N
  Sr2       Sr1       O7                 93.6(7)      1_566  .      2_656  N
  Sr2       Sr1       O7                 38.6(6)      1_566  .     -1_667  N
  Sr2       Sr1       O8                 96.9(8)      1_566  .     -2_566  N
  Sr2       Sr1       O9                 53.5(7)      1_566  .     -2_576  N
  Sr2       Sr1       Sr3                87.5(5)     -2_566  .      2_645  N
  Sr2       Sr1       Sr3                94.6(4)     -2_566  .      2_655  N
  Sr2       Sr1       Sr3             169.97(26)     -2_566  .     -1_666  N
  Sr2       Sr1       Ca1               124.6(5)     -2_566  .      1_555  N
  Sr2       Sr1       Ca2                55.8(4)     -2_566  .      2_656  N
  Sr2       Sr1       Ir1               133.7(5)     -2_566  .      1_555  N
  Sr2       Sr1       Ir1                55.3(4)     -2_566  .     -2_575  N
  Sr2       Sr1       Ir2               127.7(6)     -2_566  .      1_556  N
  Sr2       Sr1       Ir2                59.5(4)     -2_566  .     -2_576  N
  Sr2       Sr1       O2                 85.6(7)     -2_566  .      2_645  N
  Sr2       Sr1       O3                148.3(6)     -2_566  .      1_555  N
  Sr2       Sr1       O5                 55.1(6)     -2_566  .      1_555  N
  Sr2       Sr1       O6                130.6(8)     -2_566  .      2_646  N
  Sr2       Sr1       O7                 37.8(6)     -2_566  .      2_656  N
  Sr2       Sr1       O7                132.5(7)     -2_566  .     -1_667  N
  Sr2       Sr1       O8                 43.7(8)     -2_566  .     -2_566  N
  Sr2       Sr1       O9                 94.8(7)     -2_566  .     -2_576  N
  Sr3       Sr1       Sr3              88.16(34)      2_645  .      2_655  N
  Sr3       Sr1       Sr3                84.3(4)      2_645  .     -1_666  N
  Sr3       Sr1       Ca1              50.90(27)      2_645  .      1_555  N
  Sr3       Sr1       Ca2               123.8(6)      2_645  .      2_656  N
  Sr3       Sr1       Ir1               122.0(7)      2_645  .      1_555  N
  Sr3       Sr1       Ir1                52.5(4)      2_645  .     -2_575  N
  Sr3       Sr1       Ir2               120.1(6)      2_645  .      1_556  N
  Sr3       Sr1       Ir2               124.3(6)      2_645  .     -2_576  N
  Sr3       Sr1       O2                 39.5(5)      2_645  .      2_645  N
  Sr3       Sr1       O3                 88.4(7)      2_645  .      1_555  N
  Sr3       Sr1       O5                142.3(9)      2_645  .      1_555  N
  Sr3       Sr1       O6                 86.1(9)      2_645  .      2_646  N
  Sr3       Sr1       O7                 87.8(7)      2_645  .      2_656  N
  Sr3       Sr1       O7                139.7(8)      2_645  .     -1_667  N
  Sr3       Sr1       O8                 84.4(7)      2_645  .     -2_566  N
  Sr3       Sr1       O9                126.3(9)      2_645  .     -2_576  N
  Sr3       Sr1       Sr3                90.8(5)      2_655  .     -1_666  N
  Sr3       Sr1       Ca1                55.6(4)      2_655  .      1_555  N
  Sr3       Sr1       Ca2               130.7(5)      2_655  .      2_656  N
  Sr3       Sr1       Ir1                56.1(6)      2_655  .      1_555  N
  Sr3       Sr1       Ir1                56.6(5)      2_655  .     -2_575  N
  Sr3       Sr1       Ir2               126.7(7)      2_655  .      1_556  N
  Sr3       Sr1       Ir2                55.5(4)      2_655  .     -2_576  N
  Sr3       Sr1       O2                 49.2(5)      2_655  .      2_645  N
  Sr3       Sr1       O3                 53.8(6)      2_655  .      1_555  N
  Sr3       Sr1       O5                 90.3(8)      2_655  .      1_555  N
  Sr3       Sr1       O6               133.9(10)      2_655  .      2_646  N
  Sr3       Sr1       O7                 56.9(7)      2_655  .      2_656  N
  Sr3       Sr1       O7                 92.8(8)      2_655  .     -1_667  N
  Sr3       Sr1       O8               137.9(10)      2_655  .     -2_566  N
  Sr3       Sr1       O9                 38.2(7)      2_655  .     -2_576  N
  Sr3       Sr1       Ca1                52.9(4)     -1_666  .      1_555  N
  Sr3       Sr1       Ca2               125.4(5)     -1_666  .      2_656  N
  Sr3       Sr1       Ir1                56.1(4)     -1_666  .      1_555  N
  Sr3       Sr1       Ir1               122.3(5)     -1_666  .     -2_575  N
  Sr3       Sr1       Ir2                53.4(4)     -1_666  .      1_556  N
  Sr3       Sr1       Ir2               130.3(5)     -1_666  .     -2_576  N
  Sr3       Sr1       O2                 91.6(7)     -1_666  .      2_645  N
  Sr3       Sr1       O3                 37.3(5)     -1_666  .      1_555  N
  Sr3       Sr1       O5                133.4(7)     -1_666  .      1_555  N
  Sr3       Sr1       O6                 43.1(7)     -1_666  .      2_646  N
  Sr3       Sr1       O7                147.0(8)     -1_666  .      2_656  N
  Sr3       Sr1       O7                 55.4(6)     -1_666  .     -1_667  N
  Sr3       Sr1       O8                129.4(9)     -1_666  .     -2_566  N
  Sr3       Sr1       O9                 94.7(8)     -1_666  .     -2_576  N
  Ca1       Sr1       Ca2               173.2(5)      1_555  .      2_656  N
  Ca1       Sr1       Ir1                71.1(5)      1_555  .      1_555  N
  Ca1       Sr1       Ir1                69.6(4)      1_555  .     -2_575  N
  Ca1       Sr1       Ir2               106.2(5)      1_555  .      1_556  N
  Ca1       Sr1       Ir2               111.1(5)      1_555  .     -2_576  N
  Ca1       Sr1       O2                 39.1(5)      1_555  .      2_645  N
  Ca1       Sr1       O3                 38.3(5)      1_555  .      1_555  N
  Ca1       Sr1       O5                145.7(8)      1_555  .      1_555  N
  Ca1       Sr1       O6                 86.6(8)      1_555  .      2_646  N
  Ca1       Sr1       O7                 98.1(7)      1_555  .      2_656  N
  Ca1       Sr1       O7                 97.9(8)      1_555  .     -1_667  N
  Ca1       Sr1       O8                135.2(7)      1_555  .     -2_566  N
  Ca1       Sr1       O9                 86.6(8)      1_555  .     -2_576  N
  Ca2       Sr1       Ir1               113.9(5)      2_656  .      1_555  N
  Ca2       Sr1       Ir1               111.1(6)      2_656  .     -2_575  N
  Ca2       Sr1       Ir2                72.3(4)      2_656  .      1_556  N
  Ca2       Sr1       Ir2                75.2(4)      2_656  .     -2_576  N
  Ca2       Sr1       O2                141.0(9)      2_656  .      2_645  N
  Ca2       Sr1       O3                145.4(7)      2_656  .      1_555  N
  Ca2       Sr1       O5                 41.0(6)      2_656  .      1_555  N
  Ca2       Sr1       O6                 88.9(8)      2_656  .      2_646  N
  Ca2       Sr1       O7                 85.3(7)      2_656  .      2_656  N
  Ca2       Sr1       O7                 84.7(7)      2_656  .     -1_667  N
  Ca2       Sr1       O8                 39.3(6)      2_656  .     -2_566  N
  Ca2       Sr1       O9                100.2(8)      2_656  .     -2_576  N
  Ir1       Sr1       Ir1               112.6(7)      1_555  .     -2_575  N
  Ir1       Sr1       Ir2                70.7(6)      1_555  .      1_556  N
  Ir1       Sr1       Ir2                74.3(6)      1_555  .     -2_576  N
  Ir1       Sr1       O2                 96.1(8)      1_555  .      2_645  N
  Ir1       Sr1       O3                 34.1(6)      1_555  .      1_555  N
  Ir1       Sr1       O5                 87.1(6)      1_555  .      1_555  N
  Ir1       Sr1       O6                 89.5(9)      1_555  .      2_646  N
  Ir1       Sr1       O7                103.3(8)      1_555  .      2_656  N
  Ir1       Sr1       O7                 37.6(6)      1_555  .     -1_667  N
  Ir1       Sr1       O8                153.0(8)      1_555  .     -2_566  N
  Ir1       Sr1       O9                 39.5(7)      1_555  .     -2_576  N
  Ir1       Sr1       Ir2               172.5(6)     -2_575  .      1_556  N
  Ir1       Sr1       Ir2                71.9(5)     -2_575  .     -2_576  N
  Ir1       Sr1       O2                 30.6(5)     -2_575  .      2_645  N
  Ir1       Sr1       O3                 98.3(7)     -2_575  .      1_555  N
  Ir1       Sr1       O5                 96.4(7)     -2_575  .      1_555  N
  Ir1       Sr1       O6                138.5(9)     -2_575  .      2_646  N
  Ir1       Sr1       O7                 36.3(6)     -2_575  .      2_656  N
  Ir1       Sr1       O7                149.2(9)     -2_575  .     -1_667  N
  Ir1       Sr1       O8                 87.0(8)     -2_575  .     -2_566  N
  Ir1       Sr1       O9                 85.8(8)     -2_575  .     -2_576  N
  Ir2       Sr1       Ir2               115.6(5)      1_556  .     -2_576  N
  Ir2       Sr1       O2                144.5(8)      1_556  .      2_645  N
  Ir2       Sr1       O3                 80.8(6)      1_556  .      1_555  N
  Ir2       Sr1       O5                 90.4(7)      1_556  .      1_555  N
  Ir2       Sr1       O6                 34.0(7)      1_556  .      2_646  N
  Ir2       Sr1       O7                150.8(7)      1_556  .      2_656  N
  Ir2       Sr1       O7                 35.9(6)      1_556  .     -1_667  N
  Ir2       Sr1       O8                 92.1(8)      1_556  .     -2_566  N
  Ir2       Sr1       O9                100.3(9)      1_556  .     -2_576  N
  Ir2       Sr1       O2                 90.6(7)     -2_576  .      2_645  N
  Ir2       Sr1       O3                 98.1(7)     -2_576  .      1_555  N
  Ir2       Sr1       O5                 35.5(6)     -2_576  .      1_555  N
  Ir2       Sr1       O6                149.6(9)     -2_576  .      2_646  N
  Ir2       Sr1       O7                 38.2(6)     -2_576  .      2_656  N
  Ir2       Sr1       O7                 87.9(7)     -2_576  .     -1_667  N
  Ir2       Sr1       O8                 96.1(8)     -2_576  .     -2_566  N
  Ir2       Sr1       O9                 35.8(6)     -2_576  .     -2_576  N
  O2        Sr1       O3                 71.6(7)      2_645  .      1_555  N
  O2        Sr1       O5               122.6(10)      2_645  .      1_555  N
  O2        Sr1       O6               117.0(10)      2_645  .      2_646  N
  O2        Sr1       O7                 63.1(8)      2_645  .      2_656  N
  O2        Sr1       O7               131.7(11)      2_645  .     -1_667  N
  O2        Sr1       O8               109.4(10)      2_645  .     -2_566  N
  O2        Sr1       O9                87.1(10)      2_645  .     -2_576  N
  O3        Sr1       O5                120.2(9)      1_555  .      1_555  N
  O3        Sr1       O6                 80.3(9)      1_555  .      2_646  N
  O3        Sr1       O7                110.7(9)      1_555  .      2_656  N
  O3        Sr1       O7                 60.9(9)      1_555  .     -1_667  N
  O3        Sr1       O8               165.8(12)      1_555  .     -2_566  N
  O3        Sr1       O9                63.1(10)      1_555  .     -2_576  N
  O5        Sr1       O6               120.3(11)      1_555  .      2_646  N
  O5        Sr1       O7                 60.5(8)      1_555  .      2_656  N
  O5        Sr1       O7                 78.1(8)      1_555  .     -1_667  N
  O5        Sr1       O8                 71.8(9)      1_555  .     -2_566  N
  O5        Sr1       O9                 60.6(8)      1_555  .     -2_576  N
  O6        Sr1       O7               167.3(12)      2_646  .      2_656  N
  O6        Sr1       O7                64.7(10)      2_646  .     -1_667  N
  O6        Sr1       O8                86.9(10)      2_646  .     -2_566  N
  O6        Sr1       O9               127.4(11)      2_646  .     -2_576  N
  O7        Sr1       O7                125.8(5)      2_656  .     -1_667  N
  O7        Sr1       O8                 81.4(9)      2_656  .     -2_566  N
  O7        Sr1       O9                64.9(10)      2_656  .     -2_576  N
  O7        Sr1       O8               118.8(11)     -1_667  .     -2_566  N
  O7        Sr1       O9                64.8(10)     -1_667  .     -2_576  N
  O8        Sr1       O9               130.7(11)     -2_566  .     -2_576  N
  Sr1       Sr2       Sr1                90.8(4)      1_544  .      1_554  N
  Sr1       Sr2       Sr1                87.0(5)      1_544  .     -2_554  N
  Sr1       Sr2       Sr2                90.4(5)      1_544  .      2_645  N
  Sr1       Sr2       Sr2              179.0(11)      1_544  .      2_655  N
  Sr1       Sr2       Sr2                87.0(8)      1_544  .     -1_655  N
  Sr1       Sr2       Ca2               123.1(7)      1_544  .      1_555  N
  Sr1       Sr2       Ca2                53.9(5)      1_544  .      2_645  N
  Sr1       Sr2       Ca2               124.9(6)      1_544  .      2_655  N
  Sr1       Sr2       Ir2               123.0(6)      1_544  .      1_555  N
  Sr1       Sr2       Ir2              51.46(32)      1_544  .     -2_565  N
  Sr1       Sr2       O1                128.2(8)      1_544  .     -1_666  N
  Sr1       Sr2       O1                142.7(8)      1_544  .     -2_575  N
  Sr1       Sr2       O5                 44.1(6)      1_544  .      1_544  N
  Sr1       Sr2       O5                126.2(9)      1_544  .     -1_666  N
  Sr1       Sr2       O6                 88.7(7)      1_544  .      2_645  N
  Sr1       Sr2       O7                 43.9(7)      1_544  .     -1_656  N
  Sr1       Sr2       O8                123.3(9)      1_544  .      1_555  N
  Sr1       Sr2       O8                 85.3(7)      1_544  .     -2_565  N
  Sr1       Sr2       Sr1                94.3(5)      1_554  .     -2_554  N
  Sr1       Sr2       Sr2               178.4(9)      1_554  .      2_645  N
  Sr1       Sr2       Sr2              89.49(32)      1_554  .      2_655  N
  Sr1       Sr2       Sr2                93.4(7)      1_554  .     -1_655  N
  Sr1       Sr2       Ca2               126.8(6)      1_554  .      1_555  N
  Sr1       Sr2       Ca2               127.0(7)      1_554  .      2_645  N
  Sr1       Sr2       Ca2                54.7(4)      1_554  .      2_655  N
  Sr1       Sr2       Ir2                54.8(5)      1_554  .      1_555  N
  Sr1       Sr2       Ir2                56.5(4)      1_554  .     -2_565  N
  Sr1       Sr2       O1                141.0(8)      1_554  .     -1_666  N
  Sr1       Sr2       O1                 51.9(6)      1_554  .     -2_575  N
  Sr1       Sr2       O5                 88.3(9)      1_554  .      1_544  N
  Sr1       Sr2       O5                 96.5(8)      1_554  .     -1_666  N
  Sr1       Sr2       O6                 39.1(6)      1_554  .      2_645  N
  Sr1       Sr2       O7                 93.6(8)      1_554  .     -1_656  N
  Sr1       Sr2       O8                 89.6(7)      1_554  .      1_555  N
  Sr1       Sr2       O8                 36.4(6)      1_554  .     -2_565  N
  Sr1       Sr2       Sr2                84.8(8)     -2_565  .      2_645  N
  Sr1       Sr2       Sr2                92.0(8)     -2_565  .      2_655  N
  Sr1       Sr2       Sr2               170.3(7)     -2_565  .     -1_655  N
  Sr1       Sr2       Ca2                53.7(4)     -2_565  .      1_555  N
  Sr1       Sr2       Ca2               118.1(5)     -2_565  .      2_645  N
  Sr1       Sr2       Ca2               131.3(6)     -2_565  .      2_655  N
  Sr1       Sr2       Ir2                57.1(5)     -2_565  .      1_555  N
  Sr1       Sr2       Ir2               123.5(4)     -2_565  .     -2_565  N
  Sr1       Sr2       O1                 88.7(7)     -2_565  .     -1_666  N
  Sr1       Sr2       O1                 93.3(9)     -2_565  .     -2_575  N
  Sr1       Sr2       O5                131.1(7)     -2_565  .      1_544  N
  Sr1       Sr2       O5                144.7(7)     -2_565  .     -1_666  N
  Sr1       Sr2       O6                 55.2(7)     -2_565  .      2_645  N
  Sr1       Sr2       O7                 43.1(7)     -2_565  .     -1_656  N
  Sr1       Sr2       O8                 36.5(7)     -2_565  .      1_555  N
  Sr1       Sr2       O8                129.7(7)     -2_565  .     -2_565  N
  Sr2       Sr2       Sr2                89.2(7)      2_645  .      2_655  N
  Sr2       Sr2       Sr2                87.6(7)      2_645  .     -1_655  N
  Sr2       Sr2       Ca2                51.6(5)      2_645  .      1_555  N
  Sr2       Sr2       Ca2              54.54(34)      2_645  .      2_645  N
  Sr2       Sr2       Ca2               125.0(7)      2_645  .      2_655  N
  Sr2       Sr2       Ir2              123.7(11)      2_645  .      1_555  N
  Sr2       Sr2       Ir2               125.1(8)      2_645  .     -2_565  N
  Sr2       Sr2       O1                 37.7(6)      2_645  .     -1_666  N
  Sr2       Sr2       O1                126.8(9)      2_645  .     -2_575  N
  Sr2       Sr2       O5                 93.3(9)      2_645  .      1_544  N
  Sr2       Sr2       O5                 83.4(7)      2_645  .     -1_666  N
  Sr2       Sr2       O6               140.0(13)      2_645  .      2_645  N
  Sr2       Sr2       O7                 86.7(8)      2_645  .     -1_656  N
  Sr2       Sr2       O8                88.9(10)      2_645  .      1_555  N
  Sr2       Sr2       O8               144.7(13)      2_645  .     -2_565  N
  Sr2       Sr2       Sr2                93.9(8)      2_655  .     -1_655  N
  Sr2       Sr2       Ca2                56.0(6)      2_655  .      1_555  N
  Sr2       Sr2       Ca2               126.5(7)      2_655  .      2_645  N
  Sr2       Sr2       Ca2              56.01(32)      2_655  .      2_655  N
  Sr2       Sr2       Ir2                56.6(5)      2_655  .      1_555  N
  Sr2       Sr2       Ir2               129.4(8)      2_655  .     -2_565  N
  Sr2       Sr2       O1                 51.5(7)      2_655  .     -1_666  N
  Sr2       Sr2       O1                 37.6(5)      2_655  .     -2_575  N
  Sr2       Sr2       O5               136.8(12)      2_655  .      1_544  N
  Sr2       Sr2       O5                 54.7(6)      2_655  .     -1_666  N
  Sr2       Sr2       O6                 91.0(7)      2_655  .      2_645  N
  Sr2       Sr2       O7               135.2(13)      2_655  .     -1_656  N
  Sr2       Sr2       O8                 55.7(7)      2_655  .      1_555  N
  Sr2       Sr2       O8                 95.5(6)      2_655  .     -2_565  N
  Sr2       Sr2       Ca2               124.6(6)     -1_655  .      1_555  N
  Sr2       Sr2       Ca2                52.2(5)     -1_655  .      2_645  N
  Sr2       Sr2       Ca2                58.3(5)     -1_655  .      2_655  N
  Sr2       Sr2       Ir2               132.6(9)     -1_655  .      1_555  N
  Sr2       Sr2       Ir2                57.2(7)     -1_655  .     -2_565  N
  Sr2       Sr2       O1                 89.0(7)     -1_655  .     -1_666  N
  Sr2       Sr2       O1                 96.1(9)     -1_655  .     -2_575  N
  Sr2       Sr2       O5                 43.3(7)     -1_655  .      1_544  N
  Sr2       Sr2       O5                 39.5(5)     -1_655  .     -1_666  N
  Sr2       Sr2       O6               132.3(10)     -1_655  .      2_645  N
  Sr2       Sr2       O7               130.4(11)     -1_655  .     -1_656  N
  Sr2       Sr2       O8               149.5(10)     -1_655  .      1_555  N
  Sr2       Sr2       O8                 57.3(8)     -1_655  .     -2_565  N
  Ca2       Sr2       Ca2               106.1(4)      1_555  .      2_645  N
  Ca2       Sr2       Ca2               112.0(5)      1_555  .      2_655  N
  Ca2       Sr2       Ir2                72.1(6)      1_555  .      1_555  N
  Ca2       Sr2       Ir2               174.5(6)      1_555  .     -2_565  N
  Ca2       Sr2       O1                 35.6(5)      1_555  .     -1_666  N
  Ca2       Sr2       O1                 85.3(9)      1_555  .     -2_575  N
  Ca2       Sr2       O5               144.8(10)      1_555  .      1_544  N
  Ca2       Sr2       O5                 93.6(6)      1_555  .     -1_666  N
  Ca2       Sr2       O6                 96.9(8)      1_555  .      2_645  N
  Ca2       Sr2       O7                 87.9(9)      1_555  .     -1_656  N
  Ca2       Sr2       O8                 38.4(6)      1_555  .      1_555  N
  Ca2       Sr2       O8                150.8(8)      1_555  .     -2_565  N
  Ca2       Sr2       Ca2               110.5(7)      2_645  .      2_655  N
  Ca2       Sr2       Ir2               175.1(7)      2_645  .      1_555  N
  Ca2       Sr2       Ir2                70.6(5)      2_645  .     -2_565  N
  Ca2       Sr2       O1                 84.0(6)      2_645  .     -1_666  N
  Ca2       Sr2       O1               147.5(10)      2_645  .     -2_575  N
  Ca2       Sr2       O5                 38.7(7)      2_645  .      1_544  N
  Ca2       Sr2       O5                 80.6(6)      2_645  .     -1_666  N
  Ca2       Sr2       O6                142.4(8)      2_645  .      2_645  N
  Ca2       Sr2       O7                 85.6(7)      2_645  .     -1_656  N
  Ca2       Sr2       O8                141.3(9)      2_645  .      1_555  N
  Ca2       Sr2       O8                 96.3(9)      2_645  .     -2_565  N
  Ca2       Sr2       Ir2                74.3(5)      2_655  .      1_555  N
  Ca2       Sr2       Ir2                73.4(5)      2_655  .     -2_565  N
  Ca2       Sr2       O1                 95.3(6)      2_655  .     -1_666  N
  Ca2       Sr2       O1                 38.5(6)      2_655  .     -2_575  N
  Ca2       Sr2       O5                 88.7(9)      2_655  .      1_544  N
  Ca2       Sr2       O5                 42.4(6)      2_655  .     -1_666  N
  Ca2       Sr2       O6                 86.8(8)      2_655  .      2_645  N
  Ca2       Sr2       O7                148.2(9)      2_655  .     -1_656  N
  Ca2       Sr2       O8                100.4(8)      2_655  .      1_555  N
  Ca2       Sr2       O8                 40.7(4)      2_655  .     -2_565  N
  Ir2       Sr2       Ir2               110.8(6)      1_555  .     -2_565  N
  Ir2       Sr2       O1                 96.5(9)      1_555  .     -1_666  N
  Ir2       Sr2       O1                 37.4(6)      1_555  .     -2_575  N
  Ir2       Sr2       O5               142.8(10)      1_555  .      1_544  N
  Ir2       Sr2       O5                104.0(7)      1_555  .     -1_666  N
  Ir2       Sr2       O6                 35.2(6)      1_555  .      2_645  N
  Ir2       Sr2       O7                 89.7(8)      1_555  .     -1_656  N
  Ir2       Sr2       O8                 35.6(6)      1_555  .      1_555  N
  Ir2       Sr2       O8                 87.0(7)      1_555  .     -2_565  N
  Ir2       Sr2       O1                145.6(9)     -2_565  .     -1_666  N
  Ir2       Sr2       O1                 99.8(9)     -2_565  .     -2_575  N
  Ir2       Sr2       O5                 32.0(7)     -2_565  .      1_544  N
  Ir2       Sr2       O5                 90.1(8)     -2_565  .     -1_666  N
  Ir2       Sr2       O6                 83.8(6)     -2_565  .      2_645  N
  Ir2       Sr2       O7                 87.5(7)     -2_565  .     -1_656  N
  Ir2       Sr2       O8                143.0(7)     -2_565  .      1_555  N
  Ir2       Sr2       O8                 34.6(6)     -2_565  .     -2_565  N
  O1        Sr2       O1                 89.1(8)     -1_666  .     -2_575  N
  O1        Sr2       O5               118.2(11)     -1_666  .      1_544  N
  O1        Sr2       O5                 62.4(8)     -1_666  .     -1_666  N
  O1        Sr2       O6               128.8(11)     -1_666  .      2_645  N
  O1        Sr2       O7               114.0(10)     -1_666  .     -1_656  N
  O1        Sr2       O8                 70.2(9)     -1_666  .      1_555  N
  O1        Sr2       O8                133.1(9)     -1_666  .     -2_565  N
  O1        Sr2       O5               124.5(13)     -2_575  .      1_544  N
  O1        Sr2       O5                 68.1(8)     -2_575  .     -1_666  N
  O1        Sr2       O6                 62.0(9)     -2_575  .      2_645  N
  O1        Sr2       O7               125.8(10)     -2_575  .     -1_656  N
  O1        Sr2       O8                 62.6(9)     -2_575  .      1_555  N
  O1        Sr2       O8                 66.0(8)     -2_575  .     -2_565  N
  O5        Sr2       O5                 82.8(9)      1_544  .     -1_666  N
  O5        Sr2       O6               113.0(10)      1_544  .      2_645  N
  O5        Sr2       O7                 88.0(9)      1_544  .     -1_656  N
  O5        Sr2       O8               167.2(11)      1_544  .      1_555  N
  O5        Sr2       O8                60.1(10)      1_544  .     -2_565  N
  O5        Sr2       O6               127.7(11)     -1_666  .      2_645  N
  O5        Sr2       O7               166.0(10)     -1_666  .     -1_656  N
  O5        Sr2       O8                110.0(9)     -1_666  .      1_555  N
  O5        Sr2       O8                 71.3(8)     -1_666  .     -2_565  N
  O6        Sr2       O7                65.7(10)      2_645  .     -1_656  N
  O6        Sr2       O8                 59.2(8)      2_645  .      1_555  N
  O6        Sr2       O8                 75.0(6)      2_645  .     -2_565  N
  O7        Sr2       O8                79.6(10)     -1_656  .      1_555  N
  O7        Sr2       O8               112.8(10)     -1_656  .     -2_565  N
  O8        Sr2       O8                122.4(7)      1_555  .     -2_565  N
  Sr1       Sr3       Sr1              88.16(34)      2_645  .      2_655  N
  Sr1       Sr3       Sr1                84.3(4)      2_645  .     -1_666  N
  Sr1       Sr3       Sr3                90.4(5)      2_645  .      2_745  N
  Sr1       Sr3       Sr3               176.1(7)      2_645  .      2_755  N
  Sr1       Sr3       Sr3                87.7(8)      2_645  .     -1_765  N
  Sr1       Sr3       Ca1               122.8(6)      2_645  .      1_655  N
  Sr1       Sr3       Ca1                55.3(5)      2_645  .      2_645  N
  Sr1       Sr3       Ca1               124.1(6)      2_645  .      2_655  N
  Sr1       Sr3       Ir1               121.3(5)      2_645  .     -1_676  N
  Sr1       Sr3       Ir1               126.1(7)      2_645  .     -2_675  N
  Sr1       Sr3       Ir2                50.8(4)      2_645  .     -1_665  N
  Sr1       Sr3       O2                122.5(6)      2_645  .      1_555  N
  Sr1       Sr3       O3                 83.3(8)      2_645  .     -1_666  N
  Sr1       Sr3       O3               143.1(10)      2_645  .     -2_675  N
  Sr1       Sr3       O4                 92.3(9)      2_645  .      1_655  N
  Sr1       Sr3       O4                138.2(9)      2_645  .      2_655  N
  Sr1       Sr3       O4                 84.9(7)      2_645  .     -1_665  N
  Sr1       Sr3       O6                 84.4(7)      2_645  .     -2_575  N
  Sr1       Sr3       O9                 40.2(5)      2_645  .     -1_665  N
  Sr1       Sr3       Sr1                90.9(5)      2_655  .     -1_666  N
  Sr1       Sr3       Sr3               176.9(9)      2_655  .      2_745  N
  Sr1       Sr3       Sr3                89.1(4)      2_655  .      2_755  N
  Sr1       Sr3       Sr3                93.2(7)      2_655  .     -1_765  N
  Sr1       Sr3       Ca1               125.7(6)      2_655  .      1_655  N
  Sr1       Sr3       Ca1               126.3(6)      2_655  .      2_645  N
  Sr1       Sr3       Ca1                55.6(5)      2_655  .      2_655  N
  Sr1       Sr3       Ir1                53.5(5)      2_655  .     -1_676  N
  Sr1       Sr3       Ir1               128.4(7)      2_655  .     -2_675  N
  Sr1       Sr3       Ir2                55.5(4)      2_655  .     -1_665  N
  Sr1       Sr3       O2                 34.8(6)      2_655  .      1_555  N
  Sr1       Sr3       O3                132.9(8)      2_655  .     -1_666  N
  Sr1       Sr3       O3                 95.7(8)      2_655  .     -2_675  N
  Sr1       Sr3       O4                140.8(9)      2_655  .      1_655  N
  Sr1       Sr3       O4                 87.5(7)      2_655  .      2_655  N
  Sr1       Sr3       O4                 53.8(5)      2_655  .     -1_665  N
  Sr1       Sr3       O6                 53.4(5)      2_655  .     -2_575  N
  Sr1       Sr3       O9                 48.0(6)      2_655  .     -1_665  N
  Sr1       Sr3       Sr3                86.2(7)     -1_666  .      2_745  N
  Sr1       Sr3       Sr3                93.0(8)     -1_666  .      2_755  N
  Sr1       Sr3       Sr3               170.9(8)     -1_666  .     -1_765  N
  Sr1       Sr3       Ca1                54.9(4)     -1_666  .      1_655  N
  Sr1       Sr3       Ca1               118.6(4)     -1_666  .      2_645  N
  Sr1       Sr3       Ca1               130.7(6)     -1_666  .      2_655  N
  Sr1       Sr3       Ir1                58.0(5)     -1_666  .     -1_676  N
  Sr1       Sr3       Ir1               125.7(6)     -1_666  .     -2_675  N
  Sr1       Sr3       Ir2                53.3(5)     -1_666  .     -1_665  N
  Sr1       Sr3       O2                 89.1(8)     -1_666  .      1_555  N
  Sr1       Sr3       O3                 42.2(7)     -1_666  .     -1_666  N
  Sr1       Sr3       O3                132.2(9)     -1_666  .     -2_675  N
  Sr1       Sr3       O4                128.2(7)     -1_666  .      1_655  N
  Sr1       Sr3       O4                 54.2(6)     -1_666  .      2_655  N
  Sr1       Sr3       O4                143.3(6)     -1_666  .     -1_665  N
  Sr1       Sr3       O6                 37.6(5)     -1_666  .     -2_575  N
  Sr1       Sr3       O9                 85.8(7)     -1_666  .     -1_665  N
  Sr3       Sr3       Sr3                92.2(8)      2_745  .      2_755  N
  Sr3       Sr3       Sr3                89.4(8)      2_745  .     -1_765  N
  Sr3       Sr3       Ca1                53.2(5)      2_745  .      1_655  N
  Sr3       Sr3       Ca1              54.61(33)      2_745  .      2_645  N
  Sr3       Sr3       Ca1               127.3(7)      2_745  .      2_655  N
  Sr3       Sr3       Ir1              125.4(11)      2_745  .     -1_676  N
  Sr3       Sr3       Ir1                54.5(5)      2_745  .     -2_675  N
  Sr3       Sr3       Ir2               121.7(7)      2_745  .     -1_665  N
  Sr3       Sr3       O2               146.1(11)      2_745  .      1_555  N
  Sr3       Sr3       O3                 44.2(5)      2_745  .     -1_666  N
  Sr3       Sr3       O3                 87.1(8)      2_745  .     -2_675  N
  Sr3       Sr3       O4                 42.0(5)      2_745  .      1_655  N
  Sr3       Sr3       O4                91.8(10)      2_745  .      2_655  N
  Sr3       Sr3       O4               128.8(10)      2_745  .     -1_665  N
  Sr3       Sr3       O6                123.8(9)      2_745  .     -2_575  N
  Sr3       Sr3       O9                130.5(7)      2_745  .     -1_665  N
  Sr3       Sr3       Sr3                95.2(8)      2_755  .     -1_765  N
  Sr3       Sr3       Ca1                57.1(7)      2_755  .      1_655  N
  Sr3       Sr3       Ca1               128.6(7)      2_755  .      2_645  N
  Sr3       Sr3       Ca1              56.00(30)      2_755  .      2_655  N
  Sr3       Sr3       Ir1                54.9(4)      2_755  .     -1_676  N
  Sr3       Sr3       Ir1                57.8(6)      2_755  .     -2_675  N
  Sr3       Sr3       Ir2               125.4(7)      2_755  .     -1_665  N
  Sr3       Sr3       O2                 54.5(4)      2_755  .      1_555  N
  Sr3       Sr3       O3                96.6(12)      2_755  .     -1_666  N
  Sr3       Sr3       O3                 40.0(6)      2_755  .     -2_675  N
  Sr3       Sr3       O4                 91.5(9)      2_755  .      1_655  N
  Sr3       Sr3       O4                 38.9(6)      2_755  .      2_655  N
  Sr3       Sr3       O4                 95.7(7)      2_755  .     -1_665  N
  Sr3       Sr3       O6                 91.8(9)      2_755  .     -2_575  N
  Sr3       Sr3       O9                137.0(7)      2_755  .     -1_665  N
  Sr3       Sr3       Ca1               127.5(7)     -1_765  .      1_655  N
  Sr3       Sr3       Ca1                52.6(5)     -1_765  .      2_645  N
  Sr3       Sr3       Ca1                58.0(4)     -1_765  .      2_655  N
  Sr3       Sr3       Ir1               130.6(8)     -1_765  .     -1_676  N
  Sr3       Sr3       Ir1                56.7(6)     -1_765  .     -2_675  N
  Sr3       Sr3       Ir2               123.6(9)     -1_765  .     -1_665  N
  Sr3       Sr3       O2                 98.9(9)     -1_765  .      1_555  N
  Sr3       Sr3       O3                132.4(9)     -1_765  .     -1_666  N
  Sr3       Sr3       O3                 55.5(6)     -1_765  .     -2_675  N
  Sr3       Sr3       O4                 47.7(6)     -1_765  .      1_655  N
  Sr3       Sr3       O4               134.1(10)     -1_765  .      2_655  N
  Sr3       Sr3       O4                 39.5(6)     -1_765  .     -1_665  N
  Sr3       Sr3       O6                145.8(8)     -1_765  .     -2_575  N
  Sr3       Sr3       O9                90.9(10)     -1_765  .     -1_665  N
  Ca1       Sr3       Ca1               107.7(4)      1_655  .      2_645  N
  Ca1       Sr3       Ca1               113.1(6)      1_655  .      2_655  N
  Ca1       Sr3       Ir1                72.3(6)      1_655  .     -1_676  N
  Ca1       Sr3       Ir1                71.0(4)      1_655  .     -2_675  N
  Ca1       Sr3       Ir2               108.1(6)      1_655  .     -1_665  N
  Ca1       Sr3       O2                 97.5(9)      1_655  .      1_555  N
  Ca1       Sr3       O3                 39.5(6)      1_655  .     -1_666  N
  Ca1       Sr3       O3                 84.0(8)      1_655  .     -2_675  N
  Ca1       Sr3       O4                 86.1(7)      1_655  .      1_655  N
  Ca1       Sr3       O4                 39.0(6)      1_655  .      2_655  N
  Ca1       Sr3       O4                151.7(8)      1_655  .     -1_665  N
  Ca1       Sr3       O6                 83.9(7)      1_655  .     -2_575  N
  Ca1       Sr3       O9                140.6(9)      1_655  .     -1_665  N
  Ca1       Sr3       Ca1               110.6(6)      2_645  .      2_655  N
  Ca1       Sr3       Ir1               176.1(6)      2_645  .     -1_676  N
  Ca1       Sr3       Ir1                70.8(4)      2_645  .     -2_675  N
  Ca1       Sr3       Ir2               106.0(6)      2_645  .     -1_665  N
  Ca1       Sr3       O2               149.9(11)      2_645  .      1_555  N
  Ca1       Sr3       O3                 85.0(7)      2_645  .     -1_666  N
  Ca1       Sr3       O3                 94.7(8)      2_645  .     -2_675  N
  Ca1       Sr3       O4                 37.1(6)      2_645  .      1_655  N
  Ca1       Sr3       O4                146.2(8)      2_645  .      2_655  N
  Ca1       Sr3       O4                 82.3(7)      2_645  .     -1_665  N
  Ca1       Sr3       O6                138.3(9)      2_645  .     -2_575  N
  Ca1       Sr3       O9                 87.9(8)      2_645  .     -1_665  N
  Ca1       Sr3       Ir1                72.7(5)      2_655  .     -1_676  N
  Ca1       Sr3       Ir1                72.8(5)      2_655  .     -2_675  N
  Ca1       Sr3       Ir2               110.9(5)      2_655  .     -1_665  N
  Ca1       Sr3       O2                 42.2(5)      2_655  .      1_555  N
  Ca1       Sr3       O3               152.6(10)      2_655  .     -1_666  N
  Ca1       Sr3       O3                 40.9(5)      2_655  .     -2_675  N
  Ca1       Sr3       O4                 93.3(7)      2_655  .      1_655  N
  Ca1       Sr3       O4                 86.1(7)      2_655  .      2_655  N
  Ca1       Sr3       O4                 40.0(5)      2_655  .     -1_665  N
  Ca1       Sr3       O6                100.2(7)      2_655  .     -2_575  N
  Ca1       Sr3       O9                 93.3(7)      2_655  .     -1_665  N
  Ir1       Sr3       Ir1               112.6(7)     -1_676  .     -2_675  N
  Ir1       Sr3       Ir2                70.5(5)     -1_676  .     -1_665  N
  Ir1       Sr3       O2                 32.5(5)     -1_676  .      1_555  N
  Ir1       Sr3       O3                92.9(10)     -1_676  .     -1_666  N
  Ir1       Sr3       O3                 89.2(9)     -1_676  .     -2_675  N
  Ir1       Sr3       O4               146.1(10)     -1_676  .      1_655  N
  Ir1       Sr3       O4                 34.5(7)     -1_676  .      2_655  N
  Ir1       Sr3       O4                 99.5(6)     -1_676  .     -1_665  N
  Ir1       Sr3       O6                 37.9(7)     -1_676  .     -2_575  N
  Ir1       Sr3       O9                 89.8(8)     -1_676  .     -1_665  N
  Ir1       Sr3       Ir2               175.9(7)     -2_675  .     -1_665  N
  Ir1       Sr3       O2                103.6(7)     -2_675  .      1_555  N
  Ir1       Sr3       O3                 92.5(7)     -2_675  .     -1_666  N
  Ir1       Sr3       O3                 33.2(7)     -2_675  .     -2_675  N
  Ir1       Sr3       O4                 33.9(6)     -2_675  .      1_655  N
  Ir1       Sr3       O4                 87.7(7)     -2_675  .      2_655  N
  Ir1       Sr3       O4                 88.5(7)     -2_675  .     -1_665  N
  Ir1       Sr3       O6               147.7(10)     -2_675  .     -2_575  N
  Ir1       Sr3       O9               147.5(11)     -2_675  .     -1_665  N
  Ir2       Sr3       O2                 80.5(6)     -1_665  .      1_555  N
  Ir2       Sr3       O3                 84.6(8)     -1_665  .     -1_666  N
  Ir2       Sr3       O3                150.8(8)     -1_665  .     -2_675  N
  Ir2       Sr3       O4               142.7(10)     -1_665  .      1_655  N
  Ir2       Sr3       O4                 94.1(8)     -1_665  .      2_655  N
  Ir2       Sr3       O4                 93.6(6)     -1_665  .     -1_665  N
  Ir2       Sr3       O6                 34.5(7)     -1_665  .     -2_575  N
  Ir2       Sr3       O9                 32.7(6)     -1_665  .     -1_665  N
  O2        Sr3       O3               125.1(13)      1_555  .     -1_666  N
  O2        Sr3       O3                 71.5(8)      1_555  .     -2_675  N
  O2        Sr3       O4                133.0(9)      1_555  .      1_655  N
  O2        Sr3       O4                 59.0(9)      1_555  .      2_655  N
  O2        Sr3       O4                 67.9(7)      1_555  .     -1_665  N
  O2        Sr3       O6                 59.1(9)      1_555  .     -2_575  N
  O2        Sr3       O9                 82.5(9)      1_555  .     -1_665  N
  O3        Sr3       O3                118.1(8)     -1_666  .     -2_675  N
  O3        Sr3       O4                 86.0(7)     -1_666  .      1_655  N
  O3        Sr3       O4                69.9(11)     -1_666  .      2_655  N
  O3        Sr3       O4               166.1(12)     -1_666  .     -1_665  N
  O3        Sr3       O6                 79.7(8)     -1_666  .     -2_575  N
  O3        Sr3       O9                110.2(9)     -1_666  .     -1_665  N
  O3        Sr3       O4                 62.2(9)     -2_675  .      1_655  N
  O3        Sr3       O4                 78.7(9)     -2_675  .      2_655  N
  O3        Sr3       O4                 68.6(8)     -2_675  .     -1_665  N
  O3        Sr3       O6               126.7(11)     -2_675  .     -2_575  N
  O3        Sr3       O9               131.7(10)     -2_675  .     -1_665  N
  O4        Sr3       O4                116.2(8)      1_655  .      2_655  N
  O4        Sr3       O4                 87.2(9)      1_655  .     -1_665  N
  O4        Sr3       O6               165.5(10)      1_655  .     -2_575  N
  O4        Sr3       O9               122.4(12)      1_655  .     -1_665  N
  O4        Sr3       O4                124.0(7)      2_655  .     -1_665  N
  O4        Sr3       O6                 60.2(9)      2_655  .     -2_575  N
  O4        Sr3       O9               121.3(10)      2_655  .     -1_665  N
  O4        Sr3       O6                106.5(7)     -1_665  .     -2_575  N
  O4        Sr3       O9                 63.9(8)     -1_665  .     -1_665  N
  O6        Sr3       O9                 62.3(9)     -2_575  .     -1_665  N
  Sr1       Ca1       Sr1                  180.0      1_555  .     -1_566  N
  Sr1       Ca1       Sr3               107.7(5)      1_555  .      1_455  N
  Sr1       Ca1       Sr3                73.5(4)      1_555  .      2_645  N
  Sr1       Ca1       Sr3                69.1(4)      1_555  .      2_655  N
  Sr1       Ca1       Sr3                72.3(5)      1_555  .     -1_666  N
  Sr1       Ca1       Sr3               110.9(4)      1_555  .     -2_466  N
  Sr1       Ca1       Sr3               106.5(4)      1_555  .     -2_476  N
  Sr1       Ca1       O2                 43.0(6)      1_555  .      2_645  N
  Sr1       Ca1       O2                137.0(6)      1_555  .     -2_476  N
  Sr1       Ca1       O3                 52.7(6)      1_555  .      1_555  N
  Sr1       Ca1       O3                127.3(6)      1_555  .     -1_566  N
  Sr1       Ca1       O4                112.9(5)      1_555  .      2_555  N
  Sr1       Ca1       O4                 67.1(5)      1_555  .     -2_566  N
  Sr1       Ca1       Sr3                72.3(5)     -1_566  .      1_455  N
  Sr1       Ca1       Sr3               106.5(4)     -1_566  .      2_645  N
  Sr1       Ca1       Sr3               110.9(4)     -1_566  .      2_655  N
  Sr1       Ca1       Sr3               107.7(5)     -1_566  .     -1_666  N
  Sr1       Ca1       Sr3                69.1(4)     -1_566  .     -2_466  N
  Sr1       Ca1       Sr3                73.5(4)     -1_566  .     -2_476  N
  Sr1       Ca1       O2                137.0(6)     -1_566  .      2_645  N
  Sr1       Ca1       O2                 43.0(6)     -1_566  .     -2_476  N
  Sr1       Ca1       O3                127.3(6)     -1_566  .      1_555  N
  Sr1       Ca1       O3                 52.7(6)     -1_566  .     -1_566  N
  Sr1       Ca1       O4                 67.1(5)     -1_566  .      2_555  N
  Sr1       Ca1       O4                112.9(5)     -1_566  .     -2_566  N
  Sr3       Ca1       Sr3                70.8(4)      1_455  .      2_645  N
  Sr3       Ca1       Sr3                68.2(5)      1_455  .      2_655  N
  Sr3       Ca1       Sr3                  180.0      1_455  .     -1_666  N
  Sr3       Ca1       Sr3               111.8(5)      1_455  .     -2_466  N
  Sr3       Ca1       Sr3               109.2(4)      1_455  .     -2_476  N
  Sr3       Ca1       O2                 65.1(7)      1_455  .      2_645  N
  Sr3       Ca1       O2                114.9(7)      1_455  .     -2_476  N
  Sr3       Ca1       O3                132.7(7)      1_455  .      1_555  N
  Sr3       Ca1       O3                 47.3(7)      1_455  .     -1_566  N
  Sr3       Ca1       O4                 50.5(6)      1_455  .      2_555  N
  Sr3       Ca1       O4                129.5(6)      1_455  .     -2_566  N
  Sr3       Ca1       Sr3               110.6(6)      2_645  .      2_655  N
  Sr3       Ca1       Sr3               109.2(4)      2_645  .     -1_666  N
  Sr3       Ca1       Sr3                69.4(6)      2_645  .     -2_466  N
  Sr3       Ca1       Sr3                  180.0      2_645  .     -2_476  N
  Sr3       Ca1       O2                 54.3(6)      2_645  .      2_645  N
  Sr3       Ca1       O2                125.7(6)      2_645  .     -2_476  N
  Sr3       Ca1       O3                124.7(6)      2_645  .      1_555  N
  Sr3       Ca1       O3                 55.3(6)      2_645  .     -1_566  N
  Sr3       Ca1       O4                120.6(6)      2_645  .      2_555  N
  Sr3       Ca1       O4                 59.4(6)      2_645  .     -2_566  N
  Sr3       Ca1       Sr3               111.8(5)      2_655  .     -1_666  N
  Sr3       Ca1       Sr3                  180.0      2_655  .     -2_466  N
  Sr3       Ca1       Sr3                69.4(6)      2_655  .     -2_476  N
  Sr3       Ca1       O2                 58.3(6)      2_655  .      2_645  N
  Sr3       Ca1       O2                121.7(6)      2_655  .     -2_476  N
  Sr3       Ca1       O3                 64.5(6)      2_655  .      1_555  N
  Sr3       Ca1       O3                115.5(6)      2_655  .     -1_566  N
  Sr3       Ca1       O4                 44.0(6)      2_655  .      2_555  N
  Sr3       Ca1       O4                136.0(6)      2_655  .     -2_566  N
  Sr3       Ca1       Sr3                68.2(5)     -1_666  .     -2_466  N
  Sr3       Ca1       Sr3                70.8(4)     -1_666  .     -2_476  N
  Sr3       Ca1       O2                114.9(7)     -1_666  .      2_645  N
  Sr3       Ca1       O2                 65.1(7)     -1_666  .     -2_476  N
  Sr3       Ca1       O3                 47.3(7)     -1_666  .      1_555  N
  Sr3       Ca1       O3                132.7(7)     -1_666  .     -1_566  N
  Sr3       Ca1       O4                129.5(6)     -1_666  .      2_555  N
  Sr3       Ca1       O4                 50.5(6)     -1_666  .     -2_566  N
  Sr3       Ca1       Sr3               110.6(6)     -2_466  .     -2_476  N
  Sr3       Ca1       O2                121.7(6)     -2_466  .      2_645  N
  Sr3       Ca1       O2                 58.3(6)     -2_466  .     -2_476  N
  Sr3       Ca1       O3                115.5(6)     -2_466  .      1_555  N
  Sr3       Ca1       O3                 64.5(6)     -2_466  .     -1_566  N
  Sr3       Ca1       O4                136.0(6)     -2_466  .      2_555  N
  Sr3       Ca1       O4                 44.0(6)     -2_466  .     -2_566  N
  Sr3       Ca1       O2                125.7(6)     -2_476  .      2_645  N
  Sr3       Ca1       O2                 54.3(6)     -2_476  .     -2_476  N
  Sr3       Ca1       O3                 55.3(6)     -2_476  .      1_555  N
  Sr3       Ca1       O3                124.7(6)     -2_476  .     -1_566  N
  Sr3       Ca1       O4                 59.4(6)     -2_476  .      2_555  N
  Sr3       Ca1       O4                120.6(6)     -2_476  .     -2_566  N
  O2        Ca1       O2                   180.0      2_645  .     -2_476  N
  O2        Ca1       O3                 88.0(7)      2_645  .      1_555  N
  O2        Ca1       O3                 92.0(7)      2_645  .     -1_566  N
  O2        Ca1       O4                 89.4(7)      2_645  .      2_555  N
  O2        Ca1       O4                 90.6(7)      2_645  .     -2_566  N
  O2        Ca1       O3                 92.0(7)     -2_476  .      1_555  N
  O2        Ca1       O3                 88.0(7)     -2_476  .     -1_566  N
  O2        Ca1       O4                 90.6(7)     -2_476  .      2_555  N
  O2        Ca1       O4                 89.4(7)     -2_476  .     -2_566  N
  O3        Ca1       O3                   180.0      1_555  .     -1_566  N
  O3        Ca1       O4                 93.9(8)      1_555  .      2_555  N
  O3        Ca1       O4                 86.1(8)      1_555  .     -2_566  N
  O3        Ca1       O4                 86.1(8)     -1_566  .      2_555  N
  O3        Ca1       O4                 93.9(8)     -1_566  .     -2_566  N
  O4        Ca1       O4                   180.0      2_555  .     -2_566  N
  Sr1       Ca2       Sr1                  180.0      2_646  .     -2_554  N
  Sr1       Ca2       Sr2               109.5(5)      2_646  .      1_555  N
  Sr1       Ca2       Sr2              72.99(32)      2_646  .      2_645  N
  Sr1       Ca2       Sr2                68.6(4)      2_646  .      2_655  N
  Sr1       Ca2       Sr2                70.5(5)      2_646  .     -1_656  N
  Sr1       Ca2       Sr2               111.4(4)      2_646  .     -2_556  N
  Sr1       Ca2       Sr2             107.01(32)      2_646  .     -2_566  N
  Sr1       Ca2       O1                115.2(6)      2_646  .      1_545  N
  Sr1       Ca2       O1                 64.8(6)      2_646  .     -1_666  N
  Sr1       Ca2       O5                 53.5(5)      2_646  .      2_646  N
  Sr1       Ca2       O5                126.5(5)      2_646  .     -2_565  N
  Sr1       Ca2       O8                135.4(7)      2_646  .      1_555  N
  Sr1       Ca2       O8                 44.6(7)      2_646  .     -1_656  N
  Sr1       Ca2       Sr2                70.5(5)     -2_565  .      1_555  N
  Sr1       Ca2       Sr2             107.01(32)     -2_565  .      2_645  N
  Sr1       Ca2       Sr2               111.4(4)     -2_565  .      2_655  N
  Sr1       Ca2       Sr2               109.5(5)     -2_565  .     -1_656  N
  Sr1       Ca2       Sr2                68.6(4)     -2_565  .     -2_556  N
  Sr1       Ca2       Sr2              72.99(32)     -2_565  .     -2_566  N
  Sr1       Ca2       O1                 64.8(6)     -2_565  .      1_545  N
  Sr1       Ca2       O1                115.2(6)     -2_565  .     -1_666  N
  Sr1       Ca2       O5                126.5(5)     -2_565  .      2_646  N
  Sr1       Ca2       O5                 53.5(5)     -2_565  .     -2_565  N
  Sr1       Ca2       O8                 44.6(7)     -2_565  .      1_555  N
  Sr1       Ca2       O8                135.4(7)     -2_565  .     -1_656  N
  Sr2       Ca2       Sr2              72.37(34)      1_555  .      2_645  N
  Sr2       Ca2       Sr2                69.4(4)      1_555  .      2_655  N
  Sr2       Ca2       Sr2                  180.0      1_555  .     -1_656  N
  Sr2       Ca2       Sr2               110.6(4)      1_555  .     -2_556  N
  Sr2       Ca2       Sr2             107.63(34)      1_555  .     -2_566  N
  Sr2       Ca2       O1                134.2(6)      1_555  .      1_545  N
  Sr2       Ca2       O1                 45.8(6)      1_555  .     -1_666  N
  Sr2       Ca2       O5                113.9(6)      1_555  .      2_646  N
  Sr2       Ca2       O5                 66.1(6)      1_555  .     -2_565  N
  Sr2       Ca2       O8                 53.1(8)      1_555  .      1_555  N
  Sr2       Ca2       O8                126.9(8)      1_555  .     -1_656  N
  Sr2       Ca2       Sr2               110.5(7)      2_645  .      2_655  N
  Sr2       Ca2       Sr2             107.63(34)      2_645  .     -1_656  N
  Sr2       Ca2       Sr2                69.5(7)      2_645  .     -2_556  N
  Sr2       Ca2       Sr2                  180.0      2_645  .     -2_566  N
  Sr2       Ca2       O1                129.8(7)      2_645  .      1_545  N
  Sr2       Ca2       O1                 50.2(7)      2_645  .     -1_666  N
  Sr2       Ca2       O5                125.6(6)      2_645  .      2_646  N
  Sr2       Ca2       O5                 54.4(6)      2_645  .     -2_565  N
  Sr2       Ca2       O8                123.2(8)      2_645  .      1_555  N
  Sr2       Ca2       O8                 56.8(8)      2_645  .     -1_656  N
  Sr2       Ca2       Sr2               110.6(4)      2_655  .     -1_656  N
  Sr2       Ca2       Sr2                  180.0      2_655  .     -2_556  N
  Sr2       Ca2       Sr2                69.5(7)      2_655  .     -2_566  N
  Sr2       Ca2       O1                118.6(6)      2_655  .      1_545  N
  Sr2       Ca2       O1                 61.4(6)      2_655  .     -1_666  N
  Sr2       Ca2       O5                 44.5(7)      2_655  .      2_646  N
  Sr2       Ca2       O5                135.5(7)      2_655  .     -2_565  N
  Sr2       Ca2       O8                 66.9(6)      2_655  .      1_555  N
  Sr2       Ca2       O8                113.1(6)      2_655  .     -1_656  N
  Sr2       Ca2       Sr2                69.4(4)     -1_656  .     -2_556  N
  Sr2       Ca2       Sr2              72.37(34)     -1_656  .     -2_566  N
  Sr2       Ca2       O1                 45.8(6)     -1_656  .      1_545  N
  Sr2       Ca2       O1                134.2(6)     -1_656  .     -1_666  N
  Sr2       Ca2       O5                 66.1(6)     -1_656  .      2_646  N
  Sr2       Ca2       O5                113.9(6)     -1_656  .     -2_565  N
  Sr2       Ca2       O8                126.9(8)     -1_656  .      1_555  N
  Sr2       Ca2       O8                 53.1(8)     -1_656  .     -1_656  N
  Sr2       Ca2       Sr2               110.5(7)     -2_556  .     -2_566  N
  Sr2       Ca2       O1                 61.4(6)     -2_556  .      1_545  N
  Sr2       Ca2       O1                118.6(6)     -2_556  .     -1_666  N
  Sr2       Ca2       O5                135.5(7)     -2_556  .      2_646  N
  Sr2       Ca2       O5                 44.5(7)     -2_556  .     -2_565  N
  Sr2       Ca2       O8                113.1(6)     -2_556  .      1_555  N
  Sr2       Ca2       O8                 66.9(6)     -2_556  .     -1_656  N
  Sr2       Ca2       O1                 50.2(7)     -2_566  .      1_545  N
  Sr2       Ca2       O1                129.8(7)     -2_566  .     -1_666  N
  Sr2       Ca2       O5                 54.4(6)     -2_566  .      2_646  N
  Sr2       Ca2       O5                125.6(6)     -2_566  .     -2_565  N
  Sr2       Ca2       O8                 56.8(8)     -2_566  .      1_555  N
  Sr2       Ca2       O8                123.2(8)     -2_566  .     -1_656  N
  O1        Ca2       O1                   180.0      1_545  .     -1_666  N
  O1        Ca2       O5                 86.3(8)      1_545  .      2_646  N
  O1        Ca2       O5                 93.7(8)      1_545  .     -2_565  N
  O1        Ca2       O8                 86.9(8)      1_545  .      1_555  N
  O1        Ca2       O8                 93.1(8)      1_545  .     -1_656  N
  O1        Ca2       O5                 93.7(8)     -1_666  .      2_646  N
  O1        Ca2       O5                 86.3(8)     -1_666  .     -2_565  N
  O1        Ca2       O8                 93.1(8)     -1_666  .      1_555  N
  O1        Ca2       O8                 86.9(8)     -1_666  .     -1_656  N
  O5        Ca2       O5                   180.0      2_646  .     -2_565  N
  O5        Ca2       O8                 93.1(8)      2_646  .      1_555  N
  O5        Ca2       O8                 86.9(8)      2_646  .     -1_656  N
  O5        Ca2       O8                 86.9(8)     -2_565  .      1_555  N
  O5        Ca2       O8                 93.1(8)     -2_565  .     -1_656  N
  O8        Ca2       O8                   180.0      1_555  .     -1_656  N
  Sr1       Ir1       Sr1               107.7(5)      1_555  .     -2_565  N
  Sr1       Ir1       Sr3               177.9(8)      1_555  .     -1_676  N
  Sr1       Ir1       Sr3               109.5(6)      1_555  .     -2_476  N
  Sr1       Ir1       O2                129.0(9)      1_555  .     -1_676  N
  Sr1       Ir1       O3                 57.7(8)      1_555  .      1_555  N
  Sr1       Ir1       O4               126.9(11)      1_555  .     -2_576  N
  Sr1       Ir1       O6                122.3(8)      1_555  .      2_656  N
  Sr1       Ir1       O7                 55.6(7)      1_555  .     -1_667  N
  Sr1       Ir1       O9                 52.6(7)      1_555  .     -2_576  N
  Sr1       Ir1       Sr3                74.1(6)     -2_576  .     -1_676  N
  Sr1       Ir1       Sr3               111.1(6)     -2_576  .     -2_476  N
  Sr1       Ir1       O2                 42.9(7)     -2_576  .     -1_676  N
  Sr1       Ir1       O3               112.6(10)     -2_576  .      1_555  N
  Sr1       Ir1       O4               124.6(10)     -2_576  .     -2_576  N
  Sr1       Ir1       O6                69.1(10)     -2_576  .      2_656  N
  Sr1       Ir1       O7                 53.7(9)     -2_576  .     -1_667  N
  Sr1       Ir1       O9                134.0(9)     -2_576  .     -2_576  N
  Sr3       Ir1       Sr3                70.6(4)     -1_676  .     -2_476  N
  Sr3       Ir1       O2                 53.1(8)     -1_676  .     -1_676  N
  Sr3       Ir1       O3                122.9(8)     -1_676  .      1_555  N
  Sr3       Ir1       O4                 51.5(7)     -1_676  .     -2_576  N
  Sr3       Ir1       O6                 57.0(8)     -1_676  .      2_656  N
  Sr3       Ir1       O7               125.8(12)     -1_676  .     -1_667  N
  Sr3       Ir1       O9                125.3(9)     -1_676  .     -2_576  N
  Sr3       Ir1       O2                 68.7(6)     -2_476  .     -1_676  N
  Sr3       Ir1       O3                 53.8(8)     -2_476  .      1_555  N
  Sr3       Ir1       O4                 46.2(8)     -2_476  .     -2_576  N
  Sr3       Ir1       O6                125.7(9)     -2_476  .      2_656  N
  Sr3       Ir1       O7                137.4(9)     -2_476  .     -1_667  N
  Sr3       Ir1       O9               114.7(10)     -2_476  .     -2_576  N
  O2        Ir1       O3                 92.3(9)     -1_676  .      1_555  N
  O2        Ir1       O4                89.9(10)     -1_676  .     -2_576  N
  O2        Ir1       O6                89.0(12)     -1_676  .      2_656  N
  O2        Ir1       O7                90.2(12)     -1_676  .     -1_667  N
  O2        Ir1       O9               176.0(13)     -1_676  .     -2_576  N
  O3        Ir1       O4                91.6(12)      1_555  .     -2_576  N
  O3        Ir1       O6               178.2(16)      1_555  .      2_656  N
  O3        Ir1       O7                92.6(10)      1_555  .     -1_667  N
  O3        Ir1       O9                91.5(12)      1_555  .     -2_576  N
  O4        Ir1       O6                87.2(10)     -2_576  .      2_656  N
  O4        Ir1       O7               175.9(12)     -2_576  .     -1_667  N
  O4        Ir1       O9                91.3(11)     -2_576  .     -2_576  N
  O6        Ir1       O7                88.7(12)      2_656  .     -1_667  N
  O6        Ir1       O9                87.3(11)      2_656  .     -2_576  N
  O7        Ir1       O9                88.4(12)     -1_667  .     -2_576  N
  Sr1       Ir2       Sr1               109.5(6)      1_554  .     -2_564  N
  Sr1       Ir2       Sr2                71.7(6)      1_554  .      1_555  N
  Sr1       Ir2       Sr2               175.5(5)      1_554  .     -2_566  N
  Sr1       Ir2       Sr3                73.4(6)      1_554  .     -1_665  N
  Sr1       Ir2       O1                 64.2(8)      1_554  .     -2_575  N
  Sr1       Ir2       O5                131.6(9)      1_554  .     -2_575  N
  Sr1       Ir2       O6                 46.8(7)      1_554  .      2_645  N
  Sr1       Ir2       O7                 53.0(8)      1_554  .     -1_666  N
  Sr1       Ir2       O8               126.0(10)      1_554  .      1_555  N
  Sr1       Ir2       O9                119.2(9)      1_554  .      1_555  N
  Sr1       Ir2       Sr2               176.1(6)     -2_575  .      1_555  N
  Sr1       Ir2       Sr2                71.7(5)     -2_575  .     -2_566  N
  Sr1       Ir2       Sr3                73.8(5)     -2_575  .     -1_665  N
  Sr1       Ir2       O1                128.2(8)     -2_575  .     -2_575  N
  Sr1       Ir2       O5                 58.1(9)     -2_575  .     -2_575  N
  Sr1       Ir2       O6                127.7(9)     -2_575  .      2_645  N
  Sr1       Ir2       O7                 58.0(7)     -2_575  .     -1_666  N
  Sr1       Ir2       O8               123.8(11)     -2_575  .      1_555  N
  Sr1       Ir2       O9                 54.7(9)     -2_575  .      1_555  N
  Sr2       Ir2       Sr2               106.8(5)      1_555  .     -2_566  N
  Sr2       Ir2       Sr3               110.1(6)      1_555  .     -1_665  N
  Sr2       Ir2       O1                 48.6(7)      1_555  .     -2_575  N
  Sr2       Ir2       O5                118.2(8)      1_555  .     -2_575  N
  Sr2       Ir2       O6                 55.9(9)      1_555  .      2_645  N
  Sr2       Ir2       O7               122.1(11)      1_555  .     -1_666  N
  Sr2       Ir2       O8                 55.8(8)      1_555  .      1_555  N
  Sr2       Ir2       O9               128.3(10)      1_555  .      1_555  N
  Sr2       Ir2       Sr3               111.1(6)     -2_566  .     -1_665  N
  Sr2       Ir2       O1                111.5(9)     -2_566  .     -2_575  N
  Sr2       Ir2       O5                 45.0(8)     -2_566  .     -2_575  N
  Sr2       Ir2       O6                136.1(9)     -2_566  .      2_645  N
  Sr2       Ir2       O7               126.9(10)     -2_566  .     -1_666  N
  Sr2       Ir2       O8                 53.7(9)     -2_566  .      1_555  N
  Sr2       Ir2       O9                65.2(10)     -2_566  .      1_555  N
  Sr3       Ir2       O1                136.5(9)     -1_665  .     -2_575  N
  Sr3       Ir2       O5               130.3(10)     -1_665  .     -2_575  N
  Sr3       Ir2       O6                 55.8(8)     -1_665  .      2_645  N
  Sr3       Ir2       O7                 72.0(8)     -1_665  .     -1_666  N
  Sr3       Ir2       O8                111.7(9)     -1_665  .      1_555  N
  Sr3       Ir2       O9                46.2(10)     -1_665  .      1_555  N
  O1        Ir2       O5                87.2(11)     -2_575  .     -2_575  N
  O1        Ir2       O6                87.1(10)     -2_575  .      2_645  N
  O1        Ir2       O7                88.9(10)     -2_575  .     -1_666  N
  O1        Ir2       O8                87.4(10)     -2_575  .      1_555  N
  O1        Ir2       O9               175.4(14)     -2_575  .      1_555  N
  O5        Ir2       O6               173.8(14)     -2_575  .      2_645  N
  O5        Ir2       O7                90.9(11)     -2_575  .     -1_666  N
  O5        Ir2       O8                87.7(12)     -2_575  .      1_555  N
  O5        Ir2       O9                92.3(11)     -2_575  .      1_555  N
  O6        Ir2       O7                91.2(12)      2_645  .     -1_666  N
  O6        Ir2       O8                89.9(12)      2_645  .      1_555  N
  O6        Ir2       O9                93.3(12)      2_645  .      1_555  N
  O7        Ir2       O8               176.1(13)     -1_666  .      1_555  N
  O7        Ir2       O9                95.8(12)     -1_666  .      1_555  N
  O8        Ir2       O9                87.9(11)      1_555  .      1_555  N
  Sr2       O1        Sr2               104.7(9)     -1_666  .     -2_576  N
  Sr2       O1        Ca2                98.6(8)     -1_666  .      1_565  N
  Sr2       O1        Ir2              100.8(11)     -1_666  .     -2_576  N
  Sr2       O1        Ca2               91.3(11)     -2_576  .      1_565  N
  Sr2       O1        Ir2               94.0(10)     -2_576  .     -2_576  N
  Ca2       O1        Ir2              157.9(12)      1_565  .     -2_576  N
  Sr1       O2        Sr3               105.7(9)      2_655  .      1_555  N
  Sr1       O2        Ca1                97.9(9)      2_655  .      2_655  N
  Sr1       O2        Ir1               106.5(9)      2_655  .     -1_676  N
  Sr3       O2        Ca1                83.5(8)      1_555  .      2_655  N
  Sr3       O2        Ir1               94.4(11)      1_555  .     -1_676  N
  Ca1       O2        Ir1              155.1(11)      2_655  .     -1_676  N
  Sr1       O3        Sr3              100.5(10)      1_555  .     -1_666  N
  Sr1       O3        Sr3              162.5(11)      1_555  .     -2_476  N
  Sr1       O3        Ca1                89.0(7)      1_555  .      1_555  N
  Sr1       O3        Ir1                88.2(9)      1_555  .      1_555  N
  Sr3       O3        Sr3                95.8(8)     -1_666  .     -2_476  N
  Sr3       O3        Ca1               93.2(11)     -1_666  .      1_555  N
  Sr3       O3        Ir1              107.3(11)     -1_666  .      1_555  N
  Sr3       O3        Ca1                83.8(7)     -2_476  .      1_555  N
  Sr3       O3        Ir1               93.0(11)     -2_476  .      1_555  N
  Ca1       O3        Ir1              159.4(14)      1_555  .      1_555  N
  Sr3       O4        Sr3                99.1(8)      1_455  .      2_645  N
  Sr3       O4        Sr3                92.8(9)      1_455  .     -1_665  N
  Sr3       O4        Ca1                98.9(9)      1_455  .      2_545  N
  Sr3       O4        Ir1               99.9(11)      1_455  .     -2_575  N
  Sr3       O4        Sr3              166.1(10)      2_645  .     -1_665  N
  Sr3       O4        Ca1                90.5(8)      2_645  .      2_545  N
  Sr3       O4        Ir1               93.9(10)      2_645  .     -2_575  N
  Sr3       O4        Ca1                80.6(7)     -1_665  .      2_545  N
  Sr3       O4        Ir1               91.0(10)     -1_665  .     -2_575  N
  Ca1       O4        Ir1              159.7(12)      2_545  .     -2_575  N
  Sr1       O5        Sr2                96.4(9)      1_555  .      1_566  N
  Sr1       O5        Sr2              163.2(10)      1_555  .     -1_666  N
  Sr1       O5        Ca2                85.5(9)      1_555  .      2_656  N
  Sr1       O5        Ir2               86.4(10)      1_555  .     -2_576  N
  Sr2       O5        Sr2                97.2(9)      1_566  .     -1_666  N
  Sr2       O5        Ca2               96.8(11)      1_566  .      2_656  N
  Sr2       O5        Ir2              103.0(12)      1_566  .     -2_576  N
  Sr2       O5        Ca2                83.2(7)     -1_666  .      2_656  N
  Sr2       O5        Ir2               99.9(12)     -1_666  .     -2_576  N
  Ca2       O5        Ir2              159.3(11)      2_656  .     -2_576  N
  Sr1       O6        Sr2               96.8(10)      2_656  .      2_655  N
  Sr1       O6        Sr3               99.3(10)      2_656  .     -2_576  N
  Sr1       O6        Ir1              105.4(11)      2_656  .      2_646  N
  Sr1       O6        Ir2               99.2(12)      2_656  .      2_655  N
  Sr2       O6        Sr3              163.9(11)      2_655  .     -2_576  N
  Sr2       O6        Ir1               89.5(11)      2_655  .      2_646  N
  Sr2       O6        Ir2                88.9(9)      2_655  .      2_655  N
  Sr3       O6        Ir1               85.1(10)     -2_576  .      2_646  N
  Sr3       O6        Ir2               89.7(11)     -2_576  .      2_655  N
  Ir1       O6        Ir2              155.4(13)      2_646  .      2_655  N
  Sr1       O7        Sr1              163.4(12)      2_646  .     -1_667  N
  Sr1       O7        Sr2               99.1(11)      2_646  .     -1_656  N
  Sr1       O7        Ir1               90.1(11)      2_646  .     -1_667  N
  Sr1       O7        Ir2               83.7(10)      2_646  .     -1_666  N
  Sr1       O7        Sr2               97.5(10)     -1_667  .     -1_656  N
  Sr1       O7        Ir1               86.8(10)     -1_667  .     -1_667  N
  Sr1       O7        Ir2               91.2(10)     -1_667  .     -1_666  N
  Sr2       O7        Ir1              100.7(12)     -1_656  .     -1_667  N
  Sr2       O7        Ir2              108.1(11)     -1_656  .     -1_666  N
  Ir1       O7        Ir2              151.1(13)     -1_667  .     -1_666  N
  Sr1       O8        Sr2               99.7(12)     -2_565  .      1_555  N
  Sr1       O8        Sr2              100.2(11)     -2_565  .     -2_566  N
  Sr1       O8        Ca2                96.1(9)     -2_565  .      1_555  N
  Sr1       O8        Ir2              108.4(10)     -2_565  .      1_555  N
  Sr2       O8        Sr2              158.9(11)      1_555  .     -2_566  N
  Sr2       O8        Ca2                88.5(8)      1_555  .      1_555  N
  Sr2       O8        Ir2               88.7(10)      1_555  .      1_555  N
  Sr2       O8        Ca2                82.5(9)     -2_566  .      1_555  N
  Sr2       O8        Ir2               91.7(11)     -2_566  .      1_555  N
  Ca2       O8        Ir2              155.5(13)      1_555  .      1_555  N
  Sr1       O9        Sr3              101.7(10)     -2_575  .     -1_665  N
  Sr1       O9        Ir1               87.8(10)     -2_575  .     -2_575  N
  Sr1       O9        Ir2               89.4(11)     -2_575  .      1_555  N
  Sr3       O9        Ir1               97.4(10)     -1_665  .     -2_575  N
  Sr3       O9        Ir2              101.2(12)     -1_665  .      1_555  N
  Ir1       O9        Ir2              161.4(15)     -2_575  .      1_555  N

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sr1 Sr2 4.044(25) . 1_556 N
Sr1 Sr2 3.975(21) . 1_566 N
Sr1 Sr2 4.035(33) . -2_555 N
Sr1 Sr3 4.152(20) . 2_645 N
Sr1 Sr3 4.059(25) . 2_655 N
Sr1 Sr3 4.159(32) . -1_666 N
Sr1 Ca1 3.572(23) . 1_555 N
Sr1 Ca2 3.452(24) . 2_656 N
Sr1 Ir1 3.731(21) . 1_545 N
Sr1 Ir1 3.362(24) . 1_555 N
Sr1 Ir1 3.469(29) . -2_564 N
Sr1 Ir2 3.479(26) . 1_556 N
Sr1 Ir2 3.602(21) . -2_555 N
Sr1 Ir2 3.274(21) . -2_565 N
Sr1 O1 3.182(30) . -2_565 N
Sr1 O2 2.461(28) . 2_645 N
Sr1 O3 2.842(31) . 1_555 N
Sr1 O4 3.385(26) . -2_555 N
Sr1 O5 2.785(28) . 1_555 N
Sr1 O6 2.569(27) . 2_646 N
Sr1 O6 3.356(27) . -1_666 N
Sr1 O7 2.794(25) . 2_656 N
Sr1 O7 2.779(26) . -1_667 N
Sr1 O8 2.44(4) . -2_555 N
Sr1 O9 3.094(27) . -2_555 N
Sr1 O9 2.673(28) . -2_565 N
Sr2 Sr1 3.975(21) . 1_544 N
Sr2 Sr1 4.044(25) . 1_554 N
Sr2 Sr1 4.035(33) . -2_554 N
Sr2 Sr2 4.068(25) . 2_645 N
Sr2 Sr2 4.068(25) . 2_655 N
Sr2 Sr2 3.97(5) . -1_655 N
Sr2 Ca2 3.539(23) . 1_555 N
Sr2 Ca2 3.603(22) . 2_645 N
Sr2 Ca2 3.346(19) . 2_655 N
Sr2 Ir1 3.519(19) . 1_544 N
Sr2 Ir2 3.685(27) . 1_545 N
Sr2 Ir2 3.422(29) . 1_555 N
Sr2 Ir2 3.596(23) . 2_645 N
Sr2 Ir2 3.502(33) . -2_554 N
Sr2 O1 2.566(24) . -1_666 N
Sr2 O1 3.184(24) . -2_554 N
Sr2 O1 2.573(24) . -2_564 N
Sr2 O5 2.54(4) . 1_544 N
Sr2 O5 2.740(27) . -1_666 N
Sr2 O5 3.343(32) . -2_554 N
Sr2 O6 2.835(28) . 2_645 N
Sr2 O7 2.502(32) . -1_656 N
Sr2 O8 2.83(4) . 1_555 N
Sr2 O8 3.405(27) . 2_645 N
Sr2 O8 2.824(33) . -2_554 N
Sr2 O9 3.211(32) . -2_554 N
Sr3 Sr1 4.059(25) . 2_645 N
Sr3 Sr1 4.152(20) . 2_655 N
Sr3 Sr1 4.159(32) . -1_666 N
Sr3 Sr3 3.965(28) . 2_745 N
Sr3 Sr3 3.965(28) . 2_755 N
Sr3 Sr3 3.96(5) . -1_765 N
Sr3 Ca1 3.480(23) . 1_655 N
Sr3 Ca1 3.586(22) . 2_645 N
Sr3 Ca1 3.360(18) . 2_655 N
Sr3 Ir1 3.544(35) . 2_645 N
Sr3 Ir1 3.607(25) . -1_666 N
Sr3 Ir1 3.423(28) . -1_676 N
Sr3 Ir1 3.439(24) . -2_664 N
Sr3 Ir2 3.483(19) . -1_665 N
Sr3 O2 3.077(23) . 1_545 N
Sr3 O2 2.745(23) . 1_555 N
Sr3 O2 3.258(26) . 2_745 N
Sr3 O3 3.306(30) . 2_645 N
Sr3 O3 2.563(28) . -1_666 N
Sr3 O3 2.778(25) . -2_664 N
Sr3 O4 2.521(28) . 1_655 N
Sr3 O4 2.687(30) . 2_655 N
Sr3 O4 2.930(29) . -1_665 N
Sr3 O6 2.882(30) . -2_564 N
Sr3 O9 2.561(34) . -1_665 N
Ca1 Sr1 3.572(23) . 1_555 N
Ca1 Sr1 3.572(23) . -1_566 N
Ca1 Sr3 3.480(23) . 1_455 N
Ca1 Sr3 3.360(18) . 2_645 N
Ca1 Sr3 3.586(22) . 2_655 N
Ca1 Sr3 3.480(23) . -1_666 N
Ca1 Sr3 3.586(22) . -2_455 N
Ca1 Sr3 3.360(18) . -2_465 N
Ca1 O2 2.272(19) . 2_645 N
Ca1 O2 2.272(19) . -2_465 N
Ca1 O3 2.215(23) . 1_555 N
Ca1 O3 2.215(23) . -1_566 N
Ca1 O4 2.191(22) . 2_555 N
Ca1 O4 2.191(22) . -2_555 N
Ca2 Sr1 3.452(24) . 2_646 N
Ca2 Sr1 3.452(24) . -2_554 N
Ca2 Sr2 3.539(23) . 1_555 N
Ca2 Sr2 3.346(19) . 2_645 N
Ca2 Sr2 3.603(22) . 2_655 N
Ca2 Sr2 3.539(23) . -1_656 N
Ca2 Sr2 3.603(22) . -2_545 N
Ca2 Sr2 3.346(19) . -2_555 N
Ca2 O1 2.082(22) . 1_545 N
Ca2 O1 2.082(22) . -1_666 N
Ca2 O5 2.270(26) . 2_646 N
Ca2 O5 2.270(26) . -2_554 N
Ca2 O8 2.201(20) . 1_555 N
Ca2 O8 2.201(20) . -1_656 N
Ir1 Sr1 3.362(24) . 1_555 N
Ir1 Sr1 3.731(21) . 1_565 N
Ir1 Sr1 3.469(29) . -2_565 N
Ir1 Sr2 3.519(19) . 1_566 N
Ir1 Sr3 3.544(35) . 2_655 N
Ir1 Sr3 3.607(25) . -1_666 N
Ir1 Sr3 3.423(28) . -1_676 N
Ir1 Sr3 3.439(24) . -2_465 N
Ir1 O2 1.844(22) . -1_676 N
Ir1 O3 1.887(33) . 1_555 N
Ir1 O4 1.945(26) . -2_565 N
Ir1 O6 2.109(32) . 2_656 N
Ir1 O7 2.052(25) . -1_667 N
Ir1 O9 2.142(31) . -2_565 N
Ir2 Sr1 3.479(26) . 1_554 N
Ir2 Sr1 3.602(21) . -2_554 N
Ir2 Sr1 3.274(21) . -2_564 N
Ir2 Sr2 3.422(29) . 1_555 N
Ir2 Sr2 3.685(27) . 1_565 N
Ir2 Sr2 3.596(23) . 2_655 N
Ir2 Sr2 3.502(33) . -2_555 N
Ir2 Sr3 3.483(19) . -1_665 N
Ir2 O1 2.083(24) . -2_564 N
Ir2 O5 1.904(32) . -2_564 N
Ir2 O6 1.971(33) . 2_645 N
Ir2 O7 2.038(31) . -1_666 N
Ir2 O8 1.991(27) . 1_555 N
Ir2 O9 1.918(25) . 1_555 N
O1 Sr1 3.182(30) . -2_564 N
O1 Sr2 2.566(24) . -1_666 N
O1 Sr2 3.184(24) . -2_555 N
O1 Sr2 2.573(24) . -2_565 N
O1 Ca2 2.082(22) . 1_565 N
O1 Ir2 2.083(24) . -2_565 N
O2 Sr1 2.461(28) . 2_655 N
O2 Sr3 2.745(23) . 1_555 N
O2 Sr3 3.077(23) . 1_565 N
O2 Sr3 3.258(26) . 2_755 N
O2 Ca1 2.272(19) . 2_655 N
O2 Ir1 1.844(22) . -1_676 N
O3 Sr1 2.842(31) . 1_555 N
O3 Sr3 3.306(30) . 2_655 N
O3 Sr3 2.563(28) . -1_666 N
O3 Sr3 2.778(25) . -2_465 N
O3 Ca1 2.215(23) . 1_555 N
O3 Ir1 1.887(33) . 1_555 N
O4 Sr1 3.385(26) . -2_554 N
O4 Sr3 2.521(28) . 1_455 N
O4 Sr3 2.687(30) . 2_645 N
O4 Sr3 2.930(29) . -1_665 N
O4 Ca1 2.191(22) . 2_545 N
O4 Ir1 1.945(26) . -2_564 N
O5 Sr1 2.785(28) . 1_555 N
O5 Sr2 2.54(4) . 1_566 N
O5 Sr2 2.740(27) . -1_666 N
O5 Sr2 3.343(32) . -2_555 N
O5 Ca2 2.270(26) . 2_656 N
O5 Ir2 1.904(32) . -2_565 N
O6 Sr1 2.569(27) . 2_656 N
O6 Sr1 3.356(27) . -1_666 N
O6 Sr2 2.835(28) . 2_655 N
O6 Sr3 2.882(30) . -2_565 N
O6 Ir1 2.109(32) . 2_646 N
O6 Ir2 1.971(33) . 2_655 N
O7 Sr1 2.794(25) . 2_646 N
O7 Sr1 2.779(26) . -1_667 N
O7 Sr2 2.502(32) . -1_656 N
O7 Ir1 2.052(25) . -1_667 N
O7 Ir2 2.038(31) . -1_666 N
O8 Sr1 2.44(4) . -2_554 N
O8 Sr2 2.83(4) . 1_555 N
O8 Sr2 3.405(27) . 2_655 N
O8 Sr2 2.824(33) . -2_555 N
O8 Ca2 2.201(20) . 1_555 N
O8 Ir2 1.991(27) . 1_555 N
O9 Sr1 3.094(27) . -2_554 N
O9 Sr1 2.673(28) . -2_564 N
O9 Sr2 3.211(32) . -2_555 N
O9 Sr3 2.561(34) . -1_665 N
O9 Ir1 2.142(31) . -2_564 N
O9 Ir2 1.918(25) . 1_555 N

_diffrn_ambient_temperature      300
_diffrn_measurement_device_type  neutron
 _diffrn_radiation_type		 neutron

loop_
_atom_type_symbol
_atom_type_number_in_cell
_atom_type_scat_length_neutron
_atom_type_scat_source
Sr 12.0 0.7020 International_Tables_Vol_C
Ca 4.0 0.4700 International_Tables_Vol_C
Ir 8.0 1.0600 International_Tables_Vol_C
O 36.0 0.5803 International_Tables_Vol_C
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     2.0775
_pd_proc_ls_prof_R_factor        0.0412
_pd_proc_ls_prof_wR_factor       0.0558
_pd_proc_ls_prof_wR_expected     0.0319
_refine_ls_R_Fsqd_factor         0.07991

_pd_proc_ls_background_function  
;   GSAS Background function number 1 with  8 terms.
 Shifted Chebyshev function of 1st kind
      1:    675.105     2:   -149.349     3:    215.389     4:   -24.9233    
      5:    74.5966     6:   -9.13956     7:   -4.78014     8:   -1.97717    
;

_exptl_absorpt_process_details   
;   GSAS Absorption/surface roughness correction: function number 0
 Debye-Scherrer absorption correction
Term (= MU.r/wave) =     0.50000    
Correction is not refined.
;
_exptl_absorpt_correction_T_min  0.18502
_exptl_absorpt_correction_T_max  0.27792

_pd_proc_ls_profile_function     
;
 CW Profile function number 3 with  19 terms
 Pseudovoigt profile coefficients as parameterized in
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 Asymmetry correction of L.W. Finger, D.E. Cox & A. P. Jephcoat (1994).
 J. Appl. Cryst.,27,892-900.
 #1(GU)   =  577.646 #2(GV)   = -243.439 #3(GW)   =  111.507
 #4(GP)   =    0.000 #5(LX)   =    4.894 #6(LY)   =    6.232
 #7(S/L)  =   0.0463 #8(H/L)  =   0.0327
 #9(trns) =     0.00 #10(shft)=   0.0000
 #11(stec)=     0.40 #12(ptec)=    -0.23 #13(sfec)=     0.00
 #14(L11) =    0.000 #15(L22) =    0.000 #16(L33) =    0.000
 #17(L12) =    0.000 #18(L13) =    0.000 #19(L23) =    0.000
 Peak tails are ignored  where the intensity is below 0.0050 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_peak_cutoff          0.00500
_pd_proc_info_datetime           2015-08-04T15:46:19
_pd_calc_method                  'Rietveld Refinement'

#---- raw/calc data loop -----
_pd_meas_2theta_range_min        1.94
_pd_meas_2theta_range_max        163.64
_pd_meas_2theta_range_inc        0.05
_pd_proc_2theta_range_min        1.9469
_pd_proc_2theta_range_max        163.6469
_pd_proc_2theta_range_inc        0.05

loop_
_pd_meas_intensity_total
_pd_proc_ls_weight
_pd_proc_intensity_bkg_calc
_pd_calc_intensity_total
5620(160) 0.0 1269. .
5130(150) 0.0 1267. .
4980(150) 0.0 1265. .
4500(140) 0.0 1263. .
4340(140) 0.0 1261. .
3850(130) 0.0 1258. .
3920(130) 0.0 1256. .
3670(120) 0.0 1254. .
3680(120) 0.0 1252. .
3390(120) 0.0 1250. .
3240(110) 0.0 1248. .
3740(120) 0.0 1246. .
3720(120) 0.0 1244. .
3320(120) 0.0 1242. .
3190(110) 0.0 1240. .
3210(110) 0.0 1238. .
3070(110) 0.0 1235. .
3090(110) 0.0 1233. .
2900(110) 0.0 1231. .
2920(110) 0.0 1229. .
2630(100) 0.0 1227. .
2670(100) 0.0 1225. .
2580(100) 0.0 1223. .
2343(95) 0.0 1221. .
2401(96) 0.0 1219. .
2281(93) 0.0 1217. .
2083(88) 0.0 1215. .
2102(88) 0.0 1213. .
2128(89) 0.0 1211. .
1779(80) 0.0 1209. .
1854(82) 0.0 1207. .
1927(84) 0.0 1205. .
1927(84) 0.0 1203. .
1782(80) 0.0 1201. .
1746(79) 0.0 1199. .
1649(76) 0.0 1197. .
1719(78) 0.0 1195. .
1839(81) 0.0 1193. .
1720(78) 0.0 1191. .
1622(75) 0.0 1189. .
1594(74) 0.0 1187. .
1646(76) 0.0 1185. .
1753(79) 0.0 1184. .
1560(73) 0.0 1182. .
1638(75) 0.0 1180. .
1483(70) 0.0 1178. .
1578(73) 0.0 1176. .
1501(71) 0.0 1174. .
1399(68) 0.0 1172. .
1420(68) 0.0 1170. .
1398(68) 0.0 1168. .
1502(71) 0.0 1166. .
1345(66) 0.0 1164. .
1345(66) 0.0 1162. .
1324(65) 0.0 1161. .
1456(70) 0.0 1159. .
1344(66) 0.0 1157. .
1428(69) 0.0 1155. .
1279(63) 0.0 1153. .
1369(67) 0.0 1151. .
1228(61) 0.0 1149. .
1405(68) 0.0 1148. .
1292(64) 0.0002441 1146. 1146.
1273(63) 0.0002520 1144. 1144.
1312(65) 0.0002367 1142. 1142.
1284(63) 0.0002520 1140. 1140.
1183(60) 0.0002778 1138. 1138.
1141(58) 0.0002973 1137. 1137.
1281(63) 0.0002520 1135. 1135.
1245(62) 0.0002601 1133. 1133.
1232(62) 0.0002601 1131. 1131.
1270(63) 0.0002520 1129. 1129.
1224(61) 0.0002687 1127. 1127.
1138(58) 0.0002973 1126. 1126.
1250(62) 0.0002601 1124. 1124.
1263(63) 0.0002520 1122. 1122.
1284(63) 0.0002520 1120. 1120.
1119(57) 0.0003078 1119. 1119.
1219(61) 0.0002687 1117. 1117.
1226(61) 0.0002687 1115. 1115.
1194(60) 0.0002778 1113. 1113.
1083(56) 0.0003189 1111. 1111.
1127(57) 0.0003078 1110. 1110.
1123(57) 0.0003078 1108. 1108.
1205(61) 0.0002687 1106. 1106.
1089(56) 0.0003189 1104. 1104.
1149(58) 0.0002973 1103. 1103.
1066(55) 0.0003306 1101. 1101.
1090(56) 0.0003189 1099. 1099.
1125(57) 0.0003078 1097. 1097.
1305(64) 0.0002441 1096. 1096.
1151(58) 0.0002973 1094. 1094.
1202(60) 0.0002778 1092. 1092.
1025(53) 0.000356 1091. 1091.
1134(58) 0.0002973 1089. 1089.
1043(54) 0.0003429 1087. 1087.
1138(58) 0.0002973 1086. 1086.
975(51) 0.000384 1084. 1084.
1151(58) 0.0002973 1082. 1082.
1199(42) 0.000567 1080. 1080.
1205(42) 0.000567 1079. 1079.
1127(40) 0.000625 1077. 1077.
1171(41) 0.000595 1075. 1075.
1083(39) 0.000657 1074. 1074.
1040(38) 0.000693 1072. 1072.
1078(39) 0.000657 1070. 1070.
1059(38) 0.000693 1069. 1069.
1026(37) 0.000730 1067. 1067.
1039(38) 0.000693 1065. 1065.
1096(39) 0.000657 1064. 1064.
1114(40) 0.000625 1062. 1062.
1086(39) 0.000657 1061. 1061.
1080(39) 0.000657 1059. 1059.
1074(39) 0.000657 1057. 1057.
1060(38) 0.000693 1056. 1056.
1018(37) 0.000730 1054. 1054.
1055(38) 0.000693 1052. 1052.
1046(38) 0.000693 1051. 1051.
1012(37) 0.000730 1049. 1049.
1073(39) 0.000657 1048. 1048.
1022(37) 0.000730 1046. 1046.
1023(37) 0.000730 1044. 1045.
1013(37) 0.000730 1043. 1043.
1031(37) 0.000730 1041. 1041.
1054(38) 0.000693 1040. 1040.
1057(38) 0.000693 1038. 1038.
927(34) 0.000865 1036.5 1036.9
1000(36) 0.000772 1035. 1035.
1025(37) 0.000730 1033. 1034.
991(36) 0.000772 1032. 1032.
986(36) 0.000772 1030. 1031.
988(36) 0.000772 1029. 1029.
985(36) 0.000772 1027. 1028.
954(35) 0.000816 1025.5 1025.8
952(36) 0.000772 1024. 1024.
925(35) 0.000816 1022.4 1022.5
912(35) 0.000816 1020.9 1020.9
975(37) 0.000730 1019. 1019.
927(35) 0.000816 1017.8 1017.9
977(37) 0.000730 1016. 1016.
996(37) 0.000730 1015. 1015.
932(35) 0.000816 1013.3 1013.3
901(34) 0.000865 1011.8 1011.8
919(35) 0.000816 1010.3 1010.3
982(37) 0.000730 1009. 1009.
1002(38) 0.000693 1007. 1007.
946(36) 0.000772 1006. 1006.
930(35) 0.000816 1004.3 1004.3
990(37) 0.000730 1003. 1003.
982(37) 0.000730 1001. 1001.
1010(38) 0.000693 1000. 1000.
976(37) 0.000730 998. 998.
930(35) 0.000816 996.8 996.8
929(35) 0.000816 995.4 995.4
967(37) 0.000730 994. 994.
1044(39) 0.000657 992. 992.
975(37) 0.000730 991. 991.
962(36) 0.000772 990. 990.
978(37) 0.000730 988. 988.
1001(38) 0.000693 987. 987.
1002(38) 0.000693 985. 985.
996(38) 0.000693 984. 984.
998(38) 0.000693 982. 982.
901(34) 0.000865 980.8 980.8
994(37) 0.000730 979. 979.
1020(38) 0.000693 978. 978.
1025(38) 0.000693 977. 977.
959(36) 0.000772 975. 975.
880(34) 0.000865 973.7 973.7
915(35) 0.000816 972.3 972.3
930(35) 0.000816 970.9 970.9
954(36) 0.000772 970. 970.
891(34) 0.000865 968.1 968.1
903(34) 0.000865 966.7 966.7
983(37) 0.000730 965. 965.
938(36) 0.000772 964. 964.
932(35) 0.000816 962.5 962.5
959(36) 0.000772 961. 961.
912(35) 0.000816 959.8 959.8
923(35) 0.000816 958.4 958.4
898(34) 0.000865 957.0 957.0
876(33) 0.000918 955.7 955.7
915(35) 0.000816 954.3 954.3
926(35) 0.000816 952.9 952.9
875(34) 0.000865 951.6 951.6
925(35) 0.000816 950.2 950.2
953(36) 0.000772 949. 949.
926(48) 0.000434 948. 948.
918(47) 0.000453 946. 946.
851(44) 0.000517 945. 945.
876(46) 0.000473 943. 943.
870(45) 0.000494 942. 942.
900(47) 0.000453 941. 941.
864(45) 0.000494 939. 939.
822(43) 0.000541 938. 938.
869(45) 0.000494 937. 937.
837(44) 0.000517 936. 936.
930(48) 0.000434 934. 934.
888(46) 0.000473 933. 933.
960(37) 0.000730 932. 932.
1010(38) 0.000693 930. 930.
1027(39) 0.000657 929. 929.
928(36) 0.000772 928. 928.
918(35) 0.000816 926.4 926.4
962(37) 0.000730 925. 925.
931(36) 0.000772 924. 924.
925(36) 0.000772 923. 923.
954(37) 0.000730 921. 921.
937(36) 0.000772 920. 920.
960(37) 0.000730 919. 919.
934(36) 0.000772 917. 917.
987(37) 0.000730 916. 916.
880(34) 0.000865 914.9 914.9
900(35) 0.000816 913.7 913.7
955(37) 0.000730 912. 912.
959(37) 0.000730 911. 911.
983(37) 0.000730 910. 910.
942(36) 0.000772 909. 909.
925(36) 0.000772 907. 907.
932(36) 0.000772 906. 906.
932(36) 0.000772 905. 905.
968(37) 0.000730 904. 904.
946(36) 0.000772 903. 903.
902(35) 0.000816 901.3 901.3
908(35) 0.000816 900.1 900.1
926(36) 0.000772 899. 899.
871(34) 0.000865 897.6 897.6
932(36) 0.000772 896. 896.
897(35) 0.000816 895.2 895.2
941(36) 0.000772 894. 894.
936(36) 0.000772 893. 893.
920(35) 0.000816 891.6 891.6
927(36) 0.000772 890. 890.
882(34) 0.000865 889.2 889.2
868(35) 0.000816 888.0 888.0
857(35) 0.000816 886.8 886.8
961(38) 0.000693 886. 886.
982(39) 0.000657 884. 884.
904(36) 0.000772 883. 883.
927(37) 0.000730 882. 882.
896(36) 0.000772 881. 881.
907(36) 0.000772 880. 880.
955(38) 0.000693 879. 879.
934(37) 0.000730 877. 877.
917(37) 0.000730 876. 876.
909(36) 0.000772 875. 875.
874(35) 0.000816 874.0 874.0
885(36) 0.000772 873. 873.
847(34) 0.000865 871.7 871.7
933(37) 0.000730 871. 871.
960(38) 0.000693 869. 869.
881(35) 0.000816 868.3 868.3
862(35) 0.000816 867.2 867.2
897(36) 0.000772 866. 866.
943(38) 0.000693 865. 865.
931(37) 0.000730 864. 864.
895(36) 0.000772 863. 863.
891(36) 0.000772 862. 862.
919(37) 0.000730 860. 860.
878(35) 0.000816 859.3 859.3
821(34) 0.000865 858.2 858.2
866(35) 0.000816 857.1 857.1
910(36) 0.000772 856. 856.
873(35) 0.000816 854.9 854.9
869(35) 0.000816 853.8 853.8
897(36) 0.000772 853. 853.
822(33) 0.000918 851.6 851.6
813(33) 0.000918 850.5 850.5
828(34) 0.000865 849.5 849.5
905(36) 0.000772 848. 848.
864(35) 0.000816 847.3 847.3
892(36) 0.000772 846. 846.
857(35) 0.000816 845.1 845.1
830(34) 0.000865 844.1 844.1
812(33) 0.000918 843.0 843.0
781(32) 0.000977 841.9 841.9
819(33) 0.000918 840.9 840.9
868(35) 0.000816 839.8 842.6
796(33) 0.000918 838.8 841.8
824(34) 0.000865 837.7 841.1
859(35) 0.000816 836.7 840.4
882(36) 0.000772 836. 840.
839(34) 0.000865 834.6 839.2
835(34) 0.000865 833.6 838.8
888(36) 0.000772 833. 839.
879(36) 0.000772 831. 839.
844(34) 0.000865 830.5 839.1
821(49) 0.000416 829. 841.
895(36) 0.000772 828. 844.
900(36) 0.000772 827. 851.
876(35) 0.000816 826.4 862.0
876(35) 0.000816 825.3 879.2
962(38) 0.000693 824. 903.
978(38) 0.000693 823. 935.
977(38) 0.000693 822. 975.
1043(40) 0.000625 821. 1028.
1169(43) 0.000541 820. 1098.
1279(46) 0.000473 819. 1192.
1409(49) 0.000416 818. 1311.
1563(52) 0.000370 817. 1441.
1572(52) 0.000370 816. 1543.
1552(52) 0.000370 815. 1565.
1498(50) 0.000400 814. 1474.
1304(46) 0.000473 813. 1301.
1098(41) 0.000595 812. 1119.
1017(39) 0.000657 811. 980.
942(37) 0.000730 810. 896.
920(36) 0.000772 809. 853.
808(33) 0.000918 808.5 834.4
831(34) 0.000865 807.5 825.6
838(34) 0.000865 806.6 820.6
824(33) 0.000918 805.6 817.1
819(33) 0.000918 804.7 814.3
808(33) 0.000918 803.7 811.9
821(33) 0.000918 802.8 809.8
857(35) 0.000816 801.8 807.9
832(34) 0.000865 800.9 806.3
808(33) 0.000918 799.9 804.7
819(33) 0.000918 799.0 803.2
827(34) 0.000865 798.0 801.9
785(32) 0.000977 797.1 800.6
788(32) 0.000977 796.2 799.3
806(33) 0.000918 795.2 798.1
758(31) 0.001041 794.3 796.9
818(33) 0.000918 793.4 793.4
827(34) 0.000865 792.5 792.5
778(32) 0.000977 791.6 791.6
785(32) 0.000977 790.6 790.6
772(32) 0.000977 789.7 789.7
759(31) 0.001041 788.8 788.8
764(31) 0.001041 787.9 787.9
792(32) 0.000977 787.0 787.0
727(30) 0.001111 786.1 786.1
805(33) 0.000918 785.2 785.2
776(33) 0.000918 784.3 784.3
787(33) 0.000918 783.4 783.4
791(33) 0.000918 782.5 782.5
755(32) 0.000977 781.6 781.6
817(34) 0.000865 780.7 780.7
755(32) 0.000977 779.8 779.8
732(31) 0.001041 779.0 779.0
755(32) 0.000977 778.1 778.1
767(33) 0.000918 777.2 777.2
780(33) 0.000918 776.3 776.3
822(34) 0.000865 775.5 775.5
762(32) 0.000977 774.6 774.6
789(33) 0.000918 773.7 773.7
786(33) 0.000918 772.9 772.9
747(32) 0.000977 772.0 772.0
723(31) 0.001041 771.1 771.1
810(34) 0.000865 770.3 770.3
790(33) 0.000918 769.4 769.4
849(35) 0.000816 768.6 768.6
884(36) 0.000772 768. 768.
886(36) 0.000772 767. 767.
921(38) 0.000693 766. 766.
891(37) 0.000730 765. 765.
808(34) 0.000865 764.4 764.4
797(34) 0.000865 763.5 763.5
768(33) 0.000918 762.7 762.7
796(34) 0.000865 761.9 761.9
746(32) 0.000977 761.0 761.0
708(31) 0.001041 760.2 760.2
740(32) 0.000977 759.4 759.4
772(33) 0.000918 758.6 758.6
713(31) 0.001041 757.7 757.7
751(32) 0.000977 756.9 756.9
745(32) 0.000977 756.1 756.1
734(31) 0.001041 755.3 755.3
737(32) 0.000977 754.5 754.5
698(30) 0.001111 753.7 753.7
750(32) 0.000977 752.9 752.9
821(35) 0.000816 752.1 752.1
750(32) 0.000977 751.3 751.3
713(31) 0.001041 750.5 750.5
721(31) 0.001041 749.7 749.7
791(33) 0.000918 748.9 748.9
794(34) 0.000865 748.1 748.1
770(33) 0.000918 747.3 747.3
796(34) 0.000865 746.5 746.5
824(35) 0.000816 745.8 745.8
781(33) 0.000918 745.0 745.0
768(33) 0.000918 744.2 744.2
746(32) 0.000977 743.4 743.4
705(30) 0.001111 742.6 742.6
727(31) 0.001041 741.9 741.9
764(33) 0.000918 741.1 741.1
715(30) 0.001111 740.3 740.3
726(30) 0.001111 739.6 739.6
746(31) 0.001041 738.8 738.8
728(30) 0.001111 738.1 738.1
804(32) 0.000977 737.3 737.3
697(29) 0.001189 736.6 736.6
745(31) 0.001041 735.8 735.8
703(29) 0.001189 735.1 735.1
727(30) 0.001111 734.3 734.3
684(28) 0.001276 733.6 733.6
704(29) 0.001189 732.8 732.8
734(30) 0.001111 732.1 732.1
736(30) 0.001111 731.3 731.3
761(31) 0.001041 730.6 730.6
712(29) 0.001189 729.9 729.9
732(30) 0.001111 729.1 729.1
742(31) 0.001041 728.4 728.4
708(29) 0.001189 727.7 727.7
748(31) 0.001041 727.0 727.0
718(30) 0.001111 726.2 726.2
738(30) 0.001111 725.5 725.5
673(28) 0.001276 724.8 724.8
686(29) 0.001189 724.1 724.1
710(30) 0.001111 723.4 723.4
751(31) 0.001041 722.7 722.7
692(29) 0.001189 722.0 722.0
674(28) 0.001276 721.2 721.3
719(30) 0.001111 720.5 720.6
765(31) 0.001041 719.8 719.9
706(29) 0.001189 719.1 719.2
656(28) 0.001276 718.4 718.5
678(28) 0.001276 717.8 717.8
703(29) 0.001189 717.1 717.1
736(30) 0.001111 716.4 716.4
722(30) 0.001111 715.7 715.7
708(29) 0.001189 715.0 718.6
673(28) 0.001276 714.3 718.2
656(28) 0.001276 713.6 718.0
717(30) 0.001111 712.9 717.7
722(30) 0.001111 712.3 717.6
725(30) 0.001111 711.6 717.5
683(29) 0.001189 710.9 717.6
719(30) 0.001111 710.3 717.8
714(30) 0.001111 709.6 718.2
714(30) 0.001111 708.9 718.9
705(29) 0.001189 708.3 720.0
687(29) 0.001189 707.6 721.7
717(30) 0.001111 706.9 724.7
742(32) 0.000977 706.3 730.3
706(30) 0.001111 705.6 741.2
725(31) 0.001041 705.0 761.3
734(31) 0.001041 704.3 796.3
912(37) 0.000730 704. 853.
906(36) 0.000772 703. 940.
1060(41) 0.000595 702. 1065.
1330(47) 0.000453 702. 1234.
1510(51) 0.000384 701. 1435.
1670(54) 0.0003429 700. 1622.
1691(54) 0.0003429 700. 1721.
1571(52) 0.000370 699. 1664.
1301(46) 0.000473 699. 1461.
1166(43) 0.000541 698. 1206.
1025(40) 0.000625 697. 990.
868(35) 0.000816 696.6 848.6
807(34) 0.000865 696.0 773.5
729(31) 0.001041 695.4 739.0
751(32) 0.000977 694.8 723.7
758(32) 0.000977 694.2 716.0
743(32) 0.000977 693.5 711.1
676(29) 0.001189 692.9 707.6
719(31) 0.001041 692.3 704.7
719(31) 0.001041 691.7 702.4
625(27) 0.001372 691.1 700.4
697(30) 0.001111 690.5 698.7
702(30) 0.001111 689.9 697.2
660(29) 0.001189 689.3 695.9
656(29) 0.001189 688.7 694.8
705(30) 0.001111 688.1 693.7
754(32) 0.000977 687.5 692.9
743(31) 0.001041 686.9 692.3
780(33) 0.000918 686.3 692.2
701(30) 0.001111 685.7 689.2
703(30) 0.001111 685.1 690.9
666(29) 0.001189 684.5 693.9
754(32) 0.000977 684.0 698.3
763(32) 0.000977 683.4 704.3
744(31) 0.001041 682.8 711.0
768(32) 0.000977 682.2 716.6
752(32) 0.000977 681.6 718.6
744(32) 0.000977 681.1 715.2
758(32) 0.000977 680.5 707.1
705(30) 0.001111 679.9 697.5
703(30) 0.001111 679.3 689.5
768(32) 0.000977 678.8 684.1
729(31) 0.001041 678.2 681.0
695(30) 0.001111 677.7 679.2
690(30) 0.001111 677.1 678.2
689(30) 0.001111 676.5 677.4
681(30) 0.001111 676.0 676.7
689(30) 0.001111 675.4 676.0
650(29) 0.001189 674.9 675.4
673(30) 0.001111 674.3 674.8
690(30) 0.001111 673.8 674.2
675(30) 0.001111 673.2 673.6
675(30) 0.001111 672.7 673.0
623(28) 0.001276 672.1 672.5
656(29) 0.001189 671.6 672.0
676(30) 0.001111 671.0 671.5
662(29) 0.001189 670.5 671.1
636(29) 0.001189 670.0 670.7
676(30) 0.001111 669.4 670.6
678(30) 0.001111 668.9 670.7
633(28) 0.001276 668.4 671.2
678(30) 0.001111 667.8 672.0
647(29) 0.001189 667.3 672.9
640(29) 0.001189 666.8 673.5
657(29) 0.001189 666.3 673.2
659(29) 0.001189 665.7 671.8
675(30) 0.001111 665.2 669.6
611(28) 0.001276 664.7 667.4
650(29) 0.001189 664.2 665.7
668(30) 0.001111 663.7 664.4
656(29) 0.001189 663.1 663.6
666(29) 0.001189 662.6 662.9
668(30) 0.001111 662.1 662.3
655(29) 0.001189 661.6 661.8
636(29) 0.001189 661.1 661.2
663(29) 0.001189 660.6 660.7
652(29) 0.001189 660.1 660.2
687(30) 0.001111 659.6 659.7
698(30) 0.001111 659.1 659.2
720(31) 0.001041 658.6 658.7
762(32) 0.000977 658.1 658.2
741(32) 0.000977 657.6 657.7
772(33) 0.000918 657.1 657.2
750(32) 0.000977 656.6 656.7
730(31) 0.001041 656.2 656.2
742(32) 0.000977 655.7 655.7
700(31) 0.001041 655.2 655.2
643(29) 0.001189 654.7 654.7
614(28) 0.001276 654.2 654.2
640(29) 0.001189 653.7 653.7
628(28) 0.001276 653.3 653.3
652(29) 0.001189 652.8 652.8
635(29) 0.001189 652.3 652.3
676(30) 0.001111 651.8 661.3
674(30) 0.001111 651.4 667.7
648(30) 0.001111 650.9 668.8
638(30) 0.001111 650.4 670.1
629(29) 0.001189 650.0 671.7
622(29) 0.001189 649.5 673.6
650(30) 0.001111 649.0 675.9
692(31) 0.001041 648.6 678.8
673(31) 0.001041 648.1 682.3
651(30) 0.001111 647.7 686.6
682(31) 0.001041 647.2 692.1
704(32) 0.000977 646.7 699.0
686(31) 0.001041 646.3 708.0
667(31) 0.001041 645.8 720.8
715(32) 0.000977 645.4 740.6
767(34) 0.000865 644.9 775.4
773(34) 0.000865 644.5 841.4
873(37) 0.000730 644. 968.
1080(42) 0.000567 644. 1200.
1483(51) 0.000384 643. 1596.
2094(62) 0.0002601 643. 2212.
3047(76) 0.0001731 642. 3055.
4151(89) 0.0001262 642. 4023.
5160(100) 0.0001000 641. 4854.
5380(100) 0.0000961 641. 5190.
4869(97) 0.0001063 641. 4792.
3771(85) 0.0001384 640. 3818.
2637(70) 0.0002041 640. 2713.
1825(57) 0.0003078 639. 1824.
1321(47) 0.000453 639. 1259.
1032(41) 0.000595 638. 963.
824(35) 0.000816 638.0 826.5
821(35) 0.000816 637.6 765.3
763(34) 0.000865 637.2 734.3
697(31) 0.001041 636.7 715.3
689(31) 0.001041 636.3 701.7
654(30) 0.001111 635.9 691.2
665(30) 0.001111 635.5 682.9
667(31) 0.001041 635.1 676.2
689(31) 0.001041 634.7 670.6
651(30) 0.001111 634.3 666.0
678(31) 0.001041 633.9 662.0
710(32) 0.000977 633.5 658.7
683(31) 0.001041 633.1 655.7
616(29) 0.001189 632.7 653.2
621(29) 0.001189 632.3 650.9
635(29) 0.001189 631.9 647.9
684(31) 0.001041 631.5 631.5
642(30) 0.001111 631.1 631.1
612(29) 0.001189 630.7 630.7
624(29) 0.001189 630.3 630.3
663(30) 0.001111 629.9 629.9
629(29) 0.001189 629.5 629.5
651(30) 0.001111 629.1 629.1
643(30) 0.001111 628.7 628.7
647(29) 0.001189 628.3 628.3
664(30) 0.001111 627.9 628.0
642(29) 0.001189 627.6 627.6
600(28) 0.001276 627.2 627.2
619(28) 0.001276 626.8 626.8
609(28) 0.001276 626.4 626.4
601(28) 0.001276 626.1 626.1
597(27) 0.001372 625.7 625.7
628(28) 0.001276 625.3 625.3
660(30) 0.001111 624.9 625.0
622(28) 0.001276 624.6 624.6
630(29) 0.001189 624.2 624.3
600(27) 0.001372 623.8 624.0
591(27) 0.001372 623.5 623.7
617(28) 0.001276 623.1 623.5
633(29) 0.001189 622.7 623.4
639(29) 0.001189 622.4 623.4
643(29) 0.001189 622.0 623.4
617(28) 0.001276 621.6 623.8
615(28) 0.001276 621.3 623.5
603(28) 0.001276 620.9 622.9
614(28) 0.001276 620.6 622.2
617(28) 0.001276 620.2 621.5
657(29) 0.001189 619.9 620.9
650(29) 0.001189 619.5 620.5
604(28) 0.001276 619.2 620.2
597(27) 0.001372 618.8 619.9
601(28) 0.001276 618.5 619.7
566(26) 0.001479 618.1 619.5
558(26) 0.001479 617.8 619.4
588(27) 0.001372 617.4 619.3
627(28) 0.001276 617.1 619.4
619(28) 0.001276 616.8 619.8
605(28) 0.001276 616.4 620.7
611(28) 0.001276 616.1 622.9
605(28) 0.001276 615.8 627.4
616(28) 0.001276 615.4 635.9
672(30) 0.001111 615.1 650.2
726(31) 0.001041 614.8 670.9
763(32) 0.000977 614.4 696.4
737(32) 0.000977 614.1 719.7
768(33) 0.000918 613.8 732.2
732(32) 0.000977 613.4 726.8
672(30) 0.001111 613.1 704.9
698(31) 0.001041 612.8 676.4
668(30) 0.001111 612.5 651.2
601(28) 0.001276 612.2 633.8
609(28) 0.001276 611.8 623.9
618(29) 0.001189 611.5 619.0
621(29) 0.001189 611.2 616.7
617(29) 0.001189 610.9 615.6
613(29) 0.001189 610.6 615.1
606(29) 0.001189 610.3 614.8
607(29) 0.001189 609.9 614.9
605(29) 0.001189 609.6 615.5
624(29) 0.001189 609.3 617.2
616(29) 0.001189 609.0 621.1
602(29) 0.001189 608.7 629.0
677(31) 0.001041 608.4 643.6
707(32) 0.000977 608.1 666.8
736(33) 0.000918 607.8 698.2
774(34) 0.000865 607.5 732.1
794(34) 0.000865 607.2 757.3
794(34) 0.000865 606.9 761.6
775(34) 0.000865 606.6 739.4
763(33) 0.000918 606.3 702.7
659(30) 0.001111 606.0 666.4
660(30) 0.001111 605.7 639.4
630(29) 0.001189 605.4 623.2
611(29) 0.001189 605.1 615.0
570(28) 0.001276 604.8 611.1
557(27) 0.001372 604.6 609.2
585(28) 0.001276 604.3 608.0
564(27) 0.001372 604.0 607.3
582(28) 0.001276 603.7 606.7
625(29) 0.001189 603.4 606.2
600(28) 0.001276 603.1 605.9
568(27) 0.001372 602.8 605.8
576(28) 0.001276 602.6 606.0
581(28) 0.001276 602.3 607.0
567(27) 0.001372 602.0 609.2
596(28) 0.001276 601.7 613.7
567(27) 0.001372 601.5 621.3
576(28) 0.001276 601.2 632.0
627(29) 0.001189 600.9 644.2
632(30) 0.001111 600.6 653.7
627(29) 0.001189 600.4 657.1
566(27) 0.001372 600.1 651.3
587(28) 0.001276 599.8 638.8
563(27) 0.001372 599.6 625.1
572(28) 0.001276 599.3 614.1
572(27) 0.001372 599.0 607.0
590(28) 0.001276 598.8 603.1
573(28) 0.001276 598.5 601.2
605(29) 0.001189 598.2 600.2
603(29) 0.001189 598.0 599.6
601(29) 0.001189 597.7 599.1
584(28) 0.001276 597.5 598.7
552(27) 0.001372 597.2 598.5
625(29) 0.001189 597.0 598.3
631(23) 0.001890 596.7 598.3
595(26) 0.001479 596.4 598.6
630(27) 0.001372 596.2 599.6
624(27) 0.001372 595.9 601.6
623(27) 0.001372 595.7 605.0
603(26) 0.001479 595.4 609.7
649(27) 0.001372 595.2 614.7
676(28) 0.001276 594.9 618.3
675(28) 0.001276 594.7 618.5
661(28) 0.001276 594.5 614.8
614(26) 0.001479 594.2 609.1
567(25) 0.001600 594.0 603.4
562(25) 0.001600 593.7 599.0
545(24) 0.001736 593.5 596.3
546(25) 0.001600 593.3 594.8
588(26) 0.001479 593.0 593.9
582(26) 0.001479 592.8 593.4
594(26) 0.001479 592.5 593.0
601(26) 0.001479 592.3 592.7
636(27) 0.001372 592.1 592.4
638(27) 0.001372 591.8 592.1
670(28) 0.001276 591.6 591.9
676(28) 0.001276 591.4 591.6
653(28) 0.001276 591.1 591.3
634(27) 0.001372 590.9 591.1
611(26) 0.001479 590.7 590.8
591(26) 0.001479 590.5 590.6
576(25) 0.001600 590.2 590.4
557(25) 0.001600 590.0 590.1
561(25) 0.001600 589.8 589.9
559(25) 0.001600 589.6 589.6
582(26) 0.001479 589.4 589.4
583(26) 0.001479 589.1 589.1
569(25) 0.001600 588.9 588.9
580(26) 0.001479 588.7 588.7
613(26) 0.001479 588.5 588.5
584(26) 0.001479 588.3 588.3
567(25) 0.001600 588.0 588.0
607(26) 0.001479 587.8 587.8
575(25) 0.001600 587.6 587.6
607(26) 0.001479 587.4 587.4
582(26) 0.001479 587.2 587.2
572(25) 0.001600 587.0 587.0
594(26) 0.001479 586.8 586.8
573(25) 0.001600 586.6 586.6
602(26) 0.001479 586.4 586.4
566(25) 0.001600 586.2 586.2
571(26) 0.001479 586.0 586.0
563(26) 0.001479 585.7 585.7
603(27) 0.001372 585.5 585.5
594(27) 0.001372 585.3 585.3
580(26) 0.001479 585.1 585.1
578(26) 0.001479 584.9 584.9
560(26) 0.001479 584.7 584.7
581(26) 0.001479 584.5 584.5
549(25) 0.001600 584.3 584.3
552(25) 0.001600 584.1 584.1
593(27) 0.001372 584.0 584.0
586(26) 0.001479 583.8 583.8
553(25) 0.001600 583.6 583.6
593(27) 0.001372 583.4 583.4
568(26) 0.001479 583.2 583.2
584(26) 0.001479 583.0 583.0
564(26) 0.001479 582.8 582.8
542(25) 0.001600 582.6 582.6
564(26) 0.001479 582.4 582.4
551(25) 0.001600 582.2 582.2
566(26) 0.001479 582.1 582.1
580(26) 0.001479 581.9 581.9
541(25) 0.001600 581.7 581.7
576(26) 0.001479 581.5 581.5
543(25) 0.001600 581.3 581.3
557(26) 0.001479 581.1 581.1
579(26) 0.001479 581.0 581.0
559(26) 0.001479 580.8 580.8
551(25) 0.001600 580.6 580.6
593(27) 0.001372 580.4 580.4
601(27) 0.001372 580.2 580.2
566(26) 0.001479 580.1 580.1
582(26) 0.001479 579.9 579.9
591(27) 0.001372 579.7 579.7
564(26) 0.001479 579.5 579.5
560(26) 0.001479 579.4 579.4
575(26) 0.001479 579.2 579.2
584(26) 0.001479 579.0 579.0
559(26) 0.001479 578.9 578.9
595(27) 0.001372 578.7 578.7
572(26) 0.001479 578.5 578.5
571(26) 0.001479 578.4 578.4
583(26) 0.001479 578.2 578.2
596(27) 0.001372 578.0 578.0
536(25) 0.001600 577.9 577.9
534(25) 0.001600 577.7 577.7
559(26) 0.001479 577.5 577.6
544(25) 0.001600 577.4 577.4
585(26) 0.001479 577.2 577.2
589(27) 0.001372 577.0 577.1
576(26) 0.001479 576.9 576.9
598(27) 0.001372 576.7 576.8
547(25) 0.001600 576.6 576.7
582(24) 0.001736 576.4 576.6
586(25) 0.001600 576.3 582.2
575(24) 0.001736 576.1 594.6
599(25) 0.001600 575.9 607.7
568(24) 0.001736 575.8 618.5
561(24) 0.001736 575.6 623.0
576(24) 0.001736 575.5 627.9
593(25) 0.001600 575.3 633.3
625(26) 0.001479 575.2 639.1
551(24) 0.001736 575.0 645.8
562(24) 0.001736 574.9 653.7
584(24) 0.001736 574.7 663.5
614(25) 0.001600 574.6 675.8
637(26) 0.001479 574.4 691.2
643(26) 0.001479 574.3 710.9
646(26) 0.001479 574.1 737.1
680(27) 0.001372 574.0 774.7
735(28) 0.001276 573.9 835.9
821(30) 0.001111 573.7 949.0
1052(35) 0.000816 573.6 1172.3
1474(42) 0.000567 573. 1606.
2222(53) 0.000356 573. 2383.
3547(67) 0.0002228 573. 3618.
5523(85) 0.0001384 573. 5299.
7322(98) 0.0001041 573. 7177.
8730(110) 0.0000873 573. 8741.
9070(110) 0.0000826 573. 9399.
8230(100) 0.0000925 572. 8853.
6782(94) 0.0001132 572. 7325.
4997(80) 0.0001562 572. 5396.
3376(66) 0.0002296 572. 3645.
2261(53) 0.000356 572. 2363.
1582(44) 0.000517 572. 1571.
1153(37) 0.000730 572. 1142.
877(31) 0.001041 571.5 930.2
812(30) 0.001111 571.4 826.2
734(28) 0.001276 571.3 770.4
698(27) 0.001372 571.1 736.0
635(26) 0.001479 571.0 712.8
615(25) 0.001600 570.9 697.2
634(26) 0.001479 570.8 687.6
655(26) 0.001479 570.6 682.4
639(26) 0.001479 570.5 679.6
640(26) 0.001479 570.4 676.5
659(26) 0.001479 570.3 670.7
635(26) 0.001479 570.1 661.9
627(26) 0.001479 570.0 650.8
654(27) 0.001372 569.9 632.9
677(28) 0.001276 569.8 608.4
667(27) 0.001372 569.6 600.2
669(28) 0.001276 569.5 575.5
636(27) 0.001372 569.4 573.0
599(26) 0.001479 569.3 571.6
619(26) 0.001479 569.2 570.9
590(25) 0.001600 569.0 570.5
613(26) 0.001479 568.9 570.4
613(26) 0.001479 568.8 570.4
591(25) 0.001600 568.7 570.9
612(26) 0.001479 568.6 572.0
600(26) 0.001479 568.5 574.0
596(26) 0.001479 568.4 576.9
577(25) 0.001600 568.2 580.3
611(26) 0.001479 568.1 583.3
581(25) 0.001600 568.0 584.7
584(25) 0.001600 567.9 583.6
561(25) 0.001600 567.8 580.4
567(25) 0.001600 567.7 576.4
607(26) 0.001479 567.6 573.1
584(25) 0.001600 567.5 570.6
608(26) 0.001479 567.4 569.2
594(25) 0.001600 567.3 568.4
566(25) 0.001600 567.2 568.0
552(24) 0.001736 567.0 567.8
574(25) 0.001600 566.9 567.7
571(25) 0.001600 566.8 567.7
557(24) 0.001736 566.7 568.8
593(25) 0.001600 566.6 569.7
557(24) 0.001736 566.5 571.0
599(26) 0.001479 566.4 572.8
569(25) 0.001600 566.3 574.9
552(24) 0.001736 566.2 576.7
562(25) 0.001600 566.1 577.4
568(25) 0.001600 566.0 576.7
595(26) 0.001479 565.9 575.0
607(26) 0.001479 565.8 573.1
560(25) 0.001600 565.7 571.5
522(23) 0.001890 565.6 570.5
560(25) 0.001600 565.5 570.2
575(25) 0.001600 565.4 570.5
616(26) 0.001479 565.3 571.3
613(26) 0.001479 565.2 573.0
603(26) 0.001479 565.2 576.4
601(26) 0.001479 565.1 583.4
587(25) 0.001600 565.0 597.0
670(28) 0.001276 564.9 620.8
711(29) 0.001189 564.8 657.2
698(28) 0.001276 564.7 703.9
705(28) 0.001276 564.6 751.6
727(29) 0.001189 564.5 784.8
712(29) 0.001189 564.4 788.5
694(26) 0.001479 564.3 759.8
655(25) 0.001600 564.2 712.2
605(24) 0.001736 564.1 663.1
593(24) 0.001736 564.1 623.9
583(24) 0.001736 564.0 597.7
563(23) 0.001890 563.9 582.8
535(22) 0.002066 563.8 575.1
557(23) 0.001890 563.7 571.3
537(23) 0.001890 563.6 571.5
514(22) 0.002066 563.5 570.5
563(23) 0.001890 563.5 572.3
567(23) 0.001890 563.4 572.2
553(23) 0.001890 563.3 572.2
540(23) 0.001890 563.2 572.4
551(23) 0.001890 563.1 572.7
540(23) 0.001890 563.0 573.3
560(23) 0.001890 563.0 574.0
571(23) 0.001890 562.9 575.0
552(23) 0.001890 562.8 576.3
541(23) 0.001890 562.7 577.9
575(23) 0.001890 562.6 580.0
602(24) 0.001736 562.6 582.0
576(24) 0.001736 562.5 585.8
575(24) 0.001736 562.4 592.2
591(24) 0.001736 562.3 603.7
610(24) 0.001736 562.3 626.4
692(26) 0.001479 562.2 670.9
731(27) 0.001372 562.1 752.3
910(31) 0.001041 562.0 885.4
1107(34) 0.000865 562.0 1073.3
1278(37) 0.000730 562. 1294.
1472(40) 0.000625 562. 1494.
1547(41) 0.000595 562. 1602.
1522(41) 0.000595 562. 1566.
1287(37) 0.000730 562. 1401.
1103(34) 0.000865 561.5 1176.7
970(32) 0.000977 561.4 964.3
822(29) 0.001189 561.4 802.4
716(27) 0.001372 561.3 698.0
636(25) 0.001600 561.2 639.3
625(25) 0.001600 561.2 609.3
574(23) 0.001890 561.1 594.5
569(23) 0.001890 561.0 586.7
569(23) 0.001890 561.0 582.0
586(24) 0.001736 560.9 579.6
581(24) 0.001736 560.8 577.4
568(23) 0.001890 560.8 575.8
564(24) 0.001736 560.7 574.5
534(23) 0.001890 560.6 573.4
535(23) 0.001890 560.6 572.2
566(24) 0.001736 560.5 571.0
526(23) 0.001890 560.4 569.9
580(24) 0.001736 560.4 569.0
544(23) 0.001890 560.3 568.3
534(23) 0.001890 560.2 565.3
553(24) 0.001736 560.2 565.3
562(24) 0.001736 560.1 563.1
577(24) 0.001736 560.0 563.6
538(23) 0.001890 560.0 567.5
527(23) 0.001890 559.9 575.0
563(24) 0.001736 559.9 586.3
557(24) 0.001736 559.8 593.8
572(24) 0.001736 559.7 606.5
613(25) 0.001600 559.7 627.0
641(26) 0.001479 559.6 656.3
668(27) 0.001372 559.6 692.3
711(28) 0.001276 559.5 728.3
692(27) 0.001372 559.4 753.8
678(27) 0.001372 559.4 759.5
643(26) 0.001479 559.3 744.8
631(26) 0.001479 559.3 719.3
603(25) 0.001600 559.2 695.2
571(24) 0.001736 559.1 681.5
619(25) 0.001600 559.1 684.5
630(26) 0.001479 559.0 712.1
699(27) 0.001372 559.0 779.5
880(31) 0.001041 558.9 914.8
1190(37) 0.000730 559. 1158.
1630(44) 0.000517 559. 1546.
2376(53) 0.000356 559. 2092.
3043(61) 0.0002687 559. 2745.
3509(65) 0.0002367 559. 3379.
3875(69) 0.0002100 559. 3812.
3750(68) 0.0002163 559. 3895.
3385(64) 0.0002441 558. 3602.
2853(59) 0.0002873 558. 3040.
2172(51) 0.000384 558. 2379.
1641(44) 0.000517 558. 1775.
1323(39) 0.000657 558. 1313.
1012(34) 0.000865 558.2 1006.1
844(30) 0.001111 558.2 823.3
751(28) 0.001276 558.1 724.4
665(27) 0.001372 558.1 672.7
675(27) 0.001372 558.0 644.9
643(26) 0.001479 558.0 628.2
626(26) 0.001479 557.9 616.9
615(25) 0.001600 557.9 608.5
578(24) 0.001736 557.8 601.8
578(24) 0.001736 557.8 596.4
567(24) 0.001736 557.7 591.9
563(23) 0.001890 557.7 591.7
589(23) 0.001890 557.7 588.8
544(22) 0.002066 557.6 590.3
556(22) 0.002066 557.6 588.7
550(22) 0.002066 557.5 594.5
601(23) 0.001890 557.5 588.7
560(22) 0.002066 557.4 586.0
585(23) 0.001890 557.4 584.1
602(23) 0.001890 557.3 587.7
635(24) 0.001736 557.3 592.8
590(23) 0.001890 557.2 600.2
607(23) 0.001890 557.2 610.4
672(25) 0.001600 557.2 623.4
621(24) 0.001736 557.1 637.7
600(23) 0.001890 557.1 650.8
577(23) 0.001890 557.0 659.7
584(23) 0.001890 557.0 663.1
592(23) 0.001890 556.9 663.3
571(23) 0.001890 556.9 664.2
605(23) 0.001890 556.9 669.6
628(24) 0.001736 556.8 683.6
664(25) 0.001600 556.8 712.3
723(26) 0.001479 556.7 767.4
811(28) 0.001276 556.7 870.7
1006(31) 0.001041 556.6 1057.7
1441(38) 0.000693 557. 1376.
2003(45) 0.000494 557. 1874.
2909(54) 0.0003429 557. 2578.
3930(63) 0.0002520 556. 3451.
5022(72) 0.0001929 556. 4374.
5620(76) 0.0001731 556. 5149.
5781(77) 0.0001687 556. 5554.
5298(74) 0.0001826 556. 5415.
4544(68) 0.0002163 556. 4736.
3611(61) 0.0002687 556. 3758.
2754(53) 0.000356 556. 2770.
1983(44) 0.000517 556. 1961.
1390(37) 0.000730 556. 1393.
1056(32) 0.000977 556.1 1045.6
865(29) 0.001189 556.1 853.6
746(26) 0.001479 556.0 754.0
702(26) 0.001479 556.0 702.0
666(25) 0.001600 556.0 672.2
645(24) 0.001736 555.9 652.6
588(23) 0.001890 555.9 638.3
595(23) 0.001890 555.8 627.2
575(23) 0.001890 555.8 618.1
610(24) 0.001736 555.8 610.7
593(24) 0.001736 555.7 604.5
564(23) 0.001890 555.7 600.1
537(23) 0.001890 555.7 595.8
557(23) 0.001890 555.6 592.4
555(23) 0.001890 555.6 589.2
596(24) 0.001736 555.6 586.5
589(24) 0.001736 555.5 584.1
555(23) 0.001890 555.5 582.1
550(23) 0.001890 555.5 576.4
598(24) 0.001736 555.4 575.1
566(23) 0.001890 555.4 574.1
557(23) 0.001890 555.4 568.6
563(23) 0.001890 555.3 558.7
581(24) 0.001736 555.3 559.2
576(24) 0.001736 555.3 559.7
567(23) 0.001890 555.2 560.4
569(23) 0.001890 555.2 561.0
565(23) 0.001890 555.2 561.7
564(23) 0.001890 555.1 562.5
551(23) 0.001890 555.1 563.7
577(24) 0.001736 555.1 565.7
535(23) 0.001890 555.0 569.4
565(23) 0.001890 555.0 576.4
584(24) 0.001736 555.0 589.7
620(25) 0.001600 555.0 612.9
659(25) 0.001600 554.9 649.8
705(26) 0.001479 554.9 701.5
787(28) 0.001276 554.9 764.4
785(28) 0.001276 554.8 827.5
891(30) 0.001111 554.8 874.4
921(31) 0.001041 554.8 889.6
868(30) 0.001111 554.7 868.4
826(29) 0.001189 554.7 819.4
780(28) 0.001276 554.7 757.1
698(26) 0.001479 554.7 696.3
671(26) 0.001479 554.6 646.8
635(25) 0.001600 554.6 611.7
641(25) 0.001600 554.6 589.7
590(24) 0.001736 554.5 577.4
552(23) 0.001890 554.5 571.5
570(23) 0.001890 554.5 569.7
590(24) 0.001736 554.5 570.4
559(23) 0.001890 554.4 572.9
564(23) 0.001890 554.4 576.1
569(23) 0.001890 554.4 579.1
500(22) 0.002066 554.3 581.5
558(23) 0.001890 554.3 580.5
549(23) 0.001890 554.3 579.3
566(23) 0.001890 554.3 576.5
553(23) 0.001890 554.2 572.5
532(22) 0.002066 554.2 569.3
526(22) 0.002066 554.2 567.2
582(22) 0.002066 554.1 566.3
540(21) 0.002268 554.1 566.4
571(22) 0.002066 554.1 567.4
586(22) 0.002066 554.1 569.4
549(22) 0.002066 554.0 572.7
560(22) 0.002066 554.0 576.4
516(21) 0.002268 554.0 582.0
555(22) 0.002066 554.0 587.5
576(22) 0.002066 553.9 592.4
547(21) 0.002268 553.9 595.3
578(22) 0.002066 553.9 596.0
541(21) 0.002268 553.9 595.9
529(21) 0.002268 553.8 596.7
554(22) 0.002066 553.8 601.2
589(22) 0.002066 553.8 613.2
622(23) 0.001890 553.7 638.6
697(25) 0.001600 553.7 686.2
759(26) 0.001479 553.7 767.0
891(28) 0.001276 553.7 891.5
1132(32) 0.000977 553.6 1063.1
1324(35) 0.000816 553.6 1271.2
1565(38) 0.000693 554. 1485.
1660(40) 0.000625 554. 1659.
1719(40) 0.000625 554. 1745.
1688(40) 0.000625 554. 1716.
1558(38) 0.000693 553. 1577.
1300(35) 0.000816 553.5 1368.5
1173(33) 0.000918 553.4 1146.5
983(30) 0.001111 553.4 952.7
947(29) 0.001189 553.4 806.4
852(28) 0.001276 553.4 708.9
794(27) 0.001372 553.3 650.6
836(27) 0.001372 553.3 619.3
784(26) 0.001479 553.3 604.8
791(27) 0.001372 553.3 600.7
746(26) 0.001479 553.2 603.3
721(25) 0.001600 553.2 610.5
711(25) 0.001600 553.2 620.1
639(23) 0.001890 553.2 629.0
624(23) 0.001890 553.2 633.5
570(22) 0.002066 553.1 630.8
603(23) 0.001890 553.1 621.3
582(22) 0.002066 553.1 608.4
599(23) 0.001890 553.1 595.6
582(22) 0.002066 553.0 585.5
603(23) 0.001890 553.0 579.6
600(23) 0.001890 553.0 578.2
567(23) 0.001890 553.0 581.3
542(22) 0.002066 552.9 588.1
596(23) 0.001890 552.9 596.2
594(23) 0.001890 552.9 605.7
586(23) 0.001890 552.9 610.4
570(23) 0.001890 552.8 610.4
599(23) 0.001890 552.8 605.7
580(23) 0.001890 552.8 596.3
560(22) 0.002066 552.8 585.4
585(23) 0.001890 552.7 575.2
629(24) 0.001736 552.7 567.2
574(23) 0.001890 552.7 561.7
570(23) 0.001890 552.7 558.3
550(22) 0.002066 552.6 556.3
549(22) 0.002066 552.6 555.2
557(22) 0.002066 552.6 554.6
557(22) 0.002066 552.6 554.2
530(22) 0.002066 552.5 554.0
530(22) 0.002066 552.5 553.8
522(22) 0.002066 552.5 553.6
531(22) 0.002066 552.5 553.2
515(21) 0.002268 552.5 553.1
552(22) 0.002066 552.4 553.0
572(23) 0.001890 552.4 552.9
542(22) 0.002066 552.4 552.9
554(22) 0.002066 552.4 552.8
566(23) 0.001890 552.3 552.7
581(23) 0.001890 552.3 552.7
534(22) 0.002066 552.3 552.7
518(21) 0.002268 552.3 552.6
544(22) 0.002066 552.2 552.6
574(23) 0.001890 552.2 552.6
548(22) 0.002066 552.2 552.7
547(22) 0.002066 552.2 552.6
584(23) 0.001890 552.1 552.7
556(22) 0.002066 552.1 593.4
536(22) 0.002066 552.1 596.5
580(23) 0.001890 552.1 620.9
581(23) 0.001890 552.0 626.0
550(22) 0.002066 552.0 631.7
595(23) 0.001890 552.0 638.1
574(23) 0.001890 552.0 645.5
540(22) 0.002066 551.9 653.8
602(23) 0.001890 551.9 663.4
543(22) 0.002066 551.9 674.5
576(23) 0.001890 551.9 687.3
591(23) 0.001890 551.8 702.4
585(23) 0.001890 551.8 720.1
578(23) 0.001890 551.8 741.1
612(24) 0.001736 551.8 766.0
603(23) 0.001890 551.7 796.3
616(24) 0.001736 551.7 834.0
674(25) 0.001600 551.7 883.8
727(25) 0.001600 551.7 956.2
795(26) 0.001479 551.7 1073.8
1024(30) 0.001111 551.6 1280.8
1416(35) 0.000816 551.6 1655.4
2172(44) 0.000517 552. 2315.
3465(56) 0.0003189 552. 3401.
5634(71) 0.0001984 552. 5036.
8208(86) 0.0001352 551. 7249.
11210(100) 0.0000980 551. 9888.
13720(110) 0.0000797 551. 12562.
15590(120) 0.0000694 551. 14669.
15700(120) 0.0000694 551. 15589.
14540(120) 0.0000743 551. 15036.
12620(110) 0.0000857 551. 13215.
10200(97) 0.0001063 551. 10666.
7473(83) 0.0001452 551. 7996.
5461(70) 0.0002041 551. 5657.
3798(59) 0.0002873 551. 3862.
2618(48) 0.000434 551. 2630.
2006(42) 0.000567 551. 1861.
1455(36) 0.000772 551. 1418.
1171(32) 0.000977 551.1 1175.0
995(29) 0.001189 551.1 1042.6
886(27) 0.001372 551.1 964.5
859(27) 0.001372 551.1 910.7
785(26) 0.001479 551.0 866.3
749(25) 0.001600 551.0 827.1
706(24) 0.001736 551.0 790.5
677(24) 0.001736 551.0 758.5
601(22) 0.002066 550.9 731.9
619(22) 0.002066 550.9 711.2
631(23) 0.001890 550.9 696.3
635(23) 0.001890 550.8 686.8
628(23) 0.001890 550.8 682.3
612(22) 0.002066 550.8 681.8
606(22) 0.002066 550.8 683.9
660(23) 0.001890 550.7 686.4
650(23) 0.001890 550.7 686.7
626(23) 0.001890 550.7 638.6
627(23) 0.001890 550.6 632.4
634(23) 0.001890 550.6 601.0
597(22) 0.002066 550.6 592.4
604(22) 0.002066 550.6 585.2
626(23) 0.001890 550.5 581.0
615(22) 0.002066 550.5 581.3
602(22) 0.002066 550.5 587.8
622(23) 0.001890 550.4 603.1
720(25) 0.001600 550.4 630.8
709(25) 0.001600 550.4 674.4
772(26) 0.001479 550.4 736.0
890(28) 0.001276 550.3 813.4
976(30) 0.001111 550.3 898.4
1015(30) 0.001111 550.3 976.1
1016(30) 0.001111 550.2 1027.5
981(30) 0.001111 550.2 1037.2
1017(30) 0.001111 550.2 1000.8
905(29) 0.001189 550.2 929.6
843(28) 0.001276 550.1 843.6
748(26) 0.001479 550.1 760.6
708(25) 0.001600 550.1 691.6
644(24) 0.001736 550.0 640.6
637(24) 0.001736 550.0 606.6
623(23) 0.001890 550.0 585.8
591(23) 0.001890 549.9 573.9
578(22) 0.002066 549.9 567.0
563(22) 0.002066 549.9 563.1
560(22) 0.002066 549.8 560.8
523(21) 0.002268 549.8 559.1
536(21) 0.002268 549.8 558.0
523(21) 0.002268 549.8 557.0
520(21) 0.002268 549.7 556.1
505(21) 0.002268 549.7 555.5
534(21) 0.002268 549.7 554.9
554(22) 0.002066 549.6 554.4
535(21) 0.002268 549.6 554.0
554(22) 0.002066 549.6 553.6
544(22) 0.002066 549.5 553.3
563(22) 0.002066 549.5 553.0
545(22) 0.002066 549.5 552.8
518(21) 0.002268 549.4 552.6
557(22) 0.002066 549.4 551.9
539(21) 0.002268 549.4 551.4
561(22) 0.002066 549.3 550.1
517(21) 0.002268 549.3 550.2
525(21) 0.002268 549.3 550.4
528(21) 0.002268 549.2 550.6
572(22) 0.002066 549.2 551.2
520(21) 0.002268 549.2 552.1
541(21) 0.002268 549.1 553.7
547(22) 0.002066 549.1 556.3
611(23) 0.001890 549.1 560.3
607(23) 0.001890 549.0 565.7
596(23) 0.001890 549.0 572.2
612(23) 0.001890 548.9 579.1
581(22) 0.002066 548.9 585.1
609(23) 0.001890 548.9 588.5
591(23) 0.001890 548.8 588.4
590(23) 0.001890 548.8 584.7
618(23) 0.001890 548.8 578.6
603(23) 0.001890 548.7 571.7
598(31) 0.001041 548.7 565.3
532(20) 0.002500 548.7 560.0
547(21) 0.002268 548.6 556.2
567(21) 0.002268 548.6 553.8
560(21) 0.002268 548.5 553.4
542(20) 0.002500 548.5 552.8
525(20) 0.002500 548.5 554.6
550(21) 0.002268 548.4 554.8
557(21) 0.002268 548.4 555.9
550(21) 0.002268 548.4 557.8
544(20) 0.002500 548.3 558.1
556(21) 0.002268 548.3 558.4
550(21) 0.002268 548.2 558.7
523(20) 0.002500 548.2 559.1
525(20) 0.002500 548.2 559.8
547(20) 0.002500 548.1 561.0
549(21) 0.002268 548.1 562.7
549(21) 0.002268 548.0 565.2
565(21) 0.002268 548.0 568.7
570(21) 0.002268 548.0 573.1
532(20) 0.002500 547.9 578.6
558(21) 0.002268 547.9 584.7
573(21) 0.002268 547.8 591.1
560(21) 0.002268 547.8 597.6
575(21) 0.002268 547.8 604.8
589(21) 0.002268 547.7 614.7
585(21) 0.002268 547.7 631.6
652(23) 0.001890 547.6 661.4
761(24) 0.001736 547.6 711.4
830(26) 0.001479 547.6 788.9
921(27) 0.001372 547.5 898.7
1065(29) 0.001189 547.5 1040.2
1205(31) 0.001041 547.4 1204.3
1416(34) 0.000865 547.4 1371.9
1551(36) 0.000772 547. 1515.
1631(36) 0.000772 547. 1607.
1641(37) 0.000730 547. 1629.
1600(36) 0.000772 547. 1580.
1490(35) 0.000816 547.2 1469.2
1308(33) 0.000918 547.1 1318.0
1145(30) 0.001111 547.1 1153.0
1055(29) 0.001189 547.0 996.4
934(27) 0.001372 547.0 866.1
807(25) 0.001600 547.0 767.8
686(23) 0.001890 546.9 700.1
634(22) 0.002066 546.9 656.0
630(22) 0.002066 546.8 628.8
609(22) 0.002066 546.8 613.7
593(22) 0.002066 546.7 605.8
604(22) 0.002066 546.7 601.4
560(21) 0.002268 546.6 598.2
561(21) 0.002268 546.6 595.2
534(21) 0.002268 546.5 592.1
551(21) 0.002268 546.5 589.3
543(21) 0.002268 546.5 587.1
544(21) 0.002268 546.4 585.6
549(21) 0.002268 546.4 585.1
534(21) 0.002268 546.3 585.5
522(21) 0.002268 546.3 586.7
531(21) 0.002268 546.2 588.8
519(21) 0.002268 546.2 591.7
540(21) 0.002268 546.1 594.3
518(21) 0.002268 546.1 597.2
503(20) 0.002500 546.0 604.1
551(21) 0.002268 546.0 612.9
553(21) 0.002268 545.9 625.8
558(21) 0.002268 545.9 649.9
605(22) 0.002066 545.8 690.1
648(23) 0.001890 545.8 757.3
775(26) 0.001479 545.7 866.0
945(28) 0.001276 545.7 1032.9
1267(33) 0.000918 545.6 1272.3
1618(37) 0.000730 546. 1589.
2013(42) 0.000567 546. 1973.
2474(47) 0.000453 545. 2388.
2837(50) 0.000400 545. 2777.
3024(52) 0.000370 545. 3068.
3149(53) 0.000356 545. 3197.
3102(52) 0.000370 545. 3133.
2879(50) 0.000400 545. 2891.
2530(47) 0.000453 545. 2528.
2176(44) 0.000517 545. 2114.
1745(39) 0.000657 545. 1715.
1414(35) 0.000816 545.0 1373.2
1192(32) 0.000977 544.9 1109.1
974(29) 0.001189 544.9 918.8
801(26) 0.001479 544.8 791.9
745(25) 0.001600 544.8 712.1
674(24) 0.001736 544.7 664.0
622(23) 0.001890 544.7 635.3
616(23) 0.001890 544.6 617.9
586(22) 0.002066 544.6 606.8
611(23) 0.001890 544.5 599.0
569(22) 0.002066 544.5 593.4
562(22) 0.002066 544.4 589.1
570(22) 0.002066 544.3 585.9
555(21) 0.002268 544.3 583.7
580(22) 0.002066 544.2 582.5
562(22) 0.002066 544.2 582.3
574(22) 0.002066 544.1 583.1
564(21) 0.002268 544.1 584.9
550(21) 0.002268 544.0 587.5
562(21) 0.002268 543.9 590.4
532(20) 0.002500 543.9 593.2
541(21) 0.002268 543.8 595.9
569(21) 0.002268 543.8 598.5
585(22) 0.002066 543.7 602.4
570(21) 0.002268 543.6 608.8
562(21) 0.002268 543.6 622.9
638(23) 0.001890 543.5 645.9
664(23) 0.001890 543.5 681.6
698(24) 0.001736 543.4 734.2
800(25) 0.001600 543.3 805.4
895(27) 0.001372 543.3 892.2
994(28) 0.001276 543.2 984.2
1083(30) 0.001111 543.2 1068.7
1105(30) 0.001111 543.1 1130.3
1124(30) 0.001111 543.0 1154.9
1122(30) 0.001111 543.0 1134.3
1066(29) 0.001189 542.9 1073.0
978(28) 0.001276 542.9 985.8
900(27) 0.001372 542.8 890.2
826(26) 0.001479 542.7 800.4
755(25) 0.001600 542.7 724.9
673(23) 0.001890 542.6 667.4
655(23) 0.001890 542.5 626.7
558(21) 0.002268 542.5 600.1
549(21) 0.002268 542.4 583.4
571(21) 0.002268 542.4 573.1
600(22) 0.002066 542.3 566.6
556(21) 0.002268 542.2 562.1
535(21) 0.002268 542.2 558.9
540(21) 0.002268 542.1 556.5
521(20) 0.002500 542.0 554.6
539(21) 0.002268 542.0 553.3
527(20) 0.002500 541.9 552.4
557(21) 0.002268 541.8 552.1
561(21) 0.002268 541.8 552.4
543(21) 0.002268 541.7 553.2
533(20) 0.002500 541.6 554.9
538(21) 0.002268 541.6 557.2
553(21) 0.002268 541.5 560.0
558(21) 0.002268 541.4 562.9
556(21) 0.002268 541.4 565.3
523(20) 0.002500 541.3 566.7
550(21) 0.002268 541.2 566.7
543(21) 0.002268 541.2 565.4
556(21) 0.002268 541.1 563.8
559(22) 0.002066 541.0 561.3
556(22) 0.002066 540.9 559.9
546(21) 0.002268 540.9 559.6
542(21) 0.002268 540.8 559.2
521(21) 0.002268 540.7 562.6
531(21) 0.002268 540.7 567.5
568(22) 0.002066 540.6 573.3
536(21) 0.002268 540.5 579.2
540(21) 0.002268 540.5 583.8
535(21) 0.002268 540.4 585.9
562(22) 0.002066 540.3 584.9
558(22) 0.002066 540.2 581.2
534(21) 0.002268 540.2 575.8
537(21) 0.002268 540.1 570.2
551(22) 0.002066 540.0 565.2
540(21) 0.002268 540.0 561.7
555(22) 0.002066 539.9 559.8
555(22) 0.002066 539.8 559.5
551(22) 0.002066 539.7 560.4
568(22) 0.002066 539.7 562.0
560(22) 0.002066 539.6 563.7
531(21) 0.002268 539.5 565.4
533(21) 0.002268 539.4 567.1
574(22) 0.002066 539.4 569.7
543(21) 0.002268 539.3 574.9
557(22) 0.002066 539.2 584.3
609(23) 0.001890 539.1 600.1
626(23) 0.001890 539.1 623.7
670(24) 0.001736 539.0 656.0
708(25) 0.001600 538.9 696.1
733(25) 0.001600 538.8 740.8
811(26) 0.001479 538.7 784.9
872(27) 0.001372 538.7 820.9
874(28) 0.001276 538.6 841.1
854(27) 0.001372 538.5 840.2
844(27) 0.001372 538.4 818.7
769(26) 0.001479 538.4 782.3
752(25) 0.001600 538.3 738.0
696(24) 0.001736 538.2 693.0
693(24) 0.001736 538.1 652.3
631(23) 0.001890 538.0 618.8
612(23) 0.001890 538.0 593.4
621(23) 0.001890 537.9 575.3
560(22) 0.002066 537.8 563.1
595(22) 0.002066 537.7 555.4
578(22) 0.002066 537.6 550.7
573(22) 0.002066 537.6 547.9
535(21) 0.002268 537.5 546.2
532(21) 0.002268 537.4 545.2
510(21) 0.002268 537.3 552.0
543(21) 0.002268 537.2 552.5
527(21) 0.002268 537.2 556.1
534(17) 0.003460 537.1 565.4
555(21) 0.002268 537.0 573.5
535(21) 0.002268 536.9 590.5
555(21) 0.002268 536.8 595.3
511(20) 0.002500 536.7 600.1
570(21) 0.002268 536.7 604.5
525(21) 0.002268 536.6 608.2
546(21) 0.002268 536.5 611.1
558(21) 0.002268 536.4 613.4
562(21) 0.002268 536.3 615.6
560(21) 0.002268 536.2 618.1
550(21) 0.002268 536.1 621.5
532(21) 0.002268 536.1 626.5
559(21) 0.002268 536.0 632.5
562(21) 0.002268 535.9 639.1
542(21) 0.002268 535.8 649.1
550(21) 0.002268 535.7 661.0
561(21) 0.002268 535.6 676.0
596(22) 0.002066 535.5 695.2
633(23) 0.001890 535.5 720.8
649(23) 0.001890 535.4 756.8
665(23) 0.001890 535.3 809.9
712(24) 0.001736 535.2 891.0
833(26) 0.001479 535.1 1016.4
1056(29) 0.001189 535.0 1207.9
1332(33) 0.000918 534.9 1492.3
1726(38) 0.000693 535. 1898.
2353(44) 0.000517 535. 2450.
3248(52) 0.000370 535. 3162.
4235(59) 0.0002873 535. 4025.
5165(66) 0.0002296 534. 5000.
6241(72) 0.0001929 534. 6012.
7261(78) 0.0001644 534. 6958.
7948(81) 0.0001524 534. 7726.
8309(83) 0.0001452 534. 8212.
8318(83) 0.0001452 534. 8332.
8044(82) 0.0001487 534. 8044.
7396(79) 0.0001602 534. 7385.
6417(73) 0.0001877 534. 6462.
5514(68) 0.0002163 534. 5415.
4390(60) 0.0002778 534. 4377.
3560(54) 0.0003429 533. 3444.
2800(48) 0.000434 533. 2670.
2220(43) 0.000541 533. 2073.
1764(38) 0.000693 533. 1640.
1417(34) 0.000865 533.1 1341.3
1185(31) 0.001041 533.0 1143.0
1022(30) 0.001111 532.9 1012.6
954(29) 0.001189 532.8 924.9
857(27) 0.001372 532.7 862.6
807(26) 0.001479 532.6 814.8
727(25) 0.001600 532.5 775.4
677(24) 0.001736 532.4 741.7
653(24) 0.001736 532.3 713.2
630(23) 0.001890 532.2 688.9
635(23) 0.001890 532.1 668.6
606(23) 0.001890 532.0 652.1
585(22) 0.002066 531.9 638.9
607(23) 0.001890 531.8 628.3
581(22) 0.002066 531.8 619.6
612(23) 0.001890 531.7 612.1
582(22) 0.002066 531.6 605.7
565(22) 0.002066 531.5 600.0
553(22) 0.002066 531.4 595.0
550(22) 0.002066 531.3 582.7
555(22) 0.002066 531.2 579.8
523(21) 0.002268 531.1 575.1
528(21) 0.002268 531.0 565.0
559(22) 0.002066 530.9 559.6
548(22) 0.002066 530.8 545.8
561(22) 0.002066 530.7 548.4
550(22) 0.002066 530.6 550.4
581(22) 0.002066 530.5 552.3
538(21) 0.002268 530.4 553.6
556(22) 0.002066 530.3 554.7
592(23) 0.001890 530.2 555.2
591(23) 0.001890 530.1 556.2
560(22) 0.002066 530.0 557.6
565(22) 0.002066 529.9 560.8
591(23) 0.001890 529.8 565.9
578(22) 0.002066 529.7 574.6
612(23) 0.001890 529.5 587.1
661(24) 0.001736 529.4 603.0
670(24) 0.001736 529.3 622.1
669(24) 0.001736 529.2 642.7
699(25) 0.001600 529.1 662.2
710(25) 0.001600 529.0 677.7
699(25) 0.001600 528.9 686.3
705(25) 0.001600 528.8 686.4
702(25) 0.001600 528.7 678.0
678(24) 0.001736 528.6 663.0
616(23) 0.001890 528.5 643.9
652(24) 0.001736 528.4 623.7
623(23) 0.001890 528.3 604.5
595(23) 0.001890 528.2 588.1
561(22) 0.002066 528.1 575.2
590(23) 0.001890 528.0 566.1
567(22) 0.002066 527.9 561.0
562(22) 0.002066 527.8 559.7
560(22) 0.002066 527.7 562.5
532(29) 0.001189 527.6 570.1
567(21) 0.002268 527.4 583.6
604(21) 0.002268 527.3 604.5
627(22) 0.002066 527.2 634.3
661(22) 0.002066 527.1 674.0
744(24) 0.001736 527.0 723.5
810(25) 0.001600 526.9 781.3
851(26) 0.001479 526.8 844.0
878(26) 0.001479 526.7 905.5
928(27) 0.001372 526.6 958.2
999(28) 0.001276 526.5 996.0
991(28) 0.001276 526.4 1010.3
996(28) 0.001276 526.3 1001.5
972(27) 0.001372 526.1 970.6
955(27) 0.001372 526.0 923.6
934(27) 0.001372 525.9 866.9
864(26) 0.001479 525.8 806.8
775(24) 0.001736 525.7 749.2
728(24) 0.001736 525.6 698.0
653(22) 0.002066 525.5 655.6
650(22) 0.002066 525.4 621.8
641(22) 0.002066 525.3 597.0
621(22) 0.002066 525.1 579.7
567(21) 0.002268 525.0 568.1
545(20) 0.002500 524.9 560.5
551(20) 0.002500 524.8 555.7
549(20) 0.002500 524.7 552.5
527(20) 0.002500 524.6 550.4
566(21) 0.002268 524.5 548.9
517(20) 0.002500 524.4 547.7
548(20) 0.002500 524.2 546.8
533(20) 0.002500 524.1 546.2
523(20) 0.002500 524.0 545.9
545(20) 0.002500 523.9 546.2
573(21) 0.002268 523.8 547.2
541(20) 0.002500 523.7 549.2
554(21) 0.002268 523.6 552.7
526(20) 0.002500 523.4 558.6
529(20) 0.002500 523.3 567.9
537(20) 0.002500 523.2 582.4
597(21) 0.002268 523.1 604.1
627(22) 0.002066 523.0 635.4
700(23) 0.001890 522.9 678.6
761(24) 0.001736 522.8 734.2
829(25) 0.001600 522.6 804.4
911(26) 0.001479 522.5 886.4
996(28) 0.001276 522.4 975.9
1020(29) 0.001189 522.3 1065.8
1089(30) 0.001111 522.2 1146.6
1116(30) 0.001111 522.1 1208.1
1189(31) 0.001041 521.9 1241.2
1166(31) 0.001041 521.8 1240.9
1111(30) 0.001111 521.7 1208.3
1121(30) 0.001111 521.6 1148.0
949(28) 0.001276 521.5 1069.4
885(27) 0.001372 521.3 981.2
855(26) 0.001479 521.2 892.7
831(26) 0.001479 521.1 811.1
725(24) 0.001736 521.0 741.0
666(23) 0.001890 520.9 684.1
633(23) 0.001890 520.7 640.6
588(22) 0.002066 520.6 608.8
584(22) 0.002066 520.5 586.7
575(22) 0.002066 520.4 571.6
532(21) 0.002268 520.3 561.5
562(21) 0.002268 520.2 554.5
518(20) 0.002500 520.0 549.3
511(20) 0.002500 519.9 545.2
505(20) 0.002500 519.8 541.7
539(21) 0.002268 519.7 538.7
510(20) 0.002500 519.5 536.1
489(20) 0.002500 519.4 533.8
530(21) 0.002268 519.3 531.9
508(20) 0.002500 519.2 530.3
508(20) 0.002500 519.1 529.0
492(20) 0.002500 518.9 527.9
518(20) 0.002500 518.8 527.1
484(20) 0.002500 518.7 526.3
512(20) 0.002500 518.6 525.6
475(20) 0.002500 518.5 525.0
542(21) 0.002268 518.3 524.4
525(21) 0.002268 518.2 523.8
510(20) 0.002500 518.1 523.5
507(20) 0.002500 518.0 523.0
534(21) 0.002268 517.8 522.5
529(21) 0.002268 517.7 522.1
501(20) 0.002500 517.6 521.7
506(20) 0.002500 517.5 521.6
473(19) 0.002770 517.3 521.4
530(21) 0.002268 517.2 519.6
516(20) 0.002500 517.1 519.4
494(20) 0.002500 517.0 518.4
495(20) 0.002500 516.8 518.3
521(20) 0.002500 516.7 518.3
490(20) 0.002500 516.6 518.8
516(20) 0.002500 516.5 518.8
525(21) 0.002268 516.3 519.2
531(21) 0.002268 516.2 519.8
546(21) 0.002268 516.1 520.0
539(21) 0.002268 516.0 520.1
555(20) 0.002500 515.8 520.3
561(20) 0.002500 515.7 520.6
606(21) 0.002268 515.6 520.8
541(20) 0.002500 515.5 521.0
602(21) 0.002268 515.3 521.4
561(20) 0.002500 515.2 521.8
597(21) 0.002268 515.1 522.4
580(21) 0.002268 515.0 523.2
555(20) 0.002500 514.8 524.3
559(20) 0.002500 514.7 525.5
596(21) 0.002268 514.6 527.2
605(21) 0.002268 514.5 529.5
537(20) 0.002500 514.3 532.7
568(21) 0.002268 514.2 537.2
598(21) 0.002268 514.1 543.4
553(20) 0.002500 513.9 551.8
568(21) 0.002268 513.8 562.9
549(20) 0.002500 513.7 577.1
599(21) 0.002268 513.6 594.7
572(21) 0.002268 513.4 615.6
634(22) 0.002066 513.3 639.5
622(22) 0.002066 513.2 665.6
636(22) 0.002066 513.0 692.3
713(23) 0.001890 512.9 719.0
740(24) 0.001736 512.8 743.2
773(24) 0.001736 512.7 764.8
762(24) 0.001736 512.5 782.9
780(24) 0.001736 512.4 797.8
759(24) 0.001736 512.3 810.9
835(25) 0.001600 512.1 824.1
823(25) 0.001600 512.0 839.7
856(26) 0.001479 511.9 859.4
893(26) 0.001479 511.8 883.3
887(26) 0.001479 511.6 909.7
899(26) 0.001479 511.5 935.0
970(27) 0.001372 511.4 954.5
965(27) 0.001372 511.2 963.6
914(26) 0.001479 511.1 959.1
872(26) 0.001479 511.0 940.6
927(27) 0.001372 510.9 910.4
826(25) 0.001600 510.7 872.5
800(25) 0.001600 510.6 831.4
769(24) 0.001736 510.5 791.1
742(24) 0.001736 510.3 754.6
686(23) 0.001890 510.2 723.7
689(23) 0.001890 510.1 698.8
672(23) 0.001890 509.9 679.5
689(23) 0.001890 509.8 664.0
643(23) 0.001890 509.7 650.7
624(22) 0.002066 509.5 638.6
609(22) 0.002066 509.4 628.0
652(23) 0.001890 509.3 618.3
624(22) 0.002066 509.2 611.1
593(22) 0.002066 509.0 607.5
586(22) 0.002066 508.9 608.7
572(21) 0.002268 508.8 615.4
619(22) 0.002066 508.6 628.0
698(24) 0.001736 508.5 646.3
668(23) 0.001890 508.4 669.3
707(24) 0.001736 508.2 695.2
653(23) 0.001890 508.1 721.5
740(24) 0.001736 508.0 745.0
797(25) 0.001600 507.8 763.2
742(25) 0.001600 507.7 773.0
795(25) 0.001600 507.6 773.0
779(25) 0.001600 507.4 762.7
761(25) 0.001600 507.3 743.6
698(24) 0.001736 507.2 718.2
775(25) 0.001600 507.0 689.9
682(23) 0.001890 506.9 661.1
638(23) 0.001890 506.8 634.1
653(23) 0.001890 506.6 610.5
595(22) 0.002066 506.5 591.1
626(22) 0.002066 506.4 575.7
612(22) 0.002066 506.3 565.6
598(22) 0.002066 506.1 559.4
584(22) 0.002066 506.0 557.3
579(22) 0.002066 505.9 560.1
596(22) 0.002066 505.7 567.3
589(22) 0.002066 505.6 579.8
647(23) 0.001890 505.5 597.9
660(23) 0.001890 505.3 622.3
687(24) 0.001736 505.2 652.8
749(25) 0.001600 505.1 688.8
778(25) 0.001600 504.9 728.5
764(25) 0.001600 504.8 769.4
837(26) 0.001479 504.7 807.9
776(25) 0.001600 504.5 840.0
895(27) 0.001372 504.4 865.2
824(26) 0.001479 504.3 873.2
824(26) 0.001479 504.1 866.1
743(25) 0.001600 504.0 845.1
854(26) 0.001479 503.9 813.1
809(26) 0.001479 503.7 774.1
682(23) 0.001890 503.6 732.1
661(23) 0.001890 503.5 707.4
631(23) 0.001890 503.3 670.1
640(23) 0.001890 503.2 637.9
605(22) 0.002066 503.1 624.0
575(21) 0.002268 502.9 604.1
566(21) 0.002268 502.8 589.4
543(21) 0.002268 502.7 579.4
516(21) 0.002268 502.5 572.4
540(21) 0.002268 502.4 569.0
511(20) 0.002500 502.3 567.4
534(21) 0.002268 502.1 567.7
547(21) 0.002268 502.0 569.1
570(22) 0.002066 501.9 571.5
523(21) 0.002268 501.7 574.9
541(21) 0.002268 501.6 578.7
540(21) 0.002268 501.5 583.2
506(20) 0.002500 501.3 588.3
516(21) 0.002268 501.2 594.0
533(21) 0.002268 501.1 600.3
527(21) 0.002268 500.9 607.3
519(21) 0.002268 500.8 615.0
543(21) 0.002268 500.7 623.6
545(21) 0.002268 500.5 633.3
598(22) 0.002066 500.4 644.6
549(21) 0.002268 500.3 658.4
566(22) 0.002066 500.1 675.8
567(22) 0.002066 500.0 698.9
609(22) 0.002066 499.9 730.6
628(23) 0.001890 499.7 775.4
706(24) 0.001736 499.6 839.5
783(26) 0.001479 499.5 931.1
865(27) 0.001372 499.3 1061.8
1016(29) 0.001189 499.2 1244.6
1333(33) 0.000918 499.1 1494.0
1635(37) 0.000730 499. 1823.
2146(43) 0.000541 499. 2247.
2760(48) 0.000434 499. 2770.
3449(54) 0.0003429 499. 3394.
4141(59) 0.0002873 498. 4106.
5011(65) 0.0002367 498. 4882.
5774(70) 0.0002041 498. 5684.
6618(75) 0.0001778 498. 6459.
7146(78) 0.0001644 498. 7148.
7707(81) 0.0001524 498. 7692.
8133(83) 0.0001452 498. 8044.
7986(82) 0.0001487 497. 8177.
8259(84) 0.0001417 497. 8079.
7857(82) 0.0001487 497. 7757.
7417(79) 0.0001602 497. 7238.
6648(75) 0.0001778 497. 6566.
5982(71) 0.0001984 497. 5801.
5167(66) 0.0002296 497. 5002.
4405(63) 0.0002520 497. 4224.
3648(57) 0.0003078 496. 3507.
3087(53) 0.000356 496. 2876.
2414(47) 0.000453 496. 2346.
2023(43) 0.000541 496. 1916.
1742(40) 0.000625 496. 1580.
1466(36) 0.000772 496. 1325.
1217(33) 0.000918 495.6 1136.9
1071(31) 0.001041 495.5 1000.9
975(30) 0.001111 495.4 903.5
892(28) 0.001276 495.3 833.7
835(27) 0.001372 495.1 783.0
768(26) 0.001479 495.0 745.6
734(26) 0.001479 494.9 717.3
693(25) 0.001600 494.7 695.2
633(24) 0.001736 494.6 677.7
622(23) 0.001890 494.5 663.6
640(24) 0.001736 494.3 652.1
610(23) 0.001890 494.2 643.6
603(23) 0.001890 494.1 636.3
587(23) 0.001890 494.0 631.2
603(23) 0.001890 493.8 628.5
614(23) 0.001890 493.7 628.5
630(24) 0.001736 493.6 631.7
632(24) 0.001736 493.4 639.6
657(24) 0.001736 493.3 649.2
708(25) 0.001600 493.2 661.5
651(24) 0.001736 493.1 675.8
696(25) 0.001600 492.9 690.9
698(25) 0.001600 492.8 705.3
655(24) 0.001736 492.7 717.4
712(25) 0.001600 492.5 725.6
690(25) 0.001600 492.4 728.6
669(24) 0.001736 492.3 721.6
712(25) 0.001600 492.2 714.7
699(25) 0.001600 492.0 704.6
673(24) 0.001736 491.9 693.3
709(25) 0.001600 491.8 682.5
710(25) 0.001600 491.6 673.5
697(25) 0.001600 491.5 667.3
673(24) 0.001736 491.4 637.6
666(24) 0.001736 491.3 638.1
711(25) 0.001600 491.1 640.3
665(24) 0.001736 491.0 643.0
677(24) 0.001736 490.9 644.7
672(24) 0.001736 490.8 644.1
657(24) 0.001736 490.6 640.3
672(24) 0.001736 490.5 633.3
698(25) 0.001600 490.4 623.5
659(24) 0.001736 490.3 612.1
646(24) 0.001736 490.1 600.6
645(24) 0.001736 490.0 589.7
620(23) 0.001890 489.9 581.0
626(23) 0.001890 489.8 575.5
624(23) 0.001890 489.6 574.7
624(23) 0.001890 489.5 580.2
621(23) 0.001890 489.4 591.6
678(24) 0.001736 489.3 612.3
669(24) 0.001736 489.1 639.1
726(25) 0.001600 489.0 675.0
800(26) 0.001479 488.9 719.1
802(26) 0.001479 488.8 773.0
883(28) 0.001276 488.6 829.6
895(28) 0.001276 488.5 891.0
955(29) 0.001189 488.4 949.8
958(29) 0.001189 488.3 1004.1
1034(30) 0.001111 488.2 1049.5
1071(30) 0.001111 488.0 1082.1
1092(31) 0.001041 487.9 1099.0
1057(30) 0.001111 487.8 1098.4
1077(30) 0.001111 487.7 1080.0
1088(31) 0.001041 487.6 1045.8
993(29) 0.001189 487.4 999.1
947(29) 0.001189 487.3 944.5
927(28) 0.001276 487.2 886.7
925(28) 0.001276 487.1 829.6
816(27) 0.001372 486.9 776.5
770(26) 0.001479 486.8 729.5
768(26) 0.001479 486.7 689.0
668(24) 0.001736 486.6 656.8
700(25) 0.001600 486.5 631.9
642(24) 0.001736 486.4 613.6
585(22) 0.002066 486.2 601.1
608(23) 0.001890 486.1 593.6
587(23) 0.001890 486.0 590.3
579(22) 0.002066 485.9 591.0
612(23) 0.001890 485.8 595.6
597(23) 0.001890 485.6 604.4
609(23) 0.001890 485.5 618.2
610(23) 0.001890 485.4 637.7
621(23) 0.001890 485.3 663.8
671(24) 0.001736 485.2 699.0
655(24) 0.001736 485.1 744.9
764(26) 0.001479 484.9 804.4
834(27) 0.001372 484.8 878.3
929(28) 0.001276 484.7 970.1
1018(30) 0.001111 484.6 1081.6
1213(32) 0.000977 484.5 1213.7
1338(34) 0.000865 484.4 1367.3
1508(36) 0.000772 484. 1541.
1725(39) 0.000657 484. 1735.
1977(43) 0.000541 484. 1939.
2182(45) 0.000494 484. 2146.
2350(46) 0.000473 484. 2344.
2493(48) 0.000434 484. 2521.
2644(49) 0.000416 484. 2664.
2649(49) 0.000416 483. 2762.
2805(51) 0.000384 483. 2808.
2744(50) 0.000400 483. 2797.
2765(50) 0.000400 483. 2729.
2589(49) 0.000416 483. 2607.
2471(48) 0.000434 483. 2443.
2323(46) 0.000473 483. 2247.
2120(44) 0.000517 483. 2033.
1830(41) 0.000595 483. 1814.
1634(39) 0.000657 482. 1603.
1487(37) 0.000730 482. 1405.
1248(34) 0.000865 482.2 1229.9
1171(33) 0.000918 482.1 1079.4
1039(31) 0.001041 482.0 954.1
941(29) 0.001189 481.9 853.0
815(27) 0.001372 481.8 773.9
784(27) 0.001372 481.7 714.0
758(26) 0.001479 481.6 670.1
698(25) 0.001600 481.5 639.3
685(25) 0.001600 481.4 618.9
627(24) 0.001736 481.3 607.3
667(25) 0.001600 481.2 602.8
637(24) 0.001736 481.1 604.9
640(24) 0.001736 481.0 613.4
643(24) 0.001736 480.9 628.6
643(24) 0.001736 480.8 651.1
703(25) 0.001600 480.7 682.0
797(27) 0.001372 480.5 722.2
809(27) 0.001372 480.4 772.7
919(29) 0.001189 480.3 834.1
973(30) 0.001111 480.2 906.9
1033(31) 0.001041 480.1 990.2
1200(33) 0.000918 480.0 1082.5
1273(34) 0.000865 479.9 1181.5
1264(34) 0.000865 479.8 1283.5
1419(36) 0.000772 480. 1384.
1468(37) 0.000730 480. 1478.
1562(38) 0.000693 480. 1561.
1562(38) 0.000693 479. 1628.
1641(39) 0.000657 479. 1673.
1650(39) 0.000657 479. 1692.
1662(39) 0.000657 479. 1683.
1569(38) 0.000693 479. 1645.
1538(38) 0.000693 479. 1579.
1469(37) 0.000730 479. 1494.
1337(35) 0.000816 478.7 1392.1
1295(34) 0.000865 478.6 1281.7
1182(33) 0.000918 478.6 1166.1
1077(29) 0.001189 478.5 1057.4
956(28) 0.001276 478.4 954.2
844(26) 0.001479 478.3 864.1
823(26) 0.001479 478.2 786.2
800(25) 0.001600 478.1 720.8
688(23) 0.001890 478.0 667.6
687(23) 0.001890 477.9 625.5
651(23) 0.001890 477.8 593.1
608(22) 0.002066 477.7 568.8
579(22) 0.002066 477.6 551.6
527(21) 0.002268 477.5 539.0
560(21) 0.002268 477.4 530.2
536(21) 0.002268 477.3 524.2
560(21) 0.002268 477.2 521.0
543(21) 0.002268 477.2 518.9
536(21) 0.002268 477.1 517.9
555(21) 0.002268 477.0 517.9
554(21) 0.002268 476.9 519.5
523(20) 0.002500 476.8 522.0
524(21) 0.002268 476.7 524.5
535(21) 0.002268 476.6 527.8
542(21) 0.002268 476.5 531.8
530(21) 0.002268 476.5 536.5
523(20) 0.002500 476.4 541.8
549(21) 0.002268 476.3 547.3
546(21) 0.002268 476.2 552.9
557(21) 0.002268 476.1 558.2
573(21) 0.002268 476.0 562.9
565(21) 0.002268 475.9 566.6
555(21) 0.002268 475.9 569.1
583(22) 0.002066 475.8 570.5
593(22) 0.002066 475.7 569.9
579(22) 0.002066 475.6 569.7
603(22) 0.002066 475.5 568.9
553(21) 0.002268 475.5 568.2
615(22) 0.002066 475.4 569.2
638(23) 0.001890 475.3 571.4
628(22) 0.002066 475.2 575.2
596(22) 0.002066 475.1 578.3
634(23) 0.001890 475.1 584.5
634(23) 0.001890 475.0 590.5
595(22) 0.002066 474.9 598.6
623(22) 0.002066 474.8 606.6
648(23) 0.001890 474.7 613.7
620(22) 0.002066 474.7 619.4
628(22) 0.002066 474.6 623.3
609(23) 0.001890 474.5 625.5
654(24) 0.001736 474.4 626.2
618(23) 0.001890 474.4 626.2
627(23) 0.001890 474.3 626.3
634(23) 0.001890 474.2 627.3
660(24) 0.001736 474.2 630.3
606(23) 0.001890 474.1 635.9
626(23) 0.001890 474.0 645.1
662(24) 0.001736 473.9 658.4
634(23) 0.001890 473.9 676.4
654(24) 0.001736 473.8 699.6
705(25) 0.001600 473.7 728.0
706(25) 0.001600 473.7 761.8
801(26) 0.001479 473.6 800.8
815(26) 0.001479 473.5 844.3
862(27) 0.001372 473.5 891.6
919(28) 0.001276 473.4 941.0
911(28) 0.001276 473.3 990.8
1009(29) 0.001189 473.3 1038.7
1073(30) 0.001111 473.2 1082.2
1086(30) 0.001111 473.1 1118.9
1127(31) 0.001041 473.1 1146.4
1092(31) 0.001041 473.0 1162.6
1103(31) 0.001041 472.9 1165.8
1069(30) 0.001111 472.9 1154.9
1081(30) 0.001111 472.8 1129.9
1063(30) 0.001111 472.8 1092.2
1029(30) 0.001111 472.7 1044.2
975(29) 0.001189 472.6 988.8
992(29) 0.001189 472.6 929.7
947(28) 0.001276 472.5 869.8
859(27) 0.001372 472.5 811.7
769(26) 0.001479 472.4 757.4
769(26) 0.001479 472.4 708.2
693(24) 0.001736 472.3 665.0
678(24) 0.001736 472.2 628.1
651(24) 0.001736 472.2 597.4
605(23) 0.001890 472.1 572.4
594(23) 0.001890 472.1 552.4
588(22) 0.002066 472.0 536.7
578(22) 0.002066 472.0 524.5
535(21) 0.002268 471.9 515.1
538(21) 0.002268 471.9 507.9
543(22) 0.002066 471.8 502.3
459(20) 0.002500 471.8 499.1
507(21) 0.002268 471.7 495.7
521(21) 0.002268 471.7 494.4
510(21) 0.002268 471.6 492.4
504(21) 0.002268 471.6 490.7
490(20) 0.002500 471.5 492.3
501(21) 0.002268 471.5 493.5
482(20) 0.002500 471.4 492.7
521(21) 0.002268 471.4 493.9
475(27) 0.001372 471.3 493.5
501(20) 0.002500 471.3 493.3
480(20) 0.002500 471.3 493.2
496(20) 0.002500 471.2 493.2
506(20) 0.002500 471.2 493.3
505(20) 0.002500 471.1 493.5
511(20) 0.002500 471.1 493.9
481(20) 0.002500 471.1 494.3
475(20) 0.002500 471.0 494.9
468(20) 0.002500 471.0 495.6
500(20) 0.002500 470.9 496.5
530(21) 0.002268 470.9 497.6
495(20) 0.002500 470.9 498.8
486(20) 0.002500 470.8 500.2
498(20) 0.002500 470.8 501.8
515(21) 0.002268 470.8 503.6
497(20) 0.002500 470.7 505.7
516(21) 0.002268 470.7 507.1
511(21) 0.002268 470.7 509.6
505(20) 0.002500 470.6 512.3
520(21) 0.002268 470.6 514.4
519(21) 0.002268 470.6 517.5
497(20) 0.002500 470.5 520.9
510(20) 0.002500 470.5 524.5
522(21) 0.002268 470.5 527.9
519(21) 0.002268 470.5 531.8
515(21) 0.002268 470.4 537.6
512(21) 0.002268 470.4 544.9
518(21) 0.002268 470.4 554.3
517(21) 0.002268 470.4 566.8
544(21) 0.002268 470.3 583.5
547(21) 0.002268 470.3 605.8
578(22) 0.002066 470.3 635.4
611(22) 0.002066 470.3 674.0
653(23) 0.001890 470.2 724.2
732(24) 0.001736 470.2 787.2
833(26) 0.001479 470.2 865.3
978(28) 0.001276 470.2 960.4
1077(30) 0.001111 470.2 1073.6
1238(32) 0.000977 470.1 1205.7
1435(34) 0.000865 470.1 1355.0
1572(36) 0.000772 470. 1520.
1800(38) 0.000693 470. 1698.
1939(39) 0.000657 470. 1883.
2131(41) 0.000595 470. 2069.
2241(42) 0.000567 470. 2248.
2414(44) 0.000517 470. 2412.
2524(45) 0.000494 470. 2551.
2590(47) 0.000453 470. 2658.
2650(48) 0.000434 470. 2726.
2681(48) 0.000434 470. 2750.
2724(48) 0.000434 470. 2730.
2660(48) 0.000434 470. 2667.
2618(47) 0.000453 470. 2565.
2561(47) 0.000453 470. 2432.
2428(46) 0.000473 470. 2275.
2215(44) 0.000517 470. 2103.
2061(42) 0.000567 470. 1925.
1875(40) 0.000625 470. 1748.
1692(38) 0.000693 470. 1577.
1529(36) 0.000772 470. 1419.
1370(34) 0.000865 470.0 1275.3
1180(32) 0.000977 470.0 1148.2
1090(31) 0.001041 470.0 1038.1
983(29) 0.001189 470.0 944.6
884(28) 0.001276 470.0 866.6
837(27) 0.001372 470.0 802.3
762(26) 0.001479 470.0 750.0
744(26) 0.001479 470.0 708.2
696(25) 0.001600 470.0 675.1
675(24) 0.001736 470.0 649.2
673(24) 0.001736 470.0 629.7
627(23) 0.001890 470.0 615.2
604(23) 0.001890 470.0 605.2
611(23) 0.001890 470.0 599.2
626(23) 0.001890 470.0 596.7
622(23) 0.001890 470.0 597.7
665(24) 0.001736 470.1 601.9
635(24) 0.001736 470.1 609.2
623(23) 0.001890 470.1 619.5
632(24) 0.001736 470.1 632.7
669(24) 0.001736 470.1 648.5
698(25) 0.001600 470.1 666.5
699(25) 0.001600 470.1 686.3
743(25) 0.001600 470.2 707.2
770(26) 0.001479 470.2 728.4
734(25) 0.001600 470.2 749.1
752(26) 0.001479 470.2 768.3
787(26) 0.001479 470.2 785.0
747(26) 0.001479 470.3 798.4
772(26) 0.001479 470.3 807.8
753(26) 0.001479 470.3 812.8
773(26) 0.001479 470.3 813.1
782(26) 0.001479 470.4 808.7
794(26) 0.001479 470.4 799.7
794(26) 0.001479 470.4 786.6
764(26) 0.001479 470.5 769.7
721(25) 0.001600 470.5 750.0
721(25) 0.001600 470.5 726.8
698(25) 0.001600 470.5 702.1
648(24) 0.001736 470.6 678.8
648(23) 0.001890 470.6 655.3
624(23) 0.001890 470.6 629.3
595(22) 0.002066 470.7 606.1
569(22) 0.002066 470.7 587.6
539(21) 0.002268 470.8 568.4
584(22) 0.002066 470.8 554.1
579(22) 0.002066 470.8 541.4
536(21) 0.002268 470.9 530.8
534(21) 0.002268 470.9 522.9
523(21) 0.002268 471.0 516.3
530(21) 0.002268 471.0 511.6
517(21) 0.002268 471.0 508.5
509(21) 0.002268 471.1 508.3
508(21) 0.002268 471.1 508.8
549(21) 0.002268 471.2 510.1
542(21) 0.002268 471.2 512.5
542(21) 0.002268 471.3 516.0
537(21) 0.002268 471.3 520.7
536(21) 0.002268 471.4 526.4
529(21) 0.002268 471.4 532.9
573(22) 0.002066 471.5 540.2
558(22) 0.002066 471.5 547.9
572(22) 0.002066 471.6 556.0
608(23) 0.001890 471.6 564.1
599(22) 0.002066 471.7 572.0
594(22) 0.002066 471.7 579.4
622(23) 0.001890 471.8 586.0
610(23) 0.001890 471.9 591.6
609(23) 0.001890 471.9 596.0
617(23) 0.001890 472.0 599.1
609(23) 0.001890 472.0 600.9
570(22) 0.002066 472.1 601.3
581(22) 0.002066 472.2 600.5
616(23) 0.001890 472.2 598.4
615(23) 0.001890 472.3 595.2
613(23) 0.001890 472.4 591.1
607(23) 0.001890 472.4 586.2
591(22) 0.002066 472.5 580.8
590(22) 0.002066 472.6 575.2
614(23) 0.001890 472.6 569.6
610(23) 0.001890 472.7 563.9
572(22) 0.002066 472.8 559.2
565(22) 0.002066 472.9 555.3
584(22) 0.002066 472.9 552.4
592(22) 0.002066 473.0 550.4
596(22) 0.002066 473.1 550.7
583(22) 0.002066 473.2 552.9
576(23) 0.001890 473.2 557.3
559(22) 0.002066 473.3 564.4
562(22) 0.002066 473.4 574.4
602(23) 0.001890 473.5 587.3
666(24) 0.001736 473.6 604.0
672(24) 0.001736 473.6 624.7
692(25) 0.001600 473.7 649.5
709(25) 0.001600 473.8 678.8
727(25) 0.001600 473.9 712.7
786(26) 0.001479 474.0 750.8
826(27) 0.001372 474.1 793.0
870(28) 0.001276 474.2 839.1
901(28) 0.001276 474.3 888.6
951(29) 0.001189 474.3 940.7
1008(30) 0.001111 474.4 994.6
1045(30) 0.001111 474.5 1049.1
1099(31) 0.001041 474.6 1103.1
1194(32) 0.000977 474.7 1155.1
1214(32) 0.000977 474.8 1203.8
1239(33) 0.000918 474.9 1247.7
1291(33) 0.000918 475.0 1285.9
1300(33) 0.000918 475.1 1317.2
1352(34) 0.000865 475.2 1340.9
1356(34) 0.000865 475.3 1356.2
1370(34) 0.000865 475.4 1362.4
1367(34) 0.000865 475.5 1359.2
1317(34) 0.000865 475.6 1346.1
1293(33) 0.000918 475.7 1323.3
1290(33) 0.000918 475.8 1291.2
1256(33) 0.000918 476.0 1250.7
1233(33) 0.000918 476.1 1203.1
1163(32) 0.000977 476.2 1150.2
1066(30) 0.001111 476.3 1093.7
1016(30) 0.001111 476.4 1035.5
965(29) 0.001189 476.5 977.2
899(28) 0.001276 476.6 921.2
865(27) 0.001372 476.7 867.3
832(27) 0.001372 476.9 817.6
793(26) 0.001479 477.0 771.7
735(25) 0.001600 477.1 730.8
708(25) 0.001600 477.2 694.9
702(25) 0.001600 477.3 665.2
657(24) 0.001736 477.5 639.6
619(23) 0.001890 477.6 618.5
614(23) 0.001890 477.7 602.0
587(23) 0.001890 477.8 589.6
592(23) 0.001890 478.0 580.9
598(23) 0.001890 478.1 575.8
607(23) 0.001890 478.2 573.9
601(23) 0.001890 478.4 575.2
569(23) 0.001890 478.5 579.1
583(23) 0.001890 478.6 585.7
582(23) 0.001890 478.8 594.7
635(24) 0.001736 478.9 605.9
608(23) 0.001890 479.0 619.8
609(23) 0.001890 479.2 634.9
652(24) 0.001736 479.3 651.4
693(25) 0.001600 479.4 669.1
678(25) 0.001600 479.6 687.3
703(25) 0.001600 479.7 705.7
752(26) 0.001479 479.9 723.6
726(25) 0.001600 480.0 740.4
737(26) 0.001479 480.2 755.6
726(26) 0.001479 480.3 768.5
743(26) 0.001479 480.4 778.7
777(26) 0.001479 480.6 785.7
767(26) 0.001479 480.7 789.5
800(27) 0.001372 480.9 789.4
770(26) 0.001479 481.1 785.6
753(26) 0.001479 481.2 778.4
724(25) 0.001600 481.4 767.9
704(25) 0.001600 481.5 754.5
753(26) 0.001479 481.7 738.8
718(25) 0.001600 481.8 721.3
678(25) 0.001600 482.0 703.0
693(25) 0.001600 482.2 684.3
689(25) 0.001600 482.3 665.8
658(24) 0.001736 482.5 647.3
646(24) 0.001736 482.6 630.7
610(24) 0.001736 482.8 615.0
561(23) 0.001890 483.0 601.8
600(23) 0.001890 483.1 590.7
607(23) 0.001890 483.3 581.2
562(23) 0.001890 483.5 574.8
553(23) 0.001890 483.7 571.0
577(23) 0.001890 483.8 569.9
579(23) 0.001890 484.0 569.8
584(23) 0.001890 484.2 573.9
572(23) 0.001890 484.3 581.6
621(24) 0.001736 484.5 592.5
614(24) 0.001736 484.7 606.9
628(24) 0.001736 484.9 624.8
632(24) 0.001736 485.1 646.5
683(25) 0.001600 485.2 672.1
686(25) 0.001600 485.4 701.5
744(26) 0.001479 485.6 734.8
814(27) 0.001372 485.8 771.9
814(27) 0.001372 486.0 812.4
882(28) 0.001276 486.2 855.9
924(29) 0.001189 486.4 901.8
937(30) 0.001111 486.6 949.4
1000(31) 0.001041 486.7 997.7
1024(31) 0.001041 486.9 1045.6
1097(32) 0.000977 487.1 1091.9
1119(32) 0.000977 487.3 1135.5
1176(33) 0.000918 487.5 1175.1
1218(34) 0.000865 487.7 1209.7
1247(34) 0.000865 487.9 1238.6
1269(34) 0.000865 488.1 1261.1
1264(34) 0.000865 488.3 1276.9
1330(35) 0.000816 488.5 1285.7
1355(36) 0.000772 489. 1288.
1335(35) 0.000816 488.9 1282.7
1335(35) 0.000816 489.2 1271.5
1284(35) 0.000816 489.4 1254.6
1247(34) 0.000865 489.6 1232.8
1218(34) 0.000865 489.8 1207.1
1177(33) 0.000918 490.0 1178.4
1171(33) 0.000918 490.2 1147.2
1173(33) 0.000918 490.4 1115.0
1106(32) 0.000977 490.6 1082.0
1031(31) 0.001041 490.9 1048.9
992(31) 0.001041 491.1 1016.0
961(30) 0.001111 491.3 983.5
975(30) 0.001111 491.5 952.1
923(30) 0.001111 491.7 922.1
933(30) 0.001111 492.0 893.6
935(30) 0.001111 492.2 867.3
862(29) 0.001189 492.4 843.0
802(28) 0.001276 492.6 821.1
814(28) 0.001276 492.9 801.8
835(28) 0.001276 493.1 785.2
725(26) 0.001479 493.3 770.9
744(27) 0.001372 493.6 758.9
781(27) 0.001372 493.8 748.7
765(27) 0.001372 494.0 740.2
732(27) 0.001372 494.3 733.1
766(27) 0.001372 494.5 727.0
736(27) 0.001372 494.7 721.9
705(26) 0.001479 495.0 717.1
705(26) 0.001479 495.2 712.6
707(26) 0.001479 495.5 708.1
695(26) 0.001479 495.7 703.5
666(25) 0.001600 496.0 698.6
676(26) 0.001479 496.2 693.2
690(26) 0.001479 496.5 687.3
666(25) 0.001600 496.7 680.7
673(26) 0.001479 497.0 673.5
679(26) 0.001479 497.2 665.6
684(26) 0.001479 497.5 657.2
654(25) 0.001600 497.7 648.2
625(25) 0.001600 498.0 639.0
617(20) 0.002500 498.2 629.6
639(25) 0.001600 498.5 620.1
586(24) 0.001736 498.8 610.7
632(25) 0.001600 499.0 601.5
609(24) 0.001736 499.3 592.7
586(24) 0.001736 499.5 585.8
617(24) 0.001736 499.8 577.9
565(24) 0.001736 500.1 570.6
586(24) 0.001736 500.3 563.8
590(24) 0.001736 500.6 557.8
600(24) 0.001736 500.9 552.3
535(23) 0.001890 501.2 547.6
577(24) 0.001736 501.4 543.5
561(23) 0.001890 501.7 540.0
567(24) 0.001736 502.0 539.0
542(23) 0.001890 502.3 536.7
530(23) 0.001890 502.5 535.0
542(23) 0.001890 502.8 533.8
557(23) 0.001890 503.1 538.3
506(22) 0.002066 503.4 538.1
507(22) 0.002066 503.7 537.4
539(23) 0.001890 504.0 537.9
580(24) 0.001736 504.2 538.1
554(23) 0.001890 504.5 539.4
578(24) 0.001736 504.8 540.6
532(23) 0.001890 505.1 541.9
527(23) 0.001890 505.4 542.1
517(23) 0.001890 505.7 543.1
548(23) 0.001890 506.0 544.5
560(23) 0.001890 506.3 545.5
520(23) 0.001890 506.6 546.7
530(23) 0.001890 506.9 547.7
565(23) 0.001890 507.2 548.8
563(23) 0.001890 507.5 549.5
512(22) 0.002066 507.8 549.8
592(24) 0.001736 508.1 550.3
509(22) 0.002066 508.4 550.8
564(23) 0.001890 508.7 551.2
571(24) 0.001736 509.0 551.6
587(24) 0.001736 509.3 551.6
544(23) 0.001890 509.6 552.4
567(24) 0.001736 510.0 553.4
566(24) 0.001736 510.3 554.6
588(24) 0.001736 510.6 556.1
579(24) 0.001736 510.9 558.0
583(24) 0.001736 511.2 560.3
600(24) 0.001736 511.5 563.0
581(24) 0.001736 511.9 566.0
552(24) 0.001736 512.2 569.4
566(24) 0.001736 512.5 573.2
571(24) 0.001736 512.8 577.2
549(24) 0.001736 513.2 581.5
612(25) 0.001600 513.5 586.2
617(25) 0.001600 513.8 591.2
568(24) 0.001736 514.2 596.4
574(24) 0.001736 514.5 601.8
600(25) 0.001600 514.8 607.4
587(25) 0.001600 515.2 613.2
646(26) 0.001479 515.5 619.2
574(24) 0.001736 515.8 625.7
612(25) 0.001600 516.2 633.0
586(25) 0.001600 516.5 640.7
595(25) 0.001600 516.9 650.5
650(26) 0.001479 517.2 660.9
615(25) 0.001600 517.6 673.2
648(26) 0.001479 517.9 688.4
655(26) 0.001479 518.3 705.7
667(26) 0.001479 518.6 726.2
719(27) 0.001372 519.0 750.4
731(27) 0.001372 519.3 778.8
755(28) 0.001276 519.7 812.0
765(28) 0.001276 520.0 850.6
784(28) 0.001276 520.4 894.9
855(29) 0.001189 520.7 945.4
956(31) 0.001041 521.1 1002.5
1036(32) 0.000977 521.5 1066.5
1113(33) 0.000918 521.8 1137.5
1171(34) 0.000865 522.2 1215.5
1277(35) 0.000816 522.5 1300.4
1344(36) 0.000772 523. 1392.
1510(38) 0.000693 523. 1489.
1616(39) 0.000657 524. 1591.
1740(41) 0.000595 524. 1697.
1826(42) 0.000567 524. 1806.
1898(43) 0.000541 525. 1916.
1997(44) 0.000517 525. 2025.
2083(45) 0.000494 526. 2132.
2204(46) 0.000473 526. 2235.
2301(47) 0.000453 526. 2332.
2378(48) 0.000434 527. 2421.
2324(47) 0.000453 527. 2499.
2285(47) 0.000453 527. 2565.
2431(48) 0.000434 528. 2615.
2523(49) 0.000416 528. 2649.
2534(49) 0.000416 529. 2664.
2457(48) 0.000434 529. 2660.
2523(49) 0.000416 529. 2635.
2487(49) 0.000416 530. 2592.
2444(48) 0.000434 530. 2530.
2392(48) 0.000434 531. 2452.
2328(47) 0.000453 531. 2360.
2208(43) 0.000541 531. 2259.
2156(43) 0.000541 532. 2148.
2006(41) 0.000595 532. 2033.
1930(40) 0.000625 533. 1916.
1838(39) 0.000657 533. 1798.
1677(38) 0.000693 533. 1683.
1646(37) 0.000730 534. 1571.
1500(36) 0.000772 534. 1465.
1403(35) 0.000816 534.6 1364.9
1315(34) 0.000865 535.0 1272.6
1221(32) 0.000977 535.4 1188.3
1197(32) 0.000977 535.8 1112.6
1098(31) 0.001041 536.3 1045.3
1057(30) 0.001111 536.7 986.6
954(29) 0.001189 537.1 936.1
929(28) 0.001276 537.5 893.5
866(28) 0.001276 537.9 858.5
900(28) 0.001276 538.4 830.4
834(27) 0.001372 538.8 808.9
838(27) 0.001372 539.2 793.5
843(27) 0.001372 539.6 783.5
786(26) 0.001479 540.1 778.5
816(27) 0.001372 540.5 777.8
760(26) 0.001479 540.9 781.5
857(27) 0.001372 541.4 788.8
860(27) 0.001372 541.8 799.1
877(28) 0.001276 542.2 812.5
877(28) 0.001276 542.7 827.8
864(28) 0.001276 543.1 844.9
885(28) 0.001276 543.6 863.2
843(27) 0.001372 544.0 882.3
922(28) 0.001276 544.5 901.6
921(28) 0.001276 544.9 920.5
896(28) 0.001276 545.3 938.7
917(28) 0.001276 545.8 955.4
955(29) 0.001189 546.2 970.2
945(29) 0.001189 546.7 982.6
964(29) 0.001189 547.1 992.1
1001(29) 0.001189 547.6 998.7
983(29) 0.001189 548.1 1001.7
992(29) 0.001189 548.5 1001.0
971(29) 0.001189 549.0 996.5
998(29) 0.001189 549.4 988.5
935(29) 0.001189 549.9 977.1
943(29) 0.001189 550.4 962.7
932(29) 0.001189 550.8 945.7
909(29) 0.001189 551.3 927.2
916(29) 0.001189 551.8 906.4
945(30) 0.001111 552.2 885.0
892(29) 0.001189 552.7 862.6
845(28) 0.001276 553.2 840.4
843(28) 0.001276 553.6 818.2
869(29) 0.001189 554.1 797.0
815(28) 0.001276 554.6 777.4
751(27) 0.001372 555.1 758.5
775(27) 0.001372 555.6 741.3
723(26) 0.001479 556.0 726.0
697(26) 0.001479 556.5 713.3
693(26) 0.001479 557.0 700.1
668(25) 0.001600 557.5 690.8
684(26) 0.001479 558.0 683.7
761(27) 0.001372 558.5 678.8
672(25) 0.001600 559.0 676.1
616(24) 0.001736 559.4 675.5
696(26) 0.001479 559.9 677.2
681(26) 0.001479 560.4 680.9
681(25) 0.001600 560.9 686.7
715(26) 0.001479 561.4 692.1
724(26) 0.001479 561.9 701.9
711(26) 0.001479 562.4 713.5
719(26) 0.001479 562.9 726.8
737(26) 0.001479 563.4 736.5
789(27) 0.001372 563.9 753.1
781(27) 0.001372 564.4 771.1
812(28) 0.001276 564.9 790.0
802(27) 0.001372 565.5 809.8
872(29) 0.001189 566.0 829.9
866(28) 0.001276 566.5 850.6
890(29) 0.001189 567.0 871.2
887(29) 0.001189 567.5 891.5
977(30) 0.001111 568.0 911.1
946(30) 0.001111 568.5 929.7
953(30) 0.001111 569.1 946.9
970(30) 0.001111 569.6 962.4
961(30) 0.001111 570.1 975.7
984(30) 0.001111 570.6 986.9
968(30) 0.001111 571.2 995.3
974(30) 0.001111 571.7 1001.2
1052(31) 0.001041 572.2 1004.4
1020(31) 0.001041 572.7 1005.1
962(30) 0.001111 573.3 1003.0
985(30) 0.001111 573.8 998.5
1008(31) 0.001041 574.3 991.8
1000(30) 0.001111 574.9 983.3
987(30) 0.001111 575.4 973.3
988(30) 0.001111 575.9 962.2
979(30) 0.001111 576.5 950.4
1030(31) 0.001041 577.0 938.4
1045(31) 0.001041 577.6 926.8
966(41) 0.000595 578. 915.
993(29) 0.001189 578.7 905.7
922(28) 0.001276 579.2 896.7
927(28) 0.001276 579.8 888.8
943(28) 0.001276 580.3 882.6
962(28) 0.001276 580.9 878.1
914(28) 0.001276 581.4 875.5
893(27) 0.001372 582.0 874.8
869(27) 0.001372 582.5 875.8
881(27) 0.001372 583.1 879.0
900(28) 0.001276 583.6 884.0
917(28) 0.001276 584.2 890.9
876(27) 0.001372 584.8 899.6
860(27) 0.001372 585.3 910.1
922(28) 0.001276 585.9 922.0
949(28) 0.001276 586.4 935.8
998(29) 0.001189 587.0 950.5
999(29) 0.001189 587.6 967.7
961(28) 0.001276 588.2 986.7
1065(30) 0.001111 588.7 1006.6
1078(30) 0.001111 589.3 1029.0
1057(30) 0.001111 589.9 1053.4
1105(30) 0.001111 590.5 1079.4
1158(31) 0.001041 591.0 1107.1
1130(31) 0.001041 591.6 1136.3
1147(31) 0.001041 592.2 1166.9
1225(32) 0.000977 592.8 1198.7
1269(32) 0.000977 593.4 1231.3
1241(32) 0.000977 593.9 1264.3
1316(33) 0.000918 594.5 1297.5
1361(33) 0.000918 595.1 1330.4
1389(34) 0.000865 595.7 1362.5
1393(34) 0.000865 596.3 1393.4
1344(33) 0.000918 596.9 1422.3
1439(34) 0.000865 597.5 1449.0
1490(35) 0.000816 598.1 1472.7
1454(35) 0.000816 598.7 1493.1
1434(34) 0.000865 599.3 1509.7
1467(35) 0.000816 599.9 1522.2
1436(34) 0.000865 600.5 1530.1
1471(35) 0.000816 601.1 1533.3
1480(35) 0.000816 601.7 1531.8
1440(34) 0.000865 602.3 1525.4
1486(35) 0.000816 602.9 1514.3
1468(35) 0.000816 603.5 1498.7
1504(35) 0.000816 604.1 1478.8
1477(35) 0.000816 604.7 1454.9
1403(34) 0.000865 605.3 1427.5
1397(35) 0.000816 605.9 1397.0
1377(35) 0.000816 606.5 1363.8
1325(34) 0.000865 607.2 1328.7
1316(34) 0.000865 607.8 1292.0
1236(33) 0.000918 608.4 1254.4
1251(33) 0.000918 609.0 1216.4
1217(33) 0.000918 609.6 1178.9
1191(32) 0.000977 610.3 1141.5
1150(32) 0.000977 610.9 1105.2
1110(31) 0.001041 611.5 1071.1
1060(31) 0.001041 612.1 1037.8
999(30) 0.001111 612.8 1006.4
982(30) 0.001111 613.4 977.0
972(29) 0.001189 614.0 949.9
966(29) 0.001189 614.7 925.2
923(29) 0.001189 615.3 902.9
913(29) 0.001189 615.9 883.1
892(28) 0.001276 616.6 865.7
864(28) 0.001276 617.2 850.7
874(28) 0.001276 617.8 838.1
906(28) 0.001276 618.5 827.8
859(28) 0.001276 619.1 819.3
830(27) 0.001372 619.8 813.3
842(28) 0.001276 620.4 809.3
834(27) 0.001372 621.0 807.1
827(27) 0.001372 621.7 806.0
810(27) 0.001372 622.3 807.1
777(26) 0.001479 623.0 809.5
833(27) 0.001372 623.6 812.9
814(27) 0.001372 624.3 817.8
830(27) 0.001372 625.0 823.3
870(28) 0.001276 625.6 829.9
831(27) 0.001372 626.3 837.3
836(27) 0.001372 626.9 845.2
846(28) 0.001276 627.6 853.5
867(28) 0.001276 628.2 862.2
883(28) 0.001276 628.9 871.0
887(28) 0.001276 629.6 879.8
887(28) 0.001276 630.2 888.4
918(29) 0.001189 630.9 896.9
942(29) 0.001189 631.6 904.8
900(28) 0.001276 632.2 912.2
882(28) 0.001276 632.9 918.8
833(27) 0.001372 633.6 924.6
917(29) 0.001189 634.3 929.4
916(29) 0.001189 634.9 933.3
908(28) 0.001276 635.6 935.7
921(29) 0.001189 636.3 936.8
935(29) 0.001189 637.0 936.3
936(29) 0.001189 637.6 934.6
947(29) 0.001189 638.3 931.6
903(28) 0.001276 639.0 927.6
924(23) 0.001890 639.7 922.1
915(28) 0.001276 640.4 915.5
932(28) 0.001276 641.0 908.0
902(28) 0.001276 641.7 900.3
908(28) 0.001276 642.4 891.4
869(27) 0.001372 643.1 882.1
836(27) 0.001372 643.8 872.5
899(27) 0.001372 644.5 862.8
914(28) 0.001276 645.2 853.1
870(27) 0.001372 645.9 843.6
826(26) 0.001479 646.6 834.5
843(27) 0.001372 647.3 825.7
846(27) 0.001372 648.0 817.0
804(26) 0.001479 648.7 809.4
825(26) 0.001479 649.4 802.5
847(27) 0.001372 650.1 796.3
828(26) 0.001479 650.8 790.9
816(26) 0.001479 651.5 786.3
837(27) 0.001372 652.2 782.5
827(26) 0.001479 652.9 778.8
800(26) 0.001479 653.6 776.8
774(26) 0.001479 654.3 775.1
838(27) 0.001372 655.0 774.7
831(27) 0.001372 655.7 775.0
810(26) 0.001479 656.5 776.4
780(26) 0.001479 657.2 778.4
786(26) 0.001479 657.9 780.7
810(26) 0.001479 658.6 784.8
806(26) 0.001479 659.3 789.6
822(26) 0.001479 660.0 795.1
827(26) 0.001479 660.8 800.8
860(27) 0.001372 661.5 808.2
869(27) 0.001372 662.2 816.4
877(27) 0.001372 662.9 825.4
864(27) 0.001372 663.7 835.0
862(27) 0.001372 664.4 845.2
878(27) 0.001372 665.1 855.9
897(27) 0.001372 665.8 867.0
864(27) 0.001372 666.6 878.4
854(27) 0.001372 667.3 890.1
864(27) 0.001372 668.0 901.8
902(28) 0.001276 668.8 913.4
955(28) 0.001276 669.5 924.8
948(28) 0.001276 670.2 935.8
900(28) 0.001276 671.0 946.3
910(28) 0.001276 671.7 956.0
936(28) 0.001276 672.5 964.7
940(28) 0.001276 673.2 972.3
932(29) 0.001189 673.9 978.7
907(29) 0.001189 674.7 983.8
922(29) 0.001189 675.4 987.5
955(29) 0.001189 676.2 989.5
983(30) 0.001111 676.9 990.0
953(29) 0.001189 677.7 988.9
940(29) 0.001189 678.4 986.3
949(29) 0.001189 679.2 982.2
947(29) 0.001189 679.9 976.9
955(29) 0.001189 680.7 970.3
971(29) 0.001189 681.4 962.7
982(30) 0.001111 682.2 954.3
943(29) 0.001189 682.9 945.2
894(28) 0.001276 683.7 935.6
905(29) 0.001189 684.4 925.8
931(29) 0.001189 685.2 915.8
925(29) 0.001189 686.0 905.8
933(29) 0.001189 686.7 896.1
916(29) 0.001189 687.5 886.7
895(28) 0.001276 688.2 877.7
839(28) 0.001276 689.0 869.4
863(28) 0.001276 689.8 861.8
844(28) 0.001276 690.5 855.0
850(28) 0.001276 691.3 849.1
835(27) 0.001372 692.1 844.2
845(28) 0.001276 692.8 840.3
834(27) 0.001372 693.6 837.4
852(28) 0.001276 694.4 835.7
868(28) 0.001276 695.1 835.2
832(27) 0.001372 695.9 835.8
847(28) 0.001276 696.7 837.7
814(27) 0.001372 697.5 840.7
814(27) 0.001372 698.2 845.0
811(27) 0.001372 699.0 850.3
869(28) 0.001276 699.8 856.9
853(28) 0.001276 700.6 864.4
878(28) 0.001276 701.4 873.1
890(28) 0.001276 702.1 882.7
882(28) 0.001276 702.9 893.1
865(28) 0.001276 703.7 904.5
865(28) 0.001276 704.5 916.5
935(29) 0.001189 705.3 929.2
972(30) 0.001111 706.1 942.2
906(29) 0.001189 706.8 955.7
955(29) 0.001189 707.6 969.0
1007(30) 0.001111 708.4 982.7
1003(30) 0.001111 709.2 996.6
980(30) 0.001111 710.0 1012.6
979(30) 0.001111 710.8 1026.1
1016(30) 0.001111 711.6 1039.1
1047(31) 0.001041 712.4 1051.4
1067(31) 0.001041 713.2 1064.0
1071(31) 0.001041 714.0 1074.6
1026(30) 0.001111 714.8 1084.2
1040(30) 0.001111 715.6 1092.6
1039(30) 0.001111 716.4 1103.4
1063(30) 0.001111 717.2 1109.0
1098(31) 0.001041 718.0 1113.1
1099(31) 0.001041 718.8 1115.6
1096(31) 0.001041 719.6 1116.4
1103(31) 0.001041 720.4 1115.6
1106(31) 0.001041 721.2 1113.2
1096(31) 0.001041 722.0 1109.2
1042(30) 0.001111 722.8 1103.6
1068(30) 0.001111 723.6 1099.4
1074(30) 0.001111 724.4 1091.2
1056(30) 0.001111 725.2 1081.8
1048(30) 0.001111 726.0 1072.6
1036(30) 0.001111 726.8 1061.4
1045(30) 0.001111 727.6 1049.9
1032(30) 0.001111 728.4 1039.1
1027(30) 0.001111 729.2 1028.8
1040(30) 0.001111 730.1 1016.8
1022(30) 0.001111 730.9 1003.9
973(29) 0.001189 731.7 991.0
967(29) 0.001189 732.5 978.4
978(29) 0.001189 733.3 966.1
938(29) 0.001189 734.1 954.2
944(29) 0.001189 734.9 942.9
963(29) 0.001189 735.8 932.1
925(28) 0.001276 736.6 922.0
916(28) 0.001276 737.4 912.7
904(28) 0.001276 738.2 904.0
877(28) 0.001276 739.0 896.2
879(28) 0.001276 739.9 889.2
867(28) 0.001276 740.7 882.9
873(28) 0.001276 741.5 877.4
877(28) 0.001276 742.3 872.6
835(27) 0.001372 743.2 868.6
851(27) 0.001372 744.0 865.2
822(27) 0.001372 744.8 862.5
846(27) 0.001372 745.6 860.3
840(27) 0.001372 746.5 858.8
851(27) 0.001372 747.3 857.6
814(27) 0.001372 748.1 857.0
812(27) 0.001372 748.9 856.7
844(27) 0.001372 749.8 856.7
789(26) 0.001479 750.6 856.7
821(27) 0.001372 751.4 857.2
838(28) 0.001276 752.3 857.8
823(28) 0.001276 753.1 858.6
839(28) 0.001276 753.9 859.4
786(27) 0.001372 754.8 860.2
761(27) 0.001372 755.6 861.0
807(28) 0.001276 756.4 861.8
818(28) 0.001276 757.3 862.5
799(28) 0.001276 758.1 863.1
790(27) 0.001372 758.9 863.7
828(28) 0.001276 759.8 864.1
814(28) 0.001276 760.6 864.5
857(28) 0.001276 761.4 864.8
824(28) 0.001276 762.3 865.0
780(27) 0.001372 763.1 865.2
790(27) 0.001372 764.0 865.4
819(28) 0.001276 764.8 865.6
818(28) 0.001276 765.6 865.8
775(27) 0.001372 766.5 866.1
823(28) 0.001276 767.3 866.4
789(27) 0.001372 768.2 866.2
771(27) 0.001372 769.0 866.8
784(27) 0.001372 769.9 867.6
790(27) 0.001372 770.7 868.6
773(27) 0.001372 771.5 869.8
757(27) 0.001372 772.4 871.3
832(28) 0.001276 773.2 873.1
839(28) 0.001276 774.1 875.2
798(27) 0.001372 774.9 877.7
783(27) . . .
779(27) . . .
766(27) . . .
787(27) . . .
838(28) . . .
805(28) . . .
834(28) . . .
817(28) . . .
806(28) . . .
847(28) . . .
808(28) . . .
836(28) . . .
837(28) . . .
836(28) . . .
856(28) . . .
841(28) . . .
870(29) . . .
925(29) . . .
958(30) . . .
950(30) . . .
1004(31) . . .
1055(31) . . .
1066(31) . . .
1089(32) . . .
1168(33) . . .
1193(33) . . .
1228(33) . . .
1252(34) . . .
1334(35) . . .
1399(35) . . .
1434(36) . . .
1501(36) . . .
1546(37) . . .
1626(38) . . .
1750(39) . . .
1844(40) . . .
1915(41) . . .
2006(42) . . .
2143(43) . . .
2191(43) . . .
2261(44) . . .
2400(45) . . .
2575(47) . . .
2681(48) . . .
2779(48) . . .
2837(49) . . .
2925(50) . . .
3042(51) . . .
3144(51) . . .
3175(52) . . .
3296(52) . . .
3447(54) . . .
3541(54) . . .
3617(55) . . .
3672(55) . . .
3691(55) . . .
3751(56) . . .
3858(57) . . .
3868(57) . . .
3981(57) . . .
4054(58) . . .
4066(58) . . .
3996(58) . . .
4104(58) . . .
4184(59) . . .
4205(59) . . .
4265(59) . . .
4250(59) . . .
4225(59) . . .
4229(59) . . .
4128(58) . . .
4152(59) . . .
4153(59) . . .
4063(60) . . .
4088(60) . . .
4067(60) . . .
3956(59) . . .
3830(58) . . .
3803(58) . . .
3779(58) . . .
3702(57) . . .
3607(57) . . .
3531(56) . . .
3388(55) . . .
3331(55) . . .
3199(53) . . .
3116(53) . . .
2928(51) . . .
2887(51) . . .
2811(50) . . .
2708(49) . . .
2657(49) . . .
2542(48) . . .
2458(47) . . .
2390(47) . . .
2322(46) . . .
2227(45) . . .
2124(44) . . .
2070(44) . . .
2032(43) . . .
1945(42) . . .
1837(41) . . .
1777(41) . . .
1748(40) . . .
1697(40) . . .
1631(39) . . .
1600(39) . . .
1577(39) . . .
1516(38) . . .
1516(38) . . .
1453(37) . . .
1407(37) . . .
1402(37) . . .
1425(37) . . .
1396(37) . . .
1362(36) . . .
1304(35) . . .
1371(36) . . .
1380(36) . . .
1407(37) . . .
1354(36) . . .
1346(36) . . .
1389(36) . . .
1314(36) . . .
1286(35) . . .
1333(30) . . .
1285(36) . . .
1289(36) . . .
1341(36) . . .
1367(37) . . .
1373(37) . . .
1359(36) . . .
1338(36) . . .
1332(36) . . .
1320(36) . . .
1349(36) . . .
1360(36) . . .
1355(36) . . .
1367(37) . . .
1372(37) . . .
1421(37) . . .
1426(37) . . .
1392(37) . . .
1356(36) . . .
1352(36) . . .
1362(36) . . .
1391(37) . . .
1402(37) . . .
1413(37) . . .
1411(37) . . .
1387(37) . . .
1413(37) . . .
1415(37) . . .
1386(37) . . .
1439(37) . . .
1420(37) . . .
1455(37) . . .
1465(38) . . .
1435(37) . . .
1438(37) . . .
1435(37) . . .
1438(37) . . .
1418(37) . . .
1372(37) . . .
1362(36) . . .
1395(37) . . .
1458(38) . . .
1439(37) . . .
1400(37) . . .
1401(37) . . .
1422(37) . . .
1399(37) . . .
1373(38) . . .
1393(38) . . .
1412(38) . . .
1429(38) . . .
1452(39) . . .
1377(38) . . .
1383(38) . . .
1424(38) . . .
1370(38) . . .
1356(38) . . .
1349(38) . . .
1322(37) . . .
1352(38) . . .
1387(38) . . .
1389(38) . . .
1403(38) . . .
1404(38) . . .
1411(38) . . .
1390(38) . . .
1362(38) . . .
1364(38) . . .
1371(38) . . .
1434(39) . . .
1433(39) . . .
1404(38) . . .
1435(39) . . .
1403(38) . . .
1403(38) . . .
1472(39) . . .
1497(39) . . .
1438(39) . . .
1393(38) . . .
1408(38) . . .
1426(38) . . .
1467(39) . . .
1471(39) . . .
1401(38) . . .
1411(38) . . .
1506(39) . . .
1516(39) . . .
1430(38) . . .
1418(38) . . .
1498(39) . . .
1463(39) . . .
1426(38) . . .
1498(39) . . .
1535(40) . . .
1533(40) . . .
1529(40) . . .
1503(39) . . .
1540(40) . . .
1603(40) . . .
1571(40) . . .
1595(41) . . .
1603(41) . . .
1576(41) . . .
1565(41) . . .
1615(41) . . .
1589(41) . . .
1630(41) . . .
1638(41) . . .
1658(42) . . .
1681(42) . . .
1685(42) . . .
1647(42) . . .
1706(42) . . .
1650(42) . . .
1748(42) . . .
1772(43) . . .
1775(43) . . .
1760(43) . . .
1764(43) . . .
1794(43) . . .
1816(43) . . .
1783(43) . . .
1852(43) . . .
1880(44) . . .
1827(43) . . .
1805(43) . . .
1805(43) . . .
1870(44) . . .
1879(44) . . .
1885(44) . . .
1884(44) . . .
1929(44) . . .
1921(44) . . .
1891(44) . . .
1989(45) . . .
1982(45) . . .
1999(45) . . .
1994(45) . . .
1977(45) . . .
2000(45) . . .
2037(45) . . .
2130(46) . . .
2128(46) . . .
2155(46) . . .
2158(46) . . .
2144(46) . . .
2105(46) . . .
2131(48) . . .
2132(48) . . .
2177(48) . . .
2184(48) . . .
2192(48) . . .
2196(48) . . .
2245(49) . . .
2250(49) . . .
2327(49) . . .
2317(49) . . .
2353(49) . . .
2370(50) . . .
2458(50) . . .
2443(50) . . .
2465(50) . . .
2499(51) . . .
2513(51) . . .
2586(52) . . .
2508(51) . . .
2549(51) . . .
2567(51) . . .
2675(52) . . .
2679(52) . . .
2704(52) . . .
2736(53) . . .
2704(52) . . .
2751(53) . . .
2793(53) . . .
2809(53) . . .
2820(53) . . .
2981(55) . . .
2940(54) . . .
3022(55) . . .
2893(54) . . .
2883(54) . . .
3013(55) . . .
3134(56) . . .
3088(56) . . .
3144(56) . . .
3115(56) . . .
3163(56) . . .
3186(56) . . .
3198(56) . . .
3169(56) . . .
3217(56) . . .
3257(57) . . .
3325(57) . . .
3277(57) . . .
3275(57) . . .
3375(58) . . .
3413(58) . . .
3402(58) . . .
3383(58) . . .
3414(81) . . .
3498(82) . . .
3441(81) . . .
3485(81) . . .
3391(81) . . .
3365(80) . . .
3445(81) . . .
3488(81) . . .
3573(82) . . .
3573(82) . . .
3528(82) . . .
3646(83) . . .
3606(83) . . .
3566(82) . . .
3804(85) . . .
3895(85) . . .
3833(85) . . .
3645(83) . . .
3778(84) . . .
3901(85) . . .
3881(85) . . .
3856(85) . . .
3755(84) . . .
3883(85) . . .
3870(85) . . .
3878(85) . . .
3905(85) . . .
4094(87) . . .
3911(86) . . .
3973(86) . . .
3978(86) . . .
4069(87) . . .
3938(86) . . .
3970(86) . . .
3949(86) . . .
4025(87) . . .
3963(86) . . .
4159(88) . . .
4117(87) . . .
4076(87) . . .
4156(88) . . .
4135(88) . . .
4099(87) . . .
4212(88) . . .
4235(88) . . .
4085(87) . . .
4122(87) . . .
4100(93) . . .
_pd_meas_number_of_points        3235
_pd_proc_number_of_points        3235

_reflns_number_total             640
_reflns_limit_h_min              0
_reflns_limit_h_max              15
_reflns_limit_k_min              0
_reflns_limit_k_max              5
_reflns_limit_l_min              -9
_reflns_limit_l_max              7
_reflns_d_resolution_high        1.092
_reflns_d_resolution_low         14.023

#--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--#

